3. TECPR 11/24/2000 8:58 AM Page v
To the past and present staff members, support staff and students in
Textile Studies at Bolton Institute, for their friendship and support over
4. TECPR 11/24/2000 8:58 AM Page xiii
Technical textiles are reported to be the fastest growing sector of the textile industrial sector and account for almost 19% (10 million tonnes) of the total world ﬁbre
consumption for all textile uses, totalling 53 tonnes in 1997. This ﬁgure is likely to
increase to 14 million tonnes by the year 2005. Technical textiles are estimated to
account for well over 40% of the total textile production in many developed countries and, at the year 2000, account for almost 20% of all textile manufacturing in
China (Byrne 1997).
The current volume of the market worldwide for technical textiles is more than
$60 billion. The average annual growth rate of technical textiles worldwide is
expected to be around 3.8% for the period 2000 to 2005.
The uniqueness and challenge of technical textiles lies in the need to understand
and apply the principles of textile science and technology to provide solutions,
in the main to technological problems but also often to engineering problems as
well. With the emphasis on measurable textile performance in a particular ﬁeld of
application, this requires the technologist to have not only an intricate knowledge
of ﬁbres and textile science and technology but also an understanding of the
application and the scientists, technologists and engineers who service it. Thus the
producer of geotextiles requires an intricate knowledge of the world of civil
engineering, and the medical textile producer, the requirements of consultant,
medical practitioner and nurse. This series attempts to provide a bridge between
producer and end-user.
The main principles involved in the selection of raw materials and their conversion into yarns and fabrics followed by dyeing, ﬁnishing and coating of technical
textiles are explored, followed by the raw materials, processing techniques, ﬁnishing, speciﬁcations, properties and special technical and commercial features of a
wide range of speciﬁc areas of application.
Each of the chapters has been specially prepared and edited to cover current
developments as well as future trends in both the principles of manufacture and the
state-of-the-art constructional speciﬁcations, properties, test methods and standards
of the major product areas and applications of technical textiles.
5. TECPR 11/24/2000 8:58 AM Page xiv
A team of internationally famous authors has contributed a great deal of time,
effort and above all special and signiﬁcant expertise and experience to the preparation of this handbook. The editors wish to extend their most sincere thanks to all
the authors for their important contribution, patience and cooperation. This book
once again conﬁrms that enthusiasm and love of the subject are more important
than the ﬁnancial gains.
Special thanks are also given to Patricia Morrison of Woodhead Publishing Ltd,
Cambridge for her consistent interest and effort in keeping this project warm for
so long and her continued faith in the editors.
Professor Richard Horrocks
Professor Subhash Anand
Faculty of Technology
6. TECPR 11/24/2000 8:58 AM Page xv
List of contributors
Professor S C Anand
Faculty of Technology, Bolton Institute, Deane Road, Bolton BL3 5AB, UK
Professor P Bajaj
Department of Textile Technology, Indian Institute of Technology, Hauz Khas,
New Delhi, India
Mr C Byrne
David Rigby Associates, Peter House, St Peter’s Square, Manchester M1 5AQ,
Dr X Chen
Department of Textiles, UMIST, P O Box 88, Sackville Street, Manchester M60
Mr W Fung
Collins and Aikman, P O Box 29, Warley Mills, Walkden, Manchester M28 3WG,
Dr R H Gong
Department of Textiles, UMIST, P O Box 88, Sackville Street, Manchester M60
Dr M Hall
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Mr E Hardman
Madison Filters (formerly Scapa Filtration), Haslingden, Rossendale, Lancashire,
7. TECPR 11/24/2000 8:58 AM Page xvi
List of contributors
Dr I Holme
Department of Textiles, University of Leeds, Leeds LS2 1JT, UK
Dr D Holmes
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Dr M Miraftab
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Dr S Ogin
School of Mechanical and Materials Engineering, University of Surrey, Guildford,
Surrey GU2 7HX, UK
Dr M Pritchard
Department of the Built Environment, Faculty of Technology, Bolton Institute,
Deane Road, Bolton BL3 5AB, UK
Professor P R Rankilor
9 Blairgowrie Drive, West Tytherington, Macclesﬁeld, Cheshire SK10 2UJ, UK
Mr A J Rigby
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Professor S W Sarsby
Department of the Built Environment, Faculty of Technology, Bolton Institute,
Deane Road, Bolton BL3 5AB, UK
Dr R A Scott
MOD, Defence Clothing and Textiles Agency Science and Technology Division,
Flagstaff Road, Colchester, Essex CO2 7SS, UK
Professor K Slater
Department of Textiles, University of Guelph, Guelph, Ontario N1G 2W1, Canada
Dr P Smith
26 Newhall Park, Otley, Leeds LS21 2RD, UK
Mr W Sondhelm
10 Bowlacre Road, Hyde, Cheshire SK14 5ES, UK
Technical textiles market – an overview
Chris Byrne, Principal Consultant
David Rigby Associates, Peter House, St Peter’s Square, Manchester M1 5AQ, UK
Although ‘technical’ textiles have attracted considerable attention, the use of ﬁbres,
yarns and fabrics for applications other than clothing and furnishing is not a new
phenomenon. Nor is it exclusively linked to the emergence of modern artiﬁcial ﬁbres
and textiles. Natural ﬁbres such as cotton, ﬂax, jute and sisal have been used for
centuries (and still are used) in applications ranging from tents and tarpaulins to
ropes, sailcloth and sacking. There is evidence of woven fabrics and meshes being
used in Roman times and before to stabilise marshy ground for road building – early
examples of what would now be termed geotextiles and geogrids.
What is relatively new is a growing recognition of the economic and strategic
potential of such textiles to the ﬁbre and fabric manufacturing and processing industries of industrial and industrialising countries alike. In some of the most developed
markets, technical products (broadly deﬁned) already account for as much as 50%
of all textile manufacturing activity and output. The technical textiles supply chain
is a long and complex one, stretching from the manufacturers of polymers for technical ﬁbres, coating and speciality membranes through to the converters and fabricators who incorporate technical textiles into ﬁnished products or use them as an
essential part of their industrial operations. The economic scope and importance of
technical textiles extends far beyond the textile industry itself and has an impact
upon just about every sphere of human economic and social activity.
And yet this dynamic sector of the textile industry has not proved entirely
immune to the effects of economic recession, of product and market maturity, and
of growing global competition which are all too well known in the more traditional
sectors of clothing and furnishings. There are no easy paths to success and manufacturers and converters still face the challenge of making economic returns commensurate with the risks involved in operating in new and complex markets. If
anything, the constant need to develop fresh products and applications, invest in
new processes and equipment, and market to an increasingly diverse range of
customers, is more demanding and costly than ever.
Handbook of technical textiles
Technical textiles has never been a single coherent industry sector and market
segment. It is developing in many different directions with varying speeds and levels
of success. There is continual erosion of the barriers between traditional deﬁnitions
of textiles and other ‘ﬂexible engineering’ materials such as paper and plastics, ﬁlms
and membranes, metals, glass and ceramics. What most participants have in common
are many of the basic textile skills of manipulating ﬁbres, fabrics and ﬁnishing
techniques as well as an understanding of how all these interact and perform in
different combinations and environments. Beyond that, much of the technology and
expertise associated with the industry resides in an understanding of the needs and
dynamics of many very different end-use and market sectors. It is here that the new
dividing lines within the industry are emerging.
An appreciation of the development and potential of technical textile markets
therefore starts with some clariﬁcation of the evolving terminology and deﬁnitions
of scope of the industry and its markets. This chapter goes on to consider some of
the factors – technical, commercial and global – which are driving the industry
It also considers how the emergence of new geographical markets in China and
other rapidly industrialising regions of the world looks set to be one of the major
inﬂuences on the growth and location of technical textiles manufacturing in the ﬁrst
10 years of the 21st century.
Deﬁnition and scope of technical textiles
The deﬁnition of technical textiles adopted by the authoritative Textile Terms and
Deﬁnitions, published by the Textile Institute1, is ‘textile materials and products
manufactured primarily for their technical and performance properties rather than
their aesthetic or decorative characteristics’.
Such a brief description clearly leaves considerable scope for interpretation,
especially when an increasing number of textile products are combining both performance and decorative properties and functions in equal measure. Examples are
ﬂame retardant furnishings and ‘breathable’ leisurewear. Indeed, no two published
sources, industry bodies or statistical organisations ever seem to adopt precisely the
same approach when it comes to describing and categorising speciﬁc products and
applications as technical textiles.
It is perhaps not surprising that any attempt to deﬁne too closely and too rigidly
the scope and content of technical textiles and their markets is doomed to failure.
In what is one of the most dynamic and broad ranging areas of modern textiles,
materials, processes, products and applications are all changing too rapidly to deﬁne
and document. There are even important linguistic and cultural perceptions of what
constitutes a technical textile from geographical region to region in what is now a
global industry and marketplace.
1.2.1 Technical or industrial textiles: what’s in a name?
For many years, the term ‘industrial textiles’ was widely used to encompass all textile
products other than those intended for apparel, household and furnishing end-uses.
It is a description still more widely favoured in the USA than in Europe and
elsewhere (see, for example, the Wellington Sears Handbook of Industrial Textiles).2
16. Technical textiles market – an overview
This usage has seemed increasingly inappropriate in the face of developing applications of textiles for medical, hygiene, sporting, transportation, construction, agricultural and many other clearly non-industrial purposes. Industrial textiles are now
more often viewed as a subgroup of a wider category of technical textiles, referring
speciﬁcally to those textile products used in the course of manufacturing operations
(such as ﬁlters, machine clothing, conveyor belts, abrasive substrates etc.) or which
are incorporated into other industrial products (such as electrical components and
cables, ﬂexible seals and diaphragms, or acoustic and thermal insulation for domestic and industrial appliances).
If this revised deﬁnition of industrial textiles is still far from satisfactory, then the
problems of ﬁnding a coherent and universally acceptable description and classiﬁcation of the scope of technical textiles are even greater. Several schemes have been
proposed. For example, the leading international trade exhibition for technical
textiles, Techtextil (organised biennially since the late 1980s by Messe Frankfurt
in Germany and also in Osaka, Japan), deﬁnes 12 main application areas (of which
textiles for industrial applications represent only one group):
agrotech: agriculture, aquaculture, horticulture and forestry
buildtech: building and construction
clothtech: technical components of footwear and clothing
geotech: geotextiles and civil engineering
hometech: technical components of furniture, household textiles and
indutech: ﬁltration, conveying, cleaning and other industrial uses
medtech: hygiene and medical
mobiltech: automobiles, shipping, railways and aerospace
oekotech: environmental protection
protech: personal and property protection
sporttech: sport and leisure.
The search for an all embracing term to describe these textiles is not conﬁned to
the words ‘technical’ and ‘industrial’. Terms such as performance textiles, functional
textiles, engineered textiles and high-tech textiles are also all used in various
contexts, sometimes with a relatively speciﬁc meaning (performance textiles are
frequently used to describe the fabrics used in activity clothing), but more often
with little or no precise signiﬁcance.
1.2.2 Operating at the boundaries of textiles
If the adjective ‘technical’ is difﬁcult to deﬁne with any precision, then so too is the
scope of the term textiles. Figure 1.1 summarises the principal materials, processes
and products which are commonly regarded as falling within the scope of technical
However, there remain many grey areas. For example, the manufacture and processing of metallic wires into products such as cables, woven or knitted screens and
meshes, and reinforcing carcasses for tyres are not generally regarded as lying within
the scope of the textile industry. This is despite the fact that many of the techniques
employed and the ﬁnal products obtained are closely related to conventional textile
Handbook of technical textiles
PES, PA, PAN, PP etc
jute, sisal etc
Silk (ﬁl.) silk (staple)
Regenerated Fibres ᭣
PRODUCTS Rope, Cord
Technical textile materials, processes and products. PES = polyester, PA = polyamide,
PAN = polyacrylonitrile.
Within the composites industry, woven, knitted, braided, nonwoven and wound
yarn reinforcements made from glass, carbon ﬁbre and organic polymer materials
such as aramids are all now widely accepted as being technical textile products. On
the other hand, more loosely structured reinforcing materials such as chopped
strand mat, milled glass and pulped organic ﬁbres are often excluded.
The nonwovens industry has developed from several different technology
directions, including paper manufacturing. The current deﬁnition of a nonwoven
promulgated, for example, under the International Standards Organization standard
ISO 90923 acknowledges a number of borderline areas, including wet-laid products
and extruded meshes and nets. Likewise, distinctions between textile ﬁbres and ﬁlaments, slit or ﬁbrillated ﬁlms, monoﬁlaments and extruded plastics inevitably boil
down to some fairly arbitrary and artiﬁcial criteria. Diameter or width is often used
as the deﬁning characteristic, irrespective of the technologies used or the end-uses
served. Many of the deﬁnitions and categories embodied within existing industry
statistics reﬂect historical divisions of the main manufacturing sectors rather than a
functional or market-based view of the products involved.
Polymer membranes, composite materials and extruded grids and nets are other
products which challenge traditional notions of the scope of technical textile materials, processes and products. Increasingly, technical textiles are likely to ﬁnd their
place within a broader industry and market for ‘ﬂexible engineering materials’
(Fig. 1.2). A number of companies and groups have already adopted this outlook
and operate across the boundaries of traditional industry sectors, focusing a range
18. Technical textiles market – an overview
Scope of ﬂexible engineering materials.
of materials, process technologies and product capabilities upon speciﬁc functions
and markets such as ﬁltration and health care.
1.2.3 Inconsistent statistical reporting
To add to this complexity, different geographical regions and countries tend to
adopt rather different viewpoints and deﬁnitions with regard to all of the above. A
widely quoted misconception that technical textiles in Japan account for over 40%
of all textile output or nearly twice the level in Western Europe can largely be put
down to the different statistical bases employed. In Europe, the most authoritative
source of ﬁbre consumption (and therefore textile output) data is CIRFS (Comité
International de la Rayonne et des Fibres Synthétiques), the European artiﬁcial
ﬁbre producers association. However, CIRFS’ reported statistics (at least until
recently) have speciﬁcally excluded tape and ﬁlm yarns (a signiﬁcant proportion
of all polyoleﬁn textiles), coarser monoﬁlaments and all glass products (as well
as natural ﬁbres such as jute, ﬂax, sisal, etc.). The merger of CIRFS and EATP, the
European Polyoleﬁn Textiles Association, should go some way towards resolving
The Japanese ‘Chemical’ Fibres Manufacturers Association, JCFA, at the other
extreme, includes all these products, including natural ﬁbres, within its deﬁnition of
technical/industrial textiles while the Fiber Statistics Bureau in the USA includes
polyoleﬁn tape and monoﬁlament yarns but excludes glass. Table 1.1 attempts to
restate the relative usage of the main technical ﬁbres and yarns on a more consistent basis.
In this new light, Japan still retains a leading position worldwide in terms of
the proportion of its total textile manufacturing output devoted to technical
textiles. However, this is largely a reﬂection of the importance of its automotive
manufacturing industry (a key user of technical textiles) combined with the relatively smaller size of its apparel and furnishing textile sectors (especially ﬂoor
coverings). The USA apparently accounts for the lowest proportion of technical
Handbook of technical textiles
Comparative levels of technical ﬁbre mill consumption, 1995
% Total ﬁbre consumption + kg per capita
Textile ﬁbres only
Textile ﬁbre, PP tape and
Textile ﬁbre, PP tape,
monoﬁlaments and glass
Source: CIRFS, Fiber Organon, JCFA and David Rigby Associates estimates.
PP = polypropylene.
textile output of the three major industrial regions but still produces and consumes
the largest quantity per capita, especially when all glass textile and technical ﬁbre
uses are included.
Milestones in the development of technical textiles
Although the development of technical and industrial applications for textiles can
be traced back many years, a number of more recent milestones have marked the
emergence of technical textiles as we know them today. Very largely, these have
centred upon new materials, new processes and new applications.
1.3.1 Developments in ﬁbre materials – natural ﬁbres
Until early in the 20th century, the major ﬁbres available for technical and industrial use were cotton and various coarser vegetable ﬁbres such as ﬂax, jute and sisal.
They were typically used to manufacture heavy canvas-type products, ropes and
twines, and were characterised by relatively heavy weight, limited resistance to
water and microbial/fungal attack as well as poor ﬂame retardancy.
Some of the present day regional patterns of technical textiles manufacturing
were established even then, for example Dundee, on the east coast of Scotland
and located at the centre (then) of an important ﬂax growing area as well as being
a whaling port. Following the discovery that whale oil could be used to lubricate
the spinning of the relatively coarse jute ﬁbres then becoming available from the
Indian subcontinent, jute fabrics were widely used for sacking, furniture and carpet
manufacturing, rooﬁng felts, linoleum ﬂooring, twine and a host of other applications.
Although its jute industry was to decline dramatically from a peak at around 1900
owing to competition from other materials as well as from cheaper imports, Dundee
and the surrounding industry subsequently become a nucleus for development of
the UK polypropylene industry in the 1960s. The then newly available polymer
proved not only to be an ideal technical substitute for the natural product but was
also much more consistent in terms of its supply and price.
Traditional end-uses for sisal were similarly rapidly substituted throughout the
established rope, twine and net making centres of Europe and America.
20. Technical textiles market – an overview
Wool proved far less versatile and economic for most industrial applications
although it is still valued for its insulating and ﬂame retardency properties and ﬁnds
use in several high temperature and protective clothing applications. Silk is an
even more exotic ﬁbre, rarely used in technical applications other than for highly
specialised uses such as surgical suture thread. However, the traces of the early
silk industry are still to be seen in the present day location of centres for technical
ﬁlament weaving such as the Lyons area of France. The traditional silk industry
has also contributed to the development of technical textiles in Asia, especially in
1.3.2 Viscose rayon
The ﬁrst commercially available synthetic ﬁbre, viscose rayon, was developed
around 1910 and by the 1920s had made its mark as reinforcement material for tyres
and, subsequently, other mechanical rubber goods such as drive belts, conveyors and
hoses. Its relatively high uniformity, tenacity and modulus (at least when kept dry
within a rubber casing), combined with good temperature resistance, proved ideal
for the fast emerging automotive and industrial equipment markets.
At a much later stage of its lifecycle, other properties of viscose such as its
good absorbency and suitability for processing by paper industry-type wet laying techniques contributed to its role as one of the earliest and most successful
ﬁbres used for nonwoven processing, especially in disposable cleaning and hygiene
1.3.3 Polyamide and polyester
Polyamide (nylon) ﬁbre, ﬁrst introduced in 1939, provided high strength and abrasion resistance, good elasticity and uniformity as well as resistance to moisture. Its
excellent energy absorbing properties proved invaluable in a range of end-uses from
climbing ropes to parachute fabrics and spinnaker sails. Polyamide-reinforced tyres
are still used much more extensively in developing countries where the quality of
road surfaces has traditionally been poor as well as in the emerging market for offroad vehicles worldwide. This contrasts to Western Europe where average road
speeds are much greater and the heat-resistant properties of viscose are still valued.
From the 1950s onwards, the huge growth in world production of polyester,
initially for apparel and household textile applications, provided the incentive
and economies of scale needed to develop and engineer this ﬁbre as a lower cost
alternative to both viscose and polyamide in an increasing range of technical
Nowhere is this more true than Japan and the developing industrial economies
of Asia, including China, where production capacities for both polyester staple and
ﬁlament yarn are extremely high and there is an urgent search for new applications.
Some high volume applications for technical textiles which would typically use polyoleﬁns in western Europe and North America such as geotextiles, carpet backing
and coverstock are more likely to use polyester in Asia largely because of the
greater availability and better economics of ﬁbre supplies in those regions.
At a slightly less obvious level, differences in the polyamide supply situation –
Western Europe and North America are more strongly oriented towards nylon 66
while Asia and Eastern Europe produce predominantly nylon 6 – are reﬂected in
Handbook of technical textiles
different manufacturing practices, product types and technical applications for this
Yet another example is the production and use of Vinylon (PVA, polyvinyl
alcohol) ﬁbres in Japan, where they were developed for a variety of industrial and
technical applications at a time when that country lacked other raw materials and
ﬁbre production capabilities. Use of this ﬁbre for technical textiles is almost nonexistent in the West.
The development of polyoleﬁn (mostly polypropylene but also some polyethylene)
ﬁbres as well as tape and ﬁlm yarns in the 1960s was another milestone in the
development of technical textiles. The low cost and easy processability of this ﬁbre,
combined with its low density and good abrasion and moisture-resistant properties,
have allowed its rapid introduction into a range of applications such as sacks, bags
and packaging, carpet backings and furniture linings as well as ropes and netting.
Many of these markets were directly taken over from jute and similar ﬁbres but
newer end-uses have also been developed, including artiﬁcial sports surfaces.
Properties of the polyoleﬁns such as their poor temperature resistance and complete hydrophobicity have been turned to advantage in nonwovens. Initially used in
conjunction with viscose to permit thermal bonding, polypropylene has now beneﬁted from a growing appreciation of the important role that moisture wicking
(as opposed to absorption) can play in hygiene applications such as coverstock
for diapers (nappies). Finally, the relatively low extrusion temperatures of the polyoleﬁns have proved ideally suited to the fast developing technologies of spin laying
(spun bonding and melt blowing).
As noted above, the development of the polypropylene industry was initially
focused on European and North American markets. However, it is undergoing a
major expansion worldwide as new investment in polymer capacity offers more
favourable economics to new geographical markets.
1.3.5 High performance ﬁbres
The above ‘conventional’ ﬁbre types, both chemical and natural, still account for
over 95% of all organic ﬁbre technical textiles in use (i.e. excluding glass, mineral
and metal ﬁbres). Many of them have been modiﬁed and tailored to highly speciﬁc
end-uses by adjustment of their tenacity, length, decitex, surface proﬁle, ﬁnish and
even by their combination into hybrid and bicomponent products. However, it is the
emergence of the so-called high performance ﬁbres since the early 1980s that has
provided some of the most signiﬁcant and dramatic impulses to the evolution of
First and foremost of these are the aramids, both the highly temperatureresistant meta-aramids (widely used in protective clothing and similar applications)
and the high strength and modulus para-aramids (used in a host of applications
ranging from bulletproof vests to reinforcement of tyres, hoses, friction materials,
ropes and advanced composites). From their commercial introduction in the 1970s,
world demand for p-aramids is expected to reach almost 40 000 tonnes per annum
by 2000 while for m-aramids, consumption will be around 17–18 000 tonnes.
While not huge in overall terms (representing less than 0.5% of total world tech-
22. Technical textiles market – an overview
nical ﬁbre and yarn usage in volume terms but closer to 3–4% in value), the aramids
represent a particularly important milestone in the development of the technical
textiles industry. Partly practical and partly symbolic, the introduction of the aramids
not only led to the injection of large amounts of technical and market support into
the industry and for users by leading ﬁbre manufacturers such as DuPont and Akzo,
but also concentrated the minds of many developers of new products upon the
possibilities (and practicalities) of using similar new generation materials.
The early success of the aramids was a welcome contrast to the development of
carbon ﬁbres, which have been commercially available since the 1960s but largely
constrained by their high material and processing costs to selected high value
markets, particularly aerospace applications. Total world demand for carbon ﬁbres
was still only some 8–9000 tonnes per annum as recently as 1995. In fact, their
market actually shrank in the early 1990s owing to cutbacks in military spending.
At long last, carbon ﬁbres appear to be emerging from the doldrums, with the
appearance not only of important new civil aerospace markets but also of high
technology sporting goods and industrial applications such as wind generator turbine
blades and reinforced fuel tanks. As new manufacturing methods and greater
economies of scale start to bring prices down, the feasibility of even larger scale
applications such as the reinforcement of buildings and structures in earthquake
zones becomes more attractive. Currently, (2000), consumption is considered to be
over 13 000 tonnes per annum, rising to almost 19 000 tonnes by the year 2005.
The introduction of other high performance ﬁbres proliferated, particularly
during the late 1980s, and in the wake of the aramids. These included a range of heat
and ﬂameproof materials suitable for protective clothing and similar applications
(such as phenolic ﬁbres and PBI, polybenzimidazole), ultra-strong high modulus
polyethylene (HMPE) for ballistic protection and rope manufacture, and chemically
stable polymers such as polytetraﬂuoroethylene (PTFE), polyphenylene sulphide
(PPS) and polyethyletherketone (PEEK) for use in ﬁltration and other chemically
Individually, none of these other ﬁbres has yet achieved volume sales anywhere
near those of the aramids (or even carbon ﬁbres). Indeed, the output of some speciality ﬁbres can still be measured in tens of tonnes per year rather than hundreds
or thousands. The widespread industrial recession of the early 1990s caused many
ﬁbre manufacturers to review their development strategies and to focus upon
narrower ranges of products and markets.
1.3.6 Glass and ceramics
Glass has, for many years, been one of the most underrated technical ﬁbres. Used
for many years as a cheap insulating material as well as a reinforcement for relatively low performance plastics (ﬁbre glass) and (especially in the USA) rooﬁng
materials, glass is increasingly being recognised as a sophisticated engineering material with excellent ﬁre and heat-resistant properties. It is now widely used in a
variety of higher performance composite applications, including sealing materials
and rubber reinforcement, as well as ﬁltration, protective clothing and packaging.
The potential adoption of high volume glass-reinforced composite manufacturing techniques by the automotive industry as a replacement for metal body parts
and components, as well as by manufacturing industry in general for all sorts of
industrial and domestic equipment, promises major new markets. Total world con-
Handbook of technical textiles
sumption of ‘textile’ glass in technical applications was some 2.3 million tonnes
per annum in 1995 and is considered likely to be over 2.9 million tonnes at 2000,
representing over 20% of all technical ﬁbre consumption.
Various higher performance ceramic ﬁbres have been developed but are
restricted to relatively specialised applications by their high cost and limited
Figure 1.1 summarises the wide range of processes employed in the manufacture of
technical textiles. Apart from the use of plaiting and knotting for the manufacture
of ropes and nets, weaving was, for many years, the pre-eminent technology employed in the manufacture of ‘industrial’ textiles. In terms of the total weight of
textiles produced, weaving still plays a leading role and developments such as threedimensional and crimpless weaving have opened up many new product and enduse possibilities.
However, the historical progress of technical textiles has seen the advance of
alternative textile forming technologies, most prominently the broad family of nonwoven techniques but also warp and weft knitting, stitchbonding and modern braiding methods. The use of loose ﬁbres with sophisticated cross-sectional proﬁles for
insulation, protection and ﬁbreﬁll applications is another important growth area.
Fibres, yarns and textiles of all types also provide the starting point for a diverse
and fast expanding range of composite reinforcement and forming technologies.
According to a major study of the world technical textiles industry and its
markets projected to 2005 (see Table 1.2), nonwovens are set to overtake weaving
(in terms of the total weight of textiles produced) by around 2002/2003. In area
terms, nonwovens already far exceed woven and other fabric forming methods
because of their lower average weight per unit area. On the other hand, woven and
other yarn-based fabrics will remain in the lead in value terms, at least for the foreseeable future.
There is, therefore, something for every section of the textile industry in the
future of technical textiles. Most product areas will see more rapid growth in value
Worldwide consumption of technical textiles by product type, 2000–2005
All textile products
Source: David Rigby Associates/Techtextil.
Includes ropes, twines, thread, ﬁbreﬁll etc.
24. Technical textiles market – an overview
Worldwide consumption of technical textiles by application, 2000–2005
Transport textiles (auto, train,
Industrial products and
Medical and hygiene textiles
Home textiles, domestic
Clothing components (thread,
Agriculture, horticulture and
Construction – building and
Packaging and containment
Sport and leisure (excluding
Geotextiles, civil engineering
Protective and safety clothing
Ecological protection textilesa
Source: David Rigby Associates/Techtextil.
Already counted in several categories above.
than in volume as technical textiles become increasingly sophisticated and employ
more specialised and higher value raw materials. On the other hand, the total value
of yarns and ﬁbres and of all technical textile products will grow slightly less fast
than their volume because of a changing mix of materials and technologies, especially reﬂecting the growth of nonwovens.
The same study identiﬁed size and growth trends in each major application area for
technical textiles, as deﬁned by the organisers of Techtextil.The results are presented
in Table 1.3.
Ecological textiles were identiﬁed as a separate and potentially important growth
segment but are not consolidated in the total consumption ﬁgure because they have
already been counted under headings such as industrial textiles (ﬁltration media,
oil spill protection and absorption) and geotextiles (geomembrane liners for toxic
waste pits, erosion protection textiles, etc.).
Some selected examples of these broad trends which illustrate key aspects of the
development and use of technical textiles are discussed in further detail below.
Handbook of technical textiles
1.5.1 Transport textiles
Transport applications (cars, lorries, buses, trains, ships and aerospace) represent the
largest single end-use area for technical textiles, accounting for some 20% of the
total. Products range from carpeting and seating (regarded as technical rather than
furnishing textiles because of the very stringent performance characteristics which
they must fulﬁl), through tyre, belt and hose reinforcement, safety belts and air
bags, to composite reinforcements for automotive bodies, civil and military aircraft
bodies, wings and engine components, and many other uses.
The fact that volume and value growth rates in these applications appear to be
amongst the lowest of any application area needs to be interpreted with caution.
The automotive industry (which accounts for a high proportion of all transport
textiles) is certainly one of the most mature in market terms. Growth rates in new
end-uses such as air bags and composite materials will continue to outstrip the
above averages by a considerable margin for many years to come. However, total
technical textile usage is, in many ways, a victim of its own success. Increasing
sophistication in the speciﬁcations and uses of textile materials has led to the
adoption of lighter, stronger, more precisely engineered yarns, woven and knitted
fabrics and nonwovens in place of established materials. The decreasing weight per
tyre of textile reinforcing cord in modern radial constructions is one example of
this. Interior textiles in cars are also making use of lighter weight and lower cost
Modern textiles also last longer. Hoses and belts which used to use substantial
quantities of textile reinforcements are now capable of lasting the lifetime of a vehicle, removing much of the large and continuing ‘after-market’ for textile products.
The automotive industry has led the world in the introduction of tightly organised supply chain structures and textiles are no exception. Technical textile producers have had to learn the language and practice of precision engineering, just-in-time
supply relationships and total quality management. The ideas and systems developed to serve the automotive industry have gradually ﬁltered through to other
markets and have had a profound effect in many different areas. Meanwhile, the
major automotive companies have become increasingly global players in a highly
competitive market and have demanded of their suppliers that they follow suit. The
supply of textiles to this market is already dominated by a relatively few large companies in each product area. Worldwide manufacturing capabilities and strategic
relationships are essential to survival and many smaller players without these
resources have already exited from the market. Recessionary cycles in automotive
markets as well as in military and civil aerospace applications have dealt some
severe blows and only those companies with the long term commitment and
strength to survive are likely to beneﬁt from the better times that the market also
1.5.2 Industrial products and components
Set to rival transport textiles for ﬁrst place by the year 2005 or shortly thereafter
(in volume terms, although not yet in value) is the diverse ﬁeld of ‘industrial’ textiles. As now more precisely deﬁned, this includes textiles used directly in industrial
processes or incorporated into industrial products such as ﬁlters, conveyor belts and
abrasive belts, as well as reinforcements for printed circuit boards, seals and gaskets,
and other industrial equipment.
26. Technical textiles market – an overview
Use of nonwovens already considerably outweighs that of woven and other
fabric types here; consumption in 2000 is estimated at 700 000 tonnes and a little
over 400 000 tonnes, respectively. However, both are surpassed by the use of
technical ﬁbres and textiles for composite reinforcement, over 740 000 tonnes in
Growth rates are generally well above average in most areas. Because of the universal nature of many industrial requirements, some large companies have emerged
with worldwide manufacturing and distribution to dominate markets for industrial
textile products. They include companies such as Scapa (UK) and Albany (US),
leaders in papermaking felts and related product areas, Milliken (USA) in textiles
for rubber reinforcement and other industrial applications and BWF (Germany) in
1.5.3 Medical and hygiene textiles
The fact that medical and hygiene textiles are expected to show below average
growth in volume but above average growth in value reﬂects the contrasting
prospects of at least two main areas of the market.
The largest use of textiles is for hygiene applications such as wipes, babies’
diapers (nappies) and adult sanitary and incontinence products. With the possible
exception of the last of these, all are relatively mature markets whose volume
growth has peaked. Manufacturers and converters now seek to develop them
further by adding value to increasingly sophisticated products. Nonwovens dominate these applications which account for over 23% of all nonwoven use, the largest
proportion of any of the 12 major markets for technical textiles.
Concern has been expressed at the growth of disposable products and the burden
which they place upon landﬁll and other waste disposal methods. Attempts have
been made to develop and introduce more efﬁcient biodegradable ﬁbres for such
end-uses but costs remain high. Meanwhile, the fastest areas of growth are in developing and newly industrialised markets where product penetration is still relatively
low; Asia is a particular target for many of the big name brand manufacturers who
operate in this area.
The other side of the medical and hygiene market is a rather smaller but higher
value market for medical and surgical products such as operating gowns and drapes,
sterilisation packs, dressings, sutures and orthopaedic pads. At the highest value end
of this segment are relatively tiny volumes of extremely sophisticated textiles for
uses such as artiﬁcial ligaments, veins and arteries, skin replacement, hollow ﬁbres
for dialysis machines and so on. Growth prospects in these areas are potentially
considerable although the proving and widespread introduction of new life-critical
products takes time.
1.5.4 Home textiles
By far the largest area of use for other textiles as deﬁned above, that is other than
fabrics, nonwovens and composite reinforcements, over 35% of the total weight
of ﬁbres and textiles in that category, lies in the ﬁeld of household textiles and
furnishing and especially in the use of loose ﬁbres in wadding and ﬁbreﬁll applications. Hollow ﬁbres with excellent insulating properties are widely used in bedding
and sleeping bags. Other types of ﬁbre are increasingly being used to replace foams
Handbook of technical textiles
in furniture because of concern over the ﬁre and health hazards posed by such
Woven fabrics are still used to a signiﬁcant extent as carpet and furniture backings and in some smaller, more specialised areas such as curtain header tapes.
However, nonwovens such as spunbondeds have made signiﬁcant inroads into these
larger markets while various drylaid and hydroentangled products are now widely
used in household cleaning applications in place of traditional mops and dusters.
1.5.5 Clothing components
This category includes ﬁbres, yarns and textiles used as technical components in the
manufacture of clothing such as sewing threads, interlinings, waddings and insulation; it does not include the main outer and lining fabrics of garments, nor does it
cover protective clothing which is discussed later.
Although the world’s consumption of clothing and therefore of these types of
technical textile continues to increase steadily, the major problem faced by established manufacturers is the relocation of garment manufacturing to lower cost
countries and therefore the need to develop extended supply lines and marketing
channels to these areas, usually in the face of growing local competition.
As for home textile applications, this is a major market for ﬁbreﬁll products. Some
of the latest and most sophisticated developments have seen the incorporation of
temperature phase change materials into such insulation products to provide an
additional degree of control and resistance to sudden extremes of temperature, be
they hot or cold.
1.5.6 Agriculture, horticulture and ﬁshing
Textiles have always been used extensively in the course of food production, most
notably by the ﬁshing industry in the form of nets, ropes and lines but also by agriculture and horticulture for a variety of covering, protection and containment applications. Although future volume growth rates appear to be relatively modest, this
is partly due to the replacement of heavier weight traditional textiles, including jute
and sisal sacking and twine, by lighter, longer lasting synthetic substitutes, especially
However, modern materials are also opening up new applications. Lightweight
spunbonded ﬂeeces are now used for shading, thermal insulation and weed suppression. Heavier nonwoven, knitted and woven constructions are employed for
wind and hail protection. Fibrillated and extruded nets are replacing traditional
baler twine for wrapping modern circular bales. Capillary nonwoven matting is used
in horticulture to distribute moisture to growing plants. Seeds themselves can be
incorporated into such matting along with any necessary nutrients and pesticides.
The bulk storage and transport of fertiliser and agricultural products is increasingly
undertaken using woven polypropylene FIBCs (ﬂexible intermediate bulk containers – big bags) in place of jute, paper or plastic sacks.
Agriculture is also an important user of products from other end-use sectors such
as geotextiles for drainage and land reclamation, protective clothing for employees
who have to handle sprays and hazardous equipment, transport textiles for tractors
and lorries, conveyor belts, hoses, ﬁlters and composite reinforcements in the construction of silos, tanks and piping.
28. Technical textiles market – an overview
At sea, ﬁsh farming is a growing industry which uses specialised netting and other
textile products. High performance ﬁbres such as HMPE (e.g. Dyneema and
Spectra) are ﬁnding their way into the ﬁshing industry for the manufacture of
lightweight, ultra-strong lines and nets.
1.5.7 Construction – building and rooﬁng
Textiles are employed in many ways in the construction of buildings, both permanent and temporary, dams, bridges, tunnels and roads. A closely related but distinct
area of use is in geotextiles by the civil engineering sector.
Temporary structures such as tents, marquees and awnings are some of the most
obvious and visible applications of textiles. Where these used to be exclusively made
from proofed heavy cotton, a variety of lighter, stronger, rot-, sunlight- and weatherproof (also often ﬁreproof) synthetic materials are now increasingly required. A
relatively new category of ‘architectural membrane’ is coming to prominence in the
construction of semipermanent structures such as sports stadia, exhibition centres
(e.g. the Greenwich Millenium Dome) and other modern buildings.
Nonwoven glass and polyester fabrics are already widely used in rooﬁng applications while other textiles are used as breathable membranes to prevent moisture
penetration of walls. Fibres and textiles also have a major role to play in building
and equipment insulation. Glass ﬁbres are almost universally used in place of
asbestos now. Modern metal-clad roofs and buildings can be lined with special
nonwovens to prevent moisture condensation and dripping.
Double wall spacer fabrics can be ﬁlled with suitable materials to provide sound
and thermal insulation or serve as lightweight cores for composite materials.
Composites generally have a bright future in building and construction. Existing
applications of glass-reinforced materials include wall panels, septic tanks and
sanitary ﬁttings. Glass, polypropylene and acrylic ﬁbres and textiles are all used to
prevent cracking of concrete, plaster and other building materials. More innovative
use is now being made of glass in bridge construction. In Japan, carbon ﬁbre is
attracting a lot of interest as a possible reinforcement for earthquake-prone buildings although price is still an important constraint upon its more widespread use.
Textiles are also widely employed in the course of construction operations themselves, in uses as diverse as safety netting, lifting and tensioning ropes and ﬂexible
shuttering for curing concrete.
The potential uses for textiles in construction are almost limitless. The difﬁculties
for textile manufacturers operating in this market include the strongly cyclical nature
of the construction industry and the unevenness of major projects, the long testing
and acceptance procedures and, perhaps above all, the task of communicating these
developments to a diverse and highly fragmented group of key speciﬁers, including
architects, construction engineers and regulatory bodies. The construction requirements, practices and standards of just about every country and region are different
and it has, so far, proved very difﬁcult for any acknowledged global leaders to emerge
in this market as they have, for example, in industrial and automotive textiles.
1.5.8 Packaging and containment
Important uses of textiles include the manufacturing of bags and sacks, traditionally from cotton, ﬂax and jute but increasingly from polypropylene. The strength
Handbook of technical textiles
and regularity of this synthetic material, combined with modern materials handling
techniques, has allowed the introduction of FIBCs for the more efﬁcient handling,
storage and distribution of a variety of powdered and granular materials ranging
from fertiliser, sand, cement, sugar and ﬂour to dyestuffs. ‘Big bags’ with typical carrying capacities from one half to 2 tonnes can be ﬁtted with special liners, carrying
straps and ﬁlling/discharge arrangements. The ability to re-use these containers in
many applications in place of disposable ‘one-trip’ bags and sacks is another powerful argument for their wider use.
An even faster growing segment of the packaging market uses lighter weight
nonwovens and knitted structures for a variety of wrapping and protection
applications, especially in the food industry. Tea and coffee bags use wet-laid nonwovens. Meats, vegetables and fruits are now frequently packed with a nonwoven
insert to absorb liquids. Other fruits and vegetable products are supplied in knitted
Strong, lightweight spunbonded and equivalent nonwoven paper-like materials
are particularly useful for courier envelopes while adhesive tapes, often reinforced
with ﬁbres, yarns and fabrics, are increasingly used in place of traditional twine.
Woven strappings are less dangerous to cut than the metal bands and wires traditionally used with densely packed bales.
A powerful driver of the development and use of textiles in this area is increasing environmental concern over the disposability and recycling of packaging
materials. Legislation across the European Union, implemented especially vigorously in countries such as Germany, is now forcing many manufacturers and
distributors of products to rethink their packaging practices fundamentally.
1.5.9 Sport and leisure
Even excluding the very considerable use of textiles in performance clothing and
footwear, there are plenty of opportunities for the use of technical textiles throughout the sports and leisure market. Applications are diverse and range from artiﬁcial
turf used in sports surfaces through to advanced carbon ﬁbre composites for racquet
frames, ﬁshing rods, golf clubs and cycle frames. Other highly visible uses are balloon
fabrics, parachute and paraglider fabrics and sailcloth.
Growth rates are well above average and unit values are often very high. The
sports sector is receptive to innovation and developers of new ﬁbres, fabrics and
coatings often aim them at this market, at least initially. Many of the products and
ideas introduced here eventually diffuse through to the volume leisure market and
even the street fashion market.
1.5.10 Geotextiles in civil engineering
Although still a surprisingly small market in volume and value terms, considering
the amount of interest and attention it has generated, the geosynthetics market
(comprising geotextiles, geogrids and geomembranes) is nevertheless expected to
show some of the highest growth rates of any sector over the foreseeable future.
The economic and environmental advantages of using textiles to reinforce, stabilise, separate, drain and ﬁlter are already well proven. Geotextiles allow the building of railway and road cuttings and embankments with steeper sides, reducing
the land required and disturbance to the local environment. Revegetation of these
30. Technical textiles market – an overview
embankments or of the banks of rivers and waterways can also be promoted using
appropriate materials. There has been renewed interest in ﬁbres such as woven jute
as a biodegradable temporary stabilising material in such applications.
As in the case of construction textiles, one of the problems faced by manufacturers and suppliers of these materials is the sheer diversity of performance
requirements. No two installations are the same in hydrological or geological terms
or in the use to which they will subsequently be put. Suppliers to this market need
to develop considerable expertise and to work closely with engineers and consultants in order to design and specify suitable products.
Because of the considerable areas (quantities) of fabric that can be required in
a single project, cost is always a consideration and it is as essential not to overspecify
a product as not to underspecify it. Much of the research and development work
undertaken has been to understand better the long term performance characteristics of textiles which may have to remain buried in unpredictable environments
(such as landﬁll and toxic waste sites) for many years and continue to perform to
an adequate standard.
Nonwovens already account for up to 80% of geotextile applications. This is
partly a question of economics but also of the suitability of such textile structures
for many of the ﬁltration and separation duties that they are called upon to perform.
Current interest is in ‘composite’ fabrics which combine the advantages of different
textile constructions such as woven, knitted, nonwoven and membrane materials. To
supply the diversity of fabrics needed for the many different applications of geotextiles, leading specialist manufacturers are beginning to assemble a wide range of
complementary capabilities by acquisition and other means.
1.5.11 Protective and safety clothing and textiles
Textiles for protective clothing and other related applications are another important growth area which has attracted attention and interest somewhat out of proportion to the size and value of the existing market. As in the case of sports textiles,
a number of relatively high value and performance critical product areas have
proved to be an ideal launch pad for a new generation of high performance ﬁbres,
most notably the aramids, but including many other speciality materials.
The variety of protective functions that needs to be provided by different textile
products is considerable and diverse. It includes protection against cuts, abrasion,
ballistic and other types of severe impact including stab wounds and explosions, ﬁre
and extreme heat, hazardous dust and particles, nuclear, biological and chemical
hazards, high voltages and static electricity, foul weather, extreme cold and poor
As well as people, sensitive instruments and processes also need to be protected.
Thus, clean room clothing is an important requirement for many industries including electronics and pharmaceuticals.
In Europe and other advanced industrial regions, strict regulations have been
placed upon employers through the introduction of legislation such as the Personal
Protective Equipment (PPE) at Work Regulations (European Union). Under such
legislation, it is not only necessary to ensure that the equipment and clothing provided is adequate to meet the anticipated hazards but also that it is also used effectively, that is that the garments are well designed and comfortable to wear. This
has opened up a need for continuing research not only into improved ﬁbres and
Handbook of technical textiles
materials but also into increasingly realistic testing and assessment of how garments
perform in practice, including the physiology of protective clothing.
In many developing countries, there has not been the same legislative framework
in the past. However, this is rapidly changing and future market growth is likely to
concentrate less on the mature industrial markets than upon the newly industrialising countries of Asia and elsewhere. The protective clothing industry is still highly
fragmented with much of the innovation and market development being provided
by the major ﬁbre and other materials producers. This could change as some global
suppliers emerge, perhaps without their own direct manufacturing but relying on
contract producers around the world, very much as the mainstream clothing industry does at present.
1.5.12 Ecological protection textiles
The ﬁnal category of technical textile markets, as deﬁned by Techtextil, is technical
textiles for protection of the environment and ecology. This is not a well deﬁned
segment yet, although it overlaps with several other areas, including industrial textiles (ﬁltration media), geotextiles (erosion protection and sealing of toxic waste)
and agricultural textiles (e.g. minimising water loss from the land and reducing the
need for use of herbicides by providing mulch to plants).
Apart from these direct applications, technical textiles can contribute towards
the environment in almost every sphere of their use, for example by reducing weight
in transport and construction and thereby saving materials and energy. Improved
recycleability is becoming an important issue not only for packaging but also for
products such as cars.
Composites is an area which potentially presents problems for the recycleability
of textile reinforcing materials encased within a thermosetting resin matrix.
However, there is considerable interest in and development work being done on
thermoplastic composites which should be far simpler to recycle, for example by
melting and recasting into lower performance products.
Globalisation of technical textiles
If North America and Western Europe have the highest levels of per capita consumption of technical textiles at present (see Table 1.1), then they are also relatively
mature markets. The emerging countries of Asia, Eastern Europe and the rest of
the world are becoming important markets in almost every sphere, from automotive manufacture through to sporting and leisure goods. Technical textiles for food
production, construction and geotextiles are likely to be particularly important. In
the case of the last of these, geotextiles, consumption up to the year 2005 is expected
to grow at over 12% per annum across the whole of Asia compared with less than
6% in Western Europe and the USA. In the case of Eastern Europe and South
America, annual growth rates could be as high as 18% and 16% per annum respectively, although from relatively small base levels at present.
In 2000, the major existing users, North America, Western Europe and Japan, are
expected to account for less than 65% of total technical textile consumption; by the
year 2005, this could be down to 60% and perhaps below 50% by 2010. Consumption of technical textiles in China already exceeds that of Japan, in weight terms at
32. Technical textiles market – an overview
Worldwide consumption of technical textiles by geographical region, 2000–2005
Rest of the world
Source: David Rigby Associates/Techtextil.
least. In 2000, Chinese technical textiles are expected to account for almost 20% of
all textile manufacturing in that country and over 12% of total world consumption
(see Table 1.4).
But globalisation is not just about increasing internationalisation of markets. It
is also about the emergence of companies and supply chains which operate across
national and continental boundaries. Such globalisation has already proceeded furthest in the automotive and transport industry, the largest of the 12 market segments
deﬁned above. It is a path already being followed within the other major segments,
most notably industrial textiles and medical/hygiene textiles and will become
increasingly evident in the remainder.
Characteristics of globalisation include higher levels of international trade and
increased specialisation of manufacture within individual districts, countries and
regions, according to availability of materials, local industry strengths and regional
Relatively low unit value products requiring a signiﬁcant amount of making-up
or other fabrication such as bags and sacks have already seen a signiﬁcant shift of
manufacturing towards the Far East and Eastern Europe. Textiles for tents, luggage
and the technical components of footwear and clothing are now increasingly
sourced close to where many of these products are manufactured for export, for
example China and Indonesia.
Manufacturers in the newly industrialising world are rapidly adopting the latest
materials and processing technologies. Taiwan already has an important composites
manufacturing sector specialising in sports equipment.
Future of the technical textiles industry
The future of technical textiles embraces a much wider economic sphere of activity
than just the direct manufacturing and processing of textiles. The industry’s suppliers include raw materials producers (both natural and artiﬁcial), machinery
and equipment manufacturers, information and management technology providers,
R&D services, testing and certiﬁcation bodies, consultants, education and training
organisations. Its customers and key speciﬁers include almost every conceivable
Table 1.5 Technical textile functions, markets and end-uses
Power, oil, gas
Welders antispatter sheets
Bags & sacks
drive belts &
Handbook of technical textiles
Technical textiles market – an overview
36. Technical textiles market – an overview
downstream industry and ﬁeld of economic activity, including the architects, engineers, designers and other advisors employed by those industries. In between lie
many other interested parties, including environmental, health, safety, business and
free trade regulators, patent and intellectual property agents and lawyers, investors,
bankers, regional investment agencies and providers of development aid.
The task of disseminating and communicating information to all these organisations and individuals is undertaken by a growing number of specialist and generalist publications as well as by international and local trade exhibitions, fairs, seminars
The economic importance of technical textiles worldwide therefore undoubtedly
far exceeds the $60 billion estimated in Tables 1.2–1.4 just for basic ﬁbres, yarns and
1.7.1 A changing strategic environment
If the 1980s was a period when the technical textiles industry enjoyed a rapid and
increasing awareness of its existence by the outside world (as well as within the
mainstream textile industry), then the 1990s was an era of more mature commercial development and consolidation as ﬁbre producers and textile manufacturers
alike concentrated on overhauling and refocusing their businesses in the wake of
The new millennium promises even ﬁercer international competition which
will see manufacturers striving to engineer costs downwards and develop global
economies of scale in production and product development. Technical textiles will
become better ‘value for money’ than ever before and this should open the way
towards further applications as existing end-uses mature.
Individual companies will become less deﬁned by the technologies and materials they use than by the markets and applications they serve. Table 1.5 summarises some of the key market areas and the functions which technical textiles
perform, with examples of individual products in each category. It does not pretend
to be an exhaustive list which would run into many thousands of products and would
constantly be changing.
1. The Textile Institute, Textile Terms and Deﬁnitions, Tenth Edition, Textile Institute, Manchester, 1994.
2. sabit adanur, Wellington Sears Handbook of Industrial Textiles, Technomic, Lancaster PA (USA),
3. ISO 9092:1988 Deﬁnition of nonwovens.
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
A number of deﬁnitions1–3 have been used to describe the term ‘technical textiles’
with respect to their intended use, functional ability and their non-aesthetic or decorative requirements. However, none of these carefully chosen words include the
fundamental ﬁbre elements, technical or otherwise, which make up the technical
textile structures. The omission of the word ‘ﬁbre’ may indeed be deliberate as most
technical textile products are made from conventional ﬁbres that are already well
established. In fact over 90% of all ﬁbres used in the technical sector are of the conventional type.4 Specially developed ﬁbres for use in technical textiles are often
expensive to produce and have limited applications.
Historically, utilisation of ﬁbres in technical capacities dates back to the early
Egyptians and Chinese who used papyrus mats to reinforce and consolidate the
foundations respectively of the pyramids and the Buddhist temples.5,6 However,
their serious use in modern civil engineering projects only began after the ﬂoods of
1953 in The Netherlands in which many people lost their lives. The event initiated
the famous Delta works project in which for the ﬁrst time synthetic ﬁbres were
written into the vast construction programme.7 Since then, geotextiles in particular
have matured into important and indispensable multifunctional materials.
Use of silk in semitechnical applications also goes back a long way to the lightweight warriors of the Mongolian armies, who did not only wear silk next to
their skin for comfort but also to reduce penetration of incoming arrows and enable
their subsequent removal with minimal injury. Use of silk in wound dressing
and open cuts in web and fabric form also dates back to the early Chinese and
In light of extensive utilization of conventional ﬁbres in the technical sector, this
chapter initially attempts to discuss ﬁbres under this category highlighting their
importance and the scope of their versatility. The discussion covers concisely an
outline of ﬁbre backgrounds, chemical compositions and their salient characteristics. It then introduces other ﬁbres which have been specially developed to perform
38. Technical ﬁbres
under extreme stress and/or temperature; ultraﬁne and novel ﬁbres are also discussed. Finally, the chapter concludes by identifying areas of application and the
roles that selected ﬁbres play in fulﬁlling their intended purpose.
Table 2.1 presents the complete range of ﬁbres available to the end-user and
some of their mechanical properties.
2.2.1 Natural ﬁbres
Cotton accounts for half of the world’s consumption of ﬁbres and is likely to remain
so owing to many of its innate properties and for economical reasons8 that will not
be discussed here. Cotton is made of long chains of natural cellulose containing
carbon, hydrogen and oxygen otherwise known as polysaccharides. The length of
the chains determines the ultimate strength of the ﬁbre. An average of 10 000 cellulosic repeat or monomeric units make up the individual cellulose chains which are
about 2 mm in length. The linear molecules combine into microﬁbrils and are held
together by strong intermolecular forces to form the cotton ﬁbre. The unique physical and aesthetic properties of the ﬁbre, combined with its natural generation and
biodegradability, are reasons for its universal appeal and popularity. Chemical treatments such as Proban9 and Pyrovatex10 are two examples of the type of durable ﬁnishes that can be applied to make cotton ﬁre retardant. High moisture absorbency,
high wet modulus and good handle are some of the more important properties of
Wool, despite its limited availability and high cost, is the second most important
natural ﬁbre. It is made of protein: a mixture of chemically linked amino acids which
are also the natural constituents of all living organisms. Keratin or the protein in
the wool ﬁbre has a helical rather than folded chain structure with strong inter- and
intrachain hydrogen bonding which are believed to be responsible for many of its
unique characteristics. Geographical location, the breeding habits of the animals,
and climatic conditions are some of the additional variables responsible for its properties. The overall high extensibility of wool, its natural waviness and ability to trap
air has a coordinated effect of comfort and warmth, which also make it an ideal
insulating material. The sophisticated dual morphology of wool produces the characteristic crimp which has also been an inspiration for the development of some
highly technical synthetic ﬁbres. Wool is inherently ﬁre retardant, but further
improvements can be achieved by a number of ﬁre-retardant treatments. Zirconium- and titanium-treated wool is one such example which is now universally
referred to as Zirpro (IWS) wool.11
Flax, jute, hemp and ramie, to name but a few of the best ﬁbres, have traditionally taken a secondary role in terms of consumption and functional requirements.
They are relatively coarse and durable, and ﬂax has traditionally been used for linen
making. Jute, ramie and to a lesser extent other ﬁbres have received attention within
the geotextile sector of the ﬁbre markets which seeks to combine the need for temporary to short-term usage with biodegradability, taking into account the regional
availability of the ﬁbres.
Silk is another protein-based ﬁbre produced naturally by the silkworm, Bombyx
Mori or other varieties of moth. Silk is structurally similar to wool with a slightly
Fibres available to the end-user and associated mechanical properties
High strength high modulus
High chemical and
Ultraﬁne and novelty ﬁbres
e.g. cotton, wool, silk, jute,
e.g. viscose, acetates tencel,
e.g. polyamide, polyester,
e.g. Kevlar (Du Pont) and
e.g. Dyneema (DSM) and
Spectra (Allied Signal)
e.g. Nomex (Du Pont)
and Conex (Teijin)
Alumina (e.g. Safﬁl)
High modulus silicon
ﬁbres, e.g. Panox (SGL) Carbide & silicon
(Victrex and Zyex)
sulphide, PPS, e.g.
PTFE, e.g. Teﬂon (Du Pont)
(Inspec formerly Lenzing) P84
Microﬁbres; (linear density
Solar energy absorbing ﬁbres
0.1–0.5 N tex-1
2–18 N tex-1
% Elongation: 2–7
1.5–3 N tex-1
25–150 N tex-1
% Elongation: 1–8
1–2 N tex-1
15–25 N tex-1
% Elongation: 1–4
0.1–0.4 N tex-1
2–15 N tex-1
% Elongation: 2–17
LOI: limiting oxygen index = minimum fraction of oxygen in nitrogen necessary to sustain burning.
0.5–2 N tex-1
70–220 N tex-1
% Elongation: 0–1.5
Handbook of technical textiles
40. Technical ﬁbres
different combination of amino acids which make up the protein or the ﬁbroin, as
it is more appropriately known. Silk is the only naturally and commercially produced continuous ﬁlament ﬁbre which has high tenacity, high lustre and good dimensional stability. Silk has been and will remain a luxury quality ﬁbre with a special
place in the ﬁbre market. However, its properties of biocompatibility and gradual
disintegration, as in sutures, have long been recognised in medical textiles.
2.2.2 Regenerated ﬁbres
Viscose rayon was the result of the human race’s ﬁrst attempts to mimic nature in
producing silk-like continuous ﬁbres through an oriﬁce. Cellulose from wood pulp is
the main constituent of this novel system, started commercially in the early 1920s.
Thin sheets of cellulose are treated with sodium hydroxide and aged to allow molecular chain breakage. Further treatment with carbon disulphide, dissolution in dilute
sodium hydroxide and ageing produces a viscous liquid, the viscose dope, which is
then extruded into an acid bath. The continuous ﬁlaments that ﬁnally emerge are
washed, dried and can be cut to staple lengths. The shorter cellulose molecules in
viscose and their partial crystallisation accounts for its rather inferior physical properties relative to cotton. Further development and reﬁnement of the manufacturing
technique have created a whole range of ﬁbres with improved properties. High tenacity and high wet modulus viscose compare in all but appearance to cotton in both dry
and wet conditions. Chemically altered regenerated cellulose di- and triacetates do
not burn like cotton and viscose to leave a ﬂuffy black ash, but melt and drip instead.
This characteristic enables them to be shaped or textured to enhance their visual and
aesthetic appeal. Hollow viscose modiﬁcations give enhanced bulk and moisture
absorbency and have an improved cotton-like feel.
Fire-retardant (FR) viscose was ﬁrst introduced in the 1960s. A major example
is produced by Lenzing in Austria by incorporating organophosphorous compounds
into the spinning dope prior to extrusion. The additive is reasonably stable and has
no chemical interaction with the cellulose molecules. It is also unaffected by bleaching, washing, dry cleaning, dyeing and ﬁnishing processes.10 Early in the 1990s
Kemira (now Sateri Fibres) of Finland introduced an alternative version of FR
viscose known as Visil in which polysilicic acid is present. The ﬁbre chars upon
heating leaving a silica residue.
Lyocell,12 is the latest addition to this series of ﬁbres, commercially known as
Tencel (Acordis), has all the conventional properties of viscose in addition to its
much praised environmentally friendly production method. The solvent used is
based on non-toxic N-methyl morpholine oxide used in a recyclable closed loop
system, which unlike the viscose process avoids discharge of waste. Highly absorbent
derivatives of Tencel, known as Hydrocell are establishing a foothold in wound
dressing and other medical-related areas of textiles.
2.2.3 Synthetic ﬁbres
All synthetic ﬁbres originate from coal or oil. The ﬁrst synthetic ﬁbre that appeared
on the world market in 1939 was nylon 6.6. It was produced by DuPont and gained
rapid public approval. A series of nylons commonly referred to as polyamides now
exists in which the amide linkage is the common factor. Nylon 6.6 and nylon 6 are
most popular in ﬁbre form. They are melt extruded in a variety of cross-sectional
shapes and drawn to achieve the desired tenacity. They are well known for their high
Handbook of technical textiles
extensibility, good recovery, dimensional stability and relatively low moisture
absorbency. Nylon 6.6 in particular soon became a popular household carpet ﬁbre
and was developed into ﬁbres commonly known as Antron13 manufactured by
DuPont. Antron ﬁbres of various generations use additives, varied cross-sectional
shapes and modiﬁed surface characteristics to enhance the aesthetic and visual
appeal of carpets as well as improving their resilience and dissipating static charges.
Nylon was later surpassed by the even more popular ﬁbre known as polyester,
ﬁrst introduced as Dacron by DuPont in 1951. Polyester is today the second most
used ﬁbre after cotton and far ahead of other synthetics both in terms of production and consumption. Polyethylene terephthalate or polyester is made by condensation polymerisation of ethylene glycol and terephthalic acid followed by melt
extrusion and drawing. It can be used in either continuous form or as short staple
of varying lengths. The popularity of polyester largely stems from its easycare characteristics, durability and compatibility with cotton in blends. Its very low moisture
absorbency, resilience and good dimensional stability are additional qualities. Many
manufacturers across the world produce polyester under different commercial
names with almost tailor-made properties. A high glass transition temperature of
around 70 °C with good resistance to heat and chemical degradation also qualiﬁes
this polymer for most technical textile applications. These will be discussed in
greater detail later. Flame-retardant Trevira CS and Trevira high tenacity, both polyesters developed and marketed by Trevira GmbH in Germany, are examples of the
many varieties available today.
Wool-like properties are shown by polyacrylic ﬁbres which are produced by the
polymerisation of acrylonitrile using the addition route into polyacrylonitrile. They
can then be spun into ﬁbres by dry or wet spinning methods. Orlon14 was produced
by DuPont. It had a distinctive dumbbell shaped cross-section and was extruded by
the dry process in which the solvent is evaporated off. Acrilan15 produced by Monsanto and Courtelle produced by Acordis are spun by the wet extrusion technique
and have near circular cross-sections. Acrylic ﬁbres now also appear in bicomponent form with wool-like characteristics. Chemically modiﬁed acrylics, principally
the modacrylics, include chlorine atoms in their molecular structure which are
responsible for their low burning behaviour and, unlike acrylics, have the ability to
self-extinguish once the source of ignition has been removed. A selected ﬁbre in
terms of ﬁbre chemistry is Oasis,16 a superabsorbent ﬁbre made by the collaborative efforts of Acordis and Allied Colloids, based on crosslinking copolymers of
acrylic acid. This ﬁbre is claimed to absorb moisture many times its own weight and
holds it even under pressure. Its application in hygiene and medical care in different forms is being pursued.
Polyoleﬁn ﬁbres include both polyethylene and polypropylene made by addition
polymerisation of ethylene and propylene and subsequent melt extrusion, respectively. Polyethylene has moderate physical properties with a low melting temperature of about 110 °C for its low density form and about 140 °C for its high density
form which severely restricts its application in low temperature applications.
Polypropylene has better mechanical properties and can withstand temperatures of
up to 140 °C before melting at about 170 °C. Both polymers have a density less than
that of water which allows them to ﬂoat as ropes, nets and other similar applications. The availability, low cost and good resistance to acid and alkaline environments of polypropylene has greatly inﬂuenced its growth and substantial use in
42. Technical ﬁbres
Stress/strain behaviour of some common ﬁbres.
Finally, elastane ﬁbres17 are synthetic-based elastomeric polymers with at least
85% segmented polyurethane in their structure. They have rubber-like properties,
which means they can be extended up to six or more times their original length.
They are used in combination with most natural and synthetic ﬁbres in knitted and
woven materials. They were initially produced by DuPont in 1959 under the now
well-known trademark of Lycra.
Figure 2.1 presents typical stress/strain behaviour for most conventional ﬁbres.
Tenacity, modulus and percentage elongation ranges for most conventional ﬁbres
are also given at the bottom of Table 2.1.
High strength and high modulus organic ﬁbres
Keller’s much-published18 contribution to the understanding of crystal growth in
1957 and conﬁrmation of the tendency of polymers to form folded-chain crystals,
provided the insight and inspiration for development of high strength, high modulus
organic ﬁbres that would surpass conventional ﬁbres. During crystallisation, long
chains of molecules fold back on themselves to form folded-chain crystals which
only partly unfold during normal drawing. In the Netherlands in the 1970s DSM
developed a super drawing technique known as gel spinning, which uses dilute solutions of ultra-high molecular weight polymers such as polyethylene to unfold the
chains further and thus increase both tensile strength and ﬁbre modulus. Ultra-high
molecular weight polyethylene (UHMWPE) ﬁbres, Dyneema or Spectra, are today
the strongest ﬁbres known, with tensile moduli in excess of 70 GN m-2. Weight for
weight this ﬁbre genus is claimed to be 15 times stronger than steel and twice as
strong as aromatic polyamides such as Kevlar.19 It is also low in density, chemically
inert and abrasion resistant. It, however, melts at around 150 °C and thermally
degrades at 350 °C which restrict its use to low temperature applications.
To achieve even better performance characteristics at higher temperatures, other
means of ﬁbre production were explored in the 1960s. One successful approach
eventually led to the advent of liquid crystalline polymers. These are based on polymerisation of long stiff molecules such as para-phenylene terephthalamide achieving molecular weights averaging to around 20 000. The inﬂuence of the stiff aromatic
rings, together with hydrogen-bonding crosslinks, combines the best features of both
the polyamides and the polyesters in an extended-chain conﬁguration.18–20 Molecular orientation of these ﬁbres is brought about by capillary shear along the ﬂow of
Handbook of technical textiles
the polymer as it exits from the spinneret thus overriding the need for subsequent
drawing. Kevlar by DuPont and Twaron by Akzo (now Acordis) were the ﬁrst of
such ﬁbres to appear in the early 1970s. There now exists a series of ﬁrst, second
and third generations of para-aramids. Kevlar HT for instance, which has 20%
higher tenacity and Kevlar HM which has 40% higher modulus than the original
Kevlar 29 are largely utilised in the composite and the aerospace industries. Paraaramids generally have high glass transition temperatures nearing 370 °C and do not
melt or burn easily, but carbonise at and above 425 °C. All aramid ﬁbres are however
prone to photodegradation and need protection against the sun when used out of
doors. These will be discussed later.
Other high tenacity and high modulus ﬁbres include the isotropically spun Technora (Teijin) and Supara, based upon para-aramid copolymers, with slightly lower
maximum strength and modulus values than Kevlar. Several other melt-spinnable
liquid crystalline polymers are also available.21
High chemical- and combustion-resistant organic ﬁbres
The ﬁbres discussed in the previous section were developed following earlier observations that aromatic polymer backbones yielded improved tensile and heat resistance compared with conventional ﬁbres. However, if the polymer chains have lower
symmetry and order, then polymer tractability and textile ﬁbre characteristics are
improved. Solvent-spun Nomex and Conex were the ﬁrst so-called meta-aramids
made from poly(meta-phenylene isophthalamide) and were produced by DuPont
in 1962 and by Teijin in 1972, respectively. The meta-phenylene isophthalamide molecule is identical in all but the position of its —NH— and —CO— groups to paraphenylene terephthalamide (or Kevlar) molecules. The different positioning of
these groups in meta-aramids creates a zig-zag molecular structure that prevents it
from full crystallisation thus accounting for its relatively poorer tensile properties.
However, Nomex is particularly well known for its resistance to combustion, high
decomposition temperature prior to melting and high limited oxygen index (LOI),
the minimum amount of oxygen required to induce ignition.
Melt-spinnable aromatic ﬁbres with chains containing paraphenylene rings, like
polyether ether ketone (PEEK),23 polyether ketone (PEK) and poly(p-phenylene
sulphide) (PPS),22 also have high melting points but, since their melting points occur
prior to their decomposition temperature, they are unsuitable for ﬁre-retardant
applications. However, their good chemical resistance renders them suitable for low
temperature ﬁltration and other corrosive environments.
The polyheterocyclic ﬁbre, polybenzimidazole or PBI, produced by HoechstCelanese has an even higher LOI than the aramids. It has excellent resistance to
both heat and chemical agents but remains rather expensive. P84, initially produced
by Lenzing and now produced by Inspec Fibres, USA, comprises polyimide groups
that yield reasonably high resistance to ﬁre and chemical attack. The acrylic
copolymer-based ﬁbre produced by Acordis known as Inidex (although now no
longer produced) unlike many aramid ﬁbres has high resistance to UV (ultraviolet)
radiation and a fairly high LOI at the expense of much reduced tenacity and rather
low long-term exposure resistance to heat.
Oxidised acrylic ﬁbre, best known as Panox (SGL, UK) is another crosslinked,
high combustion-resistant material produced by combined oxidation and pyrolysis
44. Technical ﬁbres
Table 2.2 LOI and tenacity range of some high chemicaland combustion-resistant organic ﬁbres
of acrylic ﬁbres at around 300 °C. Although black in appearance, it is not classed as
carbon ﬁbre and preserves much of its original non-carbonaceous structure. In addition, it does not have the graphitic or turbostratic structure of carbon ﬁbres. It
retains a sufﬁciently high extension-at-break to be subjected to quite normal textile
processes for yarn and fabric formation.24 Panox has a very high LOI of 0.55. Fully
carbonised, or carbon ﬁbres with even higher tensile properties, are achieved by full
carbonisation of these oxidised precursor ﬁbres or by the melt spinning of liquid
crystalline mesophase pitch followed by their oxidation and pyrolysis. These are discussed again in the section on inorganic ﬁbres.
Table 2.2 shows the LOI and tenacity range of some of the better known high
chemical- and combustion-resistant organic ﬁbres.
High performance inorganic ﬁbres
Any ﬁbre that consists of organic chemical units, where carbon is linked to hydrogen and possibly also to other elements, will decompose below about 500 °C and
cease to have long-term stability at considerably lower temperatures. For use at high
temperatures it is therefore necessary to turn to inorganic ﬁbres and ﬁbres that
consist essentially of carbon.25
Glass, asbestos and more recently carbon are three well-known inorganic ﬁbres
that have been extensively used for many of their unique characteristics. Use of glass
as a ﬁbre apparently dates back to the ancient Syrian and Egyptian civilisations26
which used them for making clothes and dresses. However, the very high modulus
or stiffness displayed by these ﬁbres means that they are quite brittle and can easily
be damaged by surface marks and defects. They are, therefore, best utilised by
embedding in matrix forms where the ﬁbres are fully protected. Epoxy resins, polyester and other polymers, as well as cement, have commonly been used both to
protect and to make use of their contributory strength. Glass-reinforced boat hulls
and car bodies, to name but two application areas of such composites, reduce overall
weight and cost of fabrication as well as eliminating the traditional problems of
rotting wood and rusting metals associated with traditional materials. Their good
resistance to heat and very high melting points have also enabled them to be used
as effective insulating materials.
Handbook of technical textiles
Asbestos27 is a generic name for a variety of crystalline silicates that occur naturally in some rocks. The ﬁbres that are extracted have all the textile-like properties
of ﬁneness, strength, ﬂexibility and more importantly, unlike conventional ﬁbres,
good resistance to heat with high decomposition temperatures of around 550 °C.
Their use as a reinforcement material has been found in clay-rich prehistoric
cooking pots discovered in Finland.28 In more recent times they have been extensively used to reinforce brittle matrices such as cement sheeting, pipes, plastics29 and
also as heat insulators. However, with the discovery of their carcinogenic hazards,
their use has gradually declined and alternative ﬁbres have been developed to
replace them totally.
High purity, pyrolysed acrylic-based ﬁbres are classiﬁed as carbon ﬁbres. The
removal of impurities enhances carbon content and prevents the nucleation and
growth of graphite crystals which are responsible for loss of strength in these ﬁbres.
Carbon ﬁbres with different structures are also made from mesophase pitch. The
graphite planes in PAN-based ﬁbres are arranged parallel to the ﬁbre axis
rather than perpendicular as is the case with pitch-based carbon ﬁbres.28 Their high
strength and modulus combined with relatively low extensibility means that they
are best utilised in association with epoxy or melt-spinnable aromatic resins as
Increasing demand in the defence and aerospace industries for even better performance under extreme conditions led, within the last quarter of the 20th century,
to yet another range of new and rather expensive metal oxides, boron and siliconbased ﬁbres. These are often referred to as ceramic ﬁbres and will now be brieﬂy
Aluminosilicate compounds are mixtures of aluminium oxide (Al2O) and silicon
oxide (SiO2); their resistance to temperature depends on the mixing ratio of the two
oxides. High aluminium oxide content increases their temperature tolerance from
a low of 1250 °C to a maximum of 1400 °C. However, despite their high temperature resistance, these ﬁbres are not used in high stress applications owing to their
tendency to creep at high temperatures.29 Their prime applications are in insulation
of furnaces and replacement of asbestos ﬁbres in friction materials, gaskets and
packings.30 Both aluminium oxide or alumina ﬁbres and silicon oxide or silica ﬁbres
are also produced. Pure boron ﬁbres are too brittle to handle but they can be coated
on tungsten or carbon cores. Their complex manufacturing process makes them
rather expensive. Their prime application is in lightweight, high strength and high
modulus composites such as racket frames and aircraft parts. Boron ﬁbre use is
limited by their thickness (about 16 mm), their relatively poor stability in metal
matrices and their gradual loss of strength with increasing temperature.31 Boron
nitrides (BN) are primarily used in the electronic industry where they perform both
as electrical insulators and thermal conductors.
The most outstanding property of silicon carbide (SiC) is the ability to function
in oxidizing conditions up to 1800 °C with little loss of mechanical properties. Silicon
carbide exceeds carbon ﬁbre in its greater resistance to oxidation at high temperatures, its higher compressive strength and better electrical resistance. SiC ﬁbres
containing carbon, however, lose some tensile properties at the expense of gaining
better electrical conductivity.
Finally, many of the inorganic ﬁbres so far referred to are now also produced
in microcrystalline or whisker form and not in the more normal textile-ﬁbre form.
Whiskers have extremely good mechanical properties and their tensile strength is
46. Technical ﬁbres
usually three to four times those of most reinforcing ﬁbres. They are, however, costly
to produce and their inclusion into composite structures is both difﬁcult and
Ultra-ﬁne and novelty ﬁbres
Ultra-ﬁne or microﬁbres were developed partly because of improved precision in
engineering techniques and better production controls, and partly because of the
need for lightweight, soft waterproof fabrics that eliminate the more conventional
coating or lamination processes.32 As yet there are no universal deﬁnitions of
microﬁbres. Textile Terms and Deﬁnitions2 simply describes them as ﬁbres or ﬁlaments with linear densities of approximately 1.0 dtex or less. Others33,34 have used
such terms as ﬁne, extra-ﬁne and micro-ﬁne corresponding to linear densities
ranging from 3.0 dtex to less than 0.1 dtex. They are usually made from polyester
and nylon polymers, but other polymers are now being made into microﬁbres. The
Japanese ﬁrst introduced microﬁbres in an attempt to reproduce silk-like properties with the addition of enhanced durability. They are produced by at least
three established methods including island-in-sea, split process and melt spinning
techniques and appear under brand names such as Mitrelle, Setila, Micrell, Tactel
and so on. Once in woven fabric form their ﬁne diameter and tight weave allows
up to 30 000 ﬁlaments cm-2, making them impermeable to water droplets whilst
allowing air and moisture vapour circulation. They can be further processed to
enhance other characteristics such as peach-skin and leather-like appearances. The
split technique of production imparts sharp-angled edges within the ﬁbre surface,
which act as gentle abraders when made into wiping cloths that are used in the
optical and precision microelectronic industries. Microﬁbres are also used to
make bacteria barrier fabrics in the medical industries. Their combined effect of low
diameter and compact packing also allows efﬁcient and more economical dyeing
Finally, constant pressure to achieve and develop even more novel applications
of ﬁbres has led to a number of other and, as yet, niche ﬁbrous products. In principle, the new ideas usually strive to combine basic functional properties of a textile
material with special needs or attractive effects.
For example, Solar-Aloha, developed by Descente and Unitika in Japan,35
absorbs light of less than 2 mm wavelength and converts it to heat owing to its zirconium carbide content. Winter sports equipment made from these materials use
the cold winter sun to capture more than 90% of this incident energy to keep the
wearer warm. Another interesting material gives rise to thermochromic fabrics
made by Toray which have a uniform coating of microcapsules containing heatsensitive dyes that change colour at 5 °C intervals over a temperature range of -40
°C to 80 °C creating ‘fun’ and special effects.
Cripy 65 is a scented ﬁbre produced by Mitsubishi Rayon (R) who have enclosed
a fragrant essence in isolated cavities along the length of hollow polyester ﬁbres.
The scent is gradually released to give a consistent and pleasant aroma. Pillows and
bed linen made from these materials are claimed32 to improve sleep and sleeping
disorders. The effect can also be achieved by printing or padding microcapsules containing perfumes into fabrics which subsequently burst and release the perfume.
With careful handling, garments made from these materials are said to maintain this
Handbook of technical textiles
Stress/strain curves of range of available ﬁbres.
property for up to two years. Infrared-emitting and bacteria-repelling ﬁbres are
some of the other emerging novel ﬁbres.
Figure 2.2 shows stress/strain values for a selected range of the ﬁbres discussed.
The remainder of this chapter focuses on the vast application areas of ﬁbres
giving examples in each category with respect to their functional requirements, limitations and means of optimising their effectiveness.
Table 2.3 summarises applications into ﬁve major areas.
Civil and agricultural engineering
Natural ﬁbres such as ﬂax, jute and ramie can be used for most temporary applications where, for instance, soil erosion is the problem. The geotextiles made from
these natural polymers help to prevent the erosion of soils by allowing vegetative
growth and their subsequent root establishment. Once the purpose is served, the
geotextile material gradually disintegrates into the soil.
In most medium to long term applications however, where physical and chemical durability and dimensional stabilities are of prime concern, synthetic ﬁbres are
preferred. There are currently at least six synthetic polymers considered suitable for
this purpose; they include:
Polypropylene is by far the most utilised geotextile, followed by polyester, the other
three trailing behind with polyamide as the least used synthetic polymer. Paraaramids are only used where very high creep resistance and tolerance to prolonged
heating are required.36
Generally, geosynthetics must have lifetimes which are deﬁned and relate to their
function. Durability, therefore, is mainly determined by the resistance offered by the
component ﬁbre and its assembled structure to the degrading species that causes a
reduction in the tensile and mechanical properties.37 At least three main degrading
mechanisms have been identiﬁed that ultimately determine the durability and life
of the contending polymer; they include:
48. Table 2.3
Applications of technical textiles
Civil & agricultural Engineering
Geotextiles, geomembranes and
Soil stabilization for vegetative
Underground hoses (used for
irrigation & addition of
fertilisers and pesticides)
Medical & hygiene
Protection & defence
Flexible container carriers
Barriers to bacteria
Synthetic sutures, etc.
Barriers to: chemical
moisture, ﬂame and
e.g. Vests, Helmets,
Sports & leisure
Clean room suits
Gas & liquid ﬁlters
Nonwoven, woven, knitted
(plastic or metal resins),
knitted (warp/weft), knitted (warp/weft),
braided, composites, etc.
Form of application
Nonwoven, woven, warp
knitted, grids, composites,
Automotive & aeronautics
Handbook of technical textiles
Physical degradation is usually sustained during transport or installation in one form
or another. Initiation of cracks is normally followed by their subsequent propagation under environmental or normal stress. In the ﬁrst instance, polymer susceptibility to physical degradation depends on such factors as the weight of the
geotextile; generally lightweight or thin geotextiles suffer larger strength losses than
thick and heavy materials. Secondly, woven geotextiles suffer slightly larger strength
losses than nonwovens, owing to their greater stiffness and, ﬁnally, the generic
nature of the polymer itself plays an important role. Polyester, for instance, suffers
greater strength losses than polyoleﬁn ﬁbres owing to its high glass transition temperature of around 70 °C. Under normal soil conditions, the polymer is relatively
brittle and therefore susceptible to physical damage.38 Polypropylene with its glass
transition averaging at about -10 °C is much more pliable under these conditions
but suffers from the rather critical phenomenon of extension with time or creep.
Chemical degradation is the next mechanism by which chemical agencies, often
in combination with ultraviolet light or/and heat, attack the polymer whilst in use
or being stored. The presence of energy starts off a self-destructing chain of events
that ultimately renders the polymer ineffective. Ultraviolet radiation normally
attacks the surface of the polymer and initiates chain breakage or scission which
leads to embrittlement and eventual failure of the polymer. Generally, chemical
degradation is a function of polymer type, thickness and availability of stabilizers.
The type, quantity, and distribution of stabilizers39 also controls the degree of resistance to degradation. Polyoleﬁns are particularly susceptible to ultraviolet degradation and need protection using light-stabilising additives. Oxidation due to heat
operates similarly by weakening the polymer thus causing rapid degradation. A
range of antioxidants are often included in the polymer during manufacture and
processing to minimise this harmful effect.
Biological degradation can result from at least three types of microbiological
attack: direct enzymatic attack, chemical production by microorganisms which may
react destructively with the polymer, and attack on the additives within the
polymer.40,41 High molecular weight polymers are much more immune to biological
attack than low molecular weight polymers because microorganisms cannot easily
locate the molecular chain endings. However, some microorganisms can permeate
less digestible polymers in order to gain access to food.
Automotive and aeronautics
Mechanical functionality has increasingly become an almost secondary requirement
for travel safety, weight efﬁciency, comfort and material durability of the transporting medium. From bicycles to spacecraft, ﬁbres in one form or another fulﬁl these
important requirements. Carbon ﬁbre reinforcement of the frame of a bicycle ridden
in the 1992 Olympics was the ﬁrst of its kind to allow a comfortable win ahead of
its competitors.41 The one-piece, light, ﬁbre-reinforced composite structure and
design of the bike have since become an earmark of this industry. In the simplest
terms, composites utilise unique ﬁbre properties such as strength, stiffness and
50. Technical ﬁbres
elasticity whilst incorporating the compression resistance, and torsion and bending
characteristics of the matrix used.42 Glass ﬁbres have been traditionally used for the
manufacture of boat hulls and car bodies. UHMWPE, aramids and carbonreinforced composites in a variety of matrix materials are now routinely produced
and utilised in low to very high temperature applications.
Reinforcement of tyres is another area where the transport industry has beneﬁted from ﬁbres and where rapid temperature change and changing weather conditions demand effective response and durability. High tenacity viscose and
polyester yarns built into the internal structure of tyres now address these needs
adequately. In addition to all the obvious upholstery materials used in the interior
of cars, trains and aeroplanes, ﬁbres are now used in one form or another in such
parts as the engine components, fan belts, brake pads, door panels, seat skeletons,
seat belts and air bags. Fire-retardant additives or inherently ﬁre-retardant ﬁbres
are today standard requirements in the public sector use of all transport in order to
Medical and hygiene applications
Fibres used in relation to health care and surgery may be classiﬁed depending on
whether they are natural or synthetic, biodegradable or non-biodegradable. All
ﬁbres used, however, must be non-toxic, non-allergenic, non-carcinogenic and must
be able to be sterilised without imparting any change in their physical or chemical
Traditionally, natural ﬁbres such as cotton, silk and later viscose have been extensively used in all areas of medical and surgical care. One such area of application is
on the wound, where moisture and liquid that exude from the wound are absorbed
by the ﬁbrous structure to promote healing in relatively dry conditions. However,
upon healing, small ﬁbrous elements protruding from the wound dressing are
usually trapped in the pores of the newly formed tissues which make their removal
distressing to the patients.
Research work44 in the early 1960s showed that wounds under ‘moist conditions’
would in fact heal better and faster, which would also remove the problem of ﬁbres
being trapped in the healing wound. The concept of moist healing has since been
responsible for the development of many ﬁbres which have vastly improved wound
management techniques and patient care. Alginate ﬁbres45 are one such example
where naturally occurring, high molecular weight carbohydrates or polysaccharides
obtained from seaweeds have found use in the medical textiles. Chemically, alginate
is a copolymer made from a-l-guluronic acid and b-d-mannuronic acid. It is made
into ﬁbres by extruding sodium alginate into a calcium chloride bath where calcium
alginate ﬁlaments precipitate.The ﬁlaments are then drawn, washed and dried. Upon
contact with wound ﬂuid, these ﬁbres are partially converted to a water-soluble
sodium alginate that swells to form a gel around the wound, thus keeping the wound
moist during the healing period.They can then be easily removed once the treatment
is complete. Artiﬁcial polymers based on a crosslinking copolymer of acrylic acid
have been developed which are claimed16 to have superior absorption properties to
alginates particularly when used under pressure. Hydrocel, a derivative of Acordis’s
environmentally friendly Lyocell, is also claimed to be more absorbent than calcium
alginate, taking up to 35 times its own weight of water whilst remaining intact.
Handbook of technical textiles
Chitin46,47 is another polysaccharide which, after cellulose, is the most abundantly
available natural polymer. It is found in the outer shells of shrimps and crabs in
combination with protein and minerals. Medicinal and medical use of this polymer
has been realised seriously since the early 1970s. High purity chitin, from which
protein, heavy metals and pyrogens have been removed, can be used for a range of
applications from food additives for controlling cholesterol levels in blood to artiﬁcial skins into which tissues can safely grow. A derivative of chitin, chitosan has
better processability and is now extensively available in ﬁbre form. The particular
appeal of both chitin and chitosan within biomedical applications is due to their
natural and biodegradable
compatible with most living systems
versatile in their physical form, i.e. powder, aqueous solutions, ﬁlms, shaped
objects, ﬁbres and sponges, and
vehicles for transporting and delivering drugs.
Finally, collagen, a protein-based polymer that is collected from bovine skin and
has traditionally been used in hydrogel or gelatine form for making jellies and
sausage casings, is now available in ﬁbre form. It is very strong and completely
Besides wound care, ﬁbre-based structures in synthetic or natural form are used
in extracorporeal devices that may be used to purify blood in kidneys, create artiﬁcial livers and function as mechanical lungs,47 as well as ﬁnding use in suture materials, artiﬁcial ligaments and cartilages and cardiovascular implants. In general,
healthcare and hygiene products, have applications that cover a wide spectrum from
disposable items to surgeons uniforms and hospital bedding and all are becoming
increasingly important across the world as the need to produce efﬁcient and effective medical care increases.
Protection and defence
In textile terms, protection and defence can be a passive response in which the textile
product receives and absorbs the impending impact or energy in order to protect the
underlying structure. Ballistic garments are obvious examples, where the assembled
ﬁbrous material is deliberately designed to slow down and reduce the penetration
of an incoming projectile. But they may also have a more active role, where the
ﬁbres show positive response by generating char or protective gases, shrinking or
expanding to prevent penetration of moisture or vapour and so on. In each scenario,
the protection of the underlying structure is the common objective.
In the early days, leather and metal mesh garments were used to protect the body
against sword and spear attacks, but with the passage of time development of new
materials occurred and, for example, early in the 1940s, nylon-based ﬂack jackets48
were introduced. They were a considerable improvement on the leather and metal
garments but were still rather heavy and uncomfortable to wear. With the advent
of para-aramids in the early 1970s, advanced ﬁbres were for the ﬁrst time used to
make much more acceptable protective gear. In these garments, Kevlar or Twaron
continuous ﬁlament yarns are woven into tight structures and assembled in a multilayer form to provide maximum protection. Their high tenacity and good energy
52. Technical ﬁbres
absorption combined with high thermal stability enables these garments to receive
and neutralise a range of projectiles from low calibre handguns, that is 0.22 to 0.44
inch (5.6–11.2 mm) to military bullets within the 5.56–7.62 mm range.49 In the latter
case, the fabric will require facing with ceramic tiles or other hard materials to blunt
the tips of metal-jacket spitzer-pointed bullets.
To strike a better balance between garment weight, comfort and protection an
even stronger and lighter ﬁbre based on ultra-high molecular weight polyethylene
(see Section 2.3) was developed and used in the early 1990s, which immediately
reduced average garment weight by 15%.50,51 UHMWPE, commercially known as
Dyneema (DSM) and in composite form as Spectra Shield by Allied Signal, is
now used to make cut-resistant gloves and helmets, as well as a wide range of
protective garments. However, unlike Kevlar, with a fairly low melting temperature
of 150 °C, it is best suited to low temperature applications.
Fire is another means by which fatal and non-fatal injuries can be sustained. No
textile-based material can withstand the power and ferocity of a ﬁre for sustained
periods of greater than 10 min or so. However, if the ﬁre ignition point could be
increased or the organic structure converted to a carbonaceous char replica and
its spreading rate delayed, then there may just be enough time gained to save an
otherwise lost life. This is in essence the nature and objective of all ﬁre-retardant
compounds. Such treatments give ﬁbres the positive role of forming char, reducing
the emission of combustible volatile gases and effectively starving the ﬁre of oxygen
or providing a barrier to underlying surfaces.
In contrast, water-repellent fabrics may shed water by preventing water droplets
from physically passing through them owing to their ﬁne ﬁbre dimensions and tight
weaves, as is the case with ventile fabrics52 or perforated barrier inlays such as
Goretex,53 whose tiny holes allow water vapour to pass through them but not water
droplets. Wax and chemically treated fabrics reduce water/fabric surface tension
by allowing water to roll off but do not allow permeation of moisture and air, so
It is not possible to categorise fully all disciplines within which textile-based materials are increasingly being applied. The spectrum of ﬁbre utilisation has already
grown to include anything from conventional ropes and industrial belts to sophisticated two- and three-dimensional composite structures. The industries they cover,
other than those already discussed, include wet/dry ﬁltration, sports and leisure gear,
inland water and marine applications, food processing, puriﬁers, electronic kit, clean
room suits and many more. It will not be long before each area develops into its
own major category.
Conventional ﬁbres dominate the technical ﬁbre market and are likely to do so for
a long time to come. The rate of growth in consumption of ﬁbres destined for technical applications, however, is now faster than those going to the traditional clothing and furnishing sectors. It was estimated that the world’s technical ﬁbres share
Handbook of technical textiles
of the market would have reached the 40% mark by the year 2000.1 Much of this
growth will depend on greater realisation of the technological and ﬁnancial beneﬁts that ﬁbre-based structures could bring to the traditional and as yet unyielding
sectors of engineering. Issues such as environment, recycling and biodegradability,
which are increasingly subjects of concern for the public, will further encourage and
beneﬁt the growth and use of technical textiles.
1. t nobolt, Keeping a competitive edge in technical textiles, Textile Month, Union des Industries,
February p16, 1992.
2. m c tubbs (ed.), Textile Terms and Deﬁnitions, 9th edition, The Textile Institute, Manchester, 1991.
3. c byrne, ‘Technical textiles’, Textiles Mag., issue 2.95, pp. 12–16, 1995.
4. j e mcintyre, Speciality Fibres for Technical Textiles, Department of Textile Industries, University of
5. a r horrocks, The Durability of Geotextiles, Comet Eurotex, UK 1992.
6. p r rankilor, Membranes in Ground Engineering, Wiley Interscience, London, 1981.
7. v van zanten, Geotextiles and Geomembranes in Civil Engineering, Balkema, Rotterdam, 1986.
8. p w harrison (ed.), Cotton in a Competitive World, The Textile Institute, 1979.
9. b k kandola and a r horrocks, ‘Complex char formation in ﬂame-retarded ﬁbre-intumescent combinations-II. Thermal analytical studies’, Polymer Degradation and Stability, 54, 289–303, 1996.
10. a r horrocks, ‘Flame-retardant ﬁnishing of textiles’, Rev. Prog. Coloration, 16, 62–101, 1986.
11. l benisek and w a phillips, Textile Res. J., 51, 1981.
12. d j cole, ‘A new cellulosic ﬁbre – Tencel’, Advances in Fibre Science, The Textile Institute, 1992.
13. c m legault, ‘Antron – a special nylon carpet ﬁbre’, Can. Textile J., April, 1982.
14. c b chapman, Fibres, Butterworths, 1974.
15. c z porczynski, Manual of Man-made Fibres, Astex, 1960.
16. p akers and r heath, Superabsorbent Fibres, The Key to the Next Generation of Medical Products,
Technical Absorbents Ltd., UK, 1996.
17. d h morton-jones, Polymer Processing, Chapman and Hall, London, 1989.
18. j w s hearle, ‘Understanding and control of ﬁbre structure, parts 1 to 3’, Textile Horizon, 1997.
19. f happey, Appl. Fibre Sci., 3.
20. a sharples, Introduction to Polymer Crystallisation, Arnold, 1966.
21. d s varma, ‘High performance organic ﬁbres for industrial applications’, Man-made Textiles in India,
380–386, August, 1986.
22. l miles (ed.), ‘Flame-resistant fabrics – Some like it hot’, Textile Month, 37–41, April, 1996.
23. p heidel, a g hoechst, Frankfurt, Germany, ‘New opportunities with aromatics’, Textile Month, 43–44,
24. l baker, ‘Polyphenylene sulphide ﬁbres for high temperature ﬁltration’, Tech. Textiles Int., 11–16,
25. e mcintyre, ‘High-performance ﬁbres for industrial textiles’, Textile Horizon, 43– 45, October,
26. f o anderegg, ‘Strength of glass ﬁbres’, Ind. Eng. Cem., 31, 290–298, 1939.
27. l michaels and s s chissick (eds.), Asbestos Properties, Applications and Hazards, Vol. 1, Wiley, New
28. i n ermolenko et al, Chemically Modiﬁed Fibres, VCH, 1990.
29. t f cooke, ‘Inorganic ﬁbres, A literature review’, J. Am. Ceramics Soc., p. 2959.
30. f d birchall, ‘Oxide inorganic ﬁbres’, Concise Encyclopedia of Composite Materials, Oxford, UK,
31. a k dhingra, ‘Advances in inorganic ﬁbre development’, Contemporary Topics in Polymer Science,
New York, 1982.
32. k nosse, ‘New developments in Japanese ﬁbres’, Textile Month, 44– 46, June, 1990.
33. d and k consulting, ‘The European potential of microﬁbres’, Textile Month, 23–25, January, 1992.
34. m golding, ‘The microﬁbre business in Japan’, Tech. Textiles Int., 18–23, May, 1992.
35. t hongu and g o phillips, New Fibres, Ellis Horwood, UK, 1990.
36. a r horrocks and j a d’souza, ‘Degradation of polymers in geomembranes and geotextiles’, Handbook of Polymer Degradation, S H Hamid, M B Amin and A G Maadhah (eds), Marcel Dekker,
New York, 1992, 433–501.
37. t m allen, ‘Determination of long-term tensile strength of geosynthetics: A state of the art review’,
Geosynthetics’91 Conference, Atlanta, USA, 351–379.
54. Technical ﬁbres
38. t m allen, j r bell and t s vinson, ‘Properties of geotextiles in cold region applications’,
Transportation Research Report, Oregon State University, 1983.
39. r m koerner et al, ‘Long-term durability and aging of geotextiles,’ Geotextiles Geomembranes, 1988.
40. g r koerner et al, ‘Biological clogging in leachate collection systems’, Durability Aging Geosynthetics, 1989.
41. s k mukhopadhyay, ‘High performance ﬁbres’, Textile Prog., 25(3/4), 1993.
42. p bracke et al, Inorganic Fibres and Composite Materials, Pergamon Press, Oxford 1984.
43. a j rigby, s c anand and m miraftab, ‘Textile materials in medicine and surgery’, Textile Horizons,
December, 1993 and Knitting Int. February, 1994, vol. 101.
44. g d winter, Nature, 1962, 193, 293.
45. y qin, c agboh, x wang and d k gilding, ‘Novel polysaccharide ﬁbres for advanced wound dressing’,
Medical Textiles 96, conference proceedings, Woodhead, 15–20, 1997.
46. p a sandford and a steinnes, ‘Biomedical applications of high purity chitosan’, American Chemical
Society, chapter 28, 1991.
47. a s hoffman, ‘Medical applications of polymeric ﬁbres’, Appl Polym Symp 31, 313–334 J. Wiley and
Sons, New York, 1977.
48. a eldib and r walther, ‘Advanced ﬁbres for personal protective clothing’, Tech. Textiles Int., June,
49. s a young, ‘The use of Kevlar para-aramid ﬁbre in ballistic protection garments’, Tech. Textiles Int.,
26–27, July/August, 1992.
50. s a young, ‘Dyneema – the strongest ﬁbre in the world’, Tech. Textiles Int., May, 1992.
51. The use of Kevlar para-aramid ﬁbre in ballistic protection garments, Tech. Textiles Int., 24–27,
52. Ventile fabrics commercial publications, Courtaulds, Chorley, Lancashire.
53. w l gore and associates, Inc, ‘Porous materials derived from tetraﬂuoroethylene and processes for
their production’, US Patent no. 1355373, USA, 1974.
R H Gong and X Chen
Department of Textiles, UMIST, PO Box 88, Sackville Street, Manchester M60 1QD, UK
Technical yarns are produced for the manufacture of technical textiles. They
have to meet the speciﬁc functional requirements of the intended end-use. This
may be achieved through special yarn production techniques or through the selection of special ﬁbre blends or a combination of both. This chapter describes the
yarn production technologies that are applicable to technical yarns and discusses
the structures and properties of the yarns that may be produced using these
Staple ﬁbre yarns
3.2.1 Ring spinning
Ring spinning is currently the most widely used yarn production method. Initially
developed in America in the 1830s, its popularity has survived the emergence of
much faster spinning technologies. In addition to the superior yarn quality, ring spinning is extremely versatile. It is capable of producing yarns with wide ranges of
linear density and twist from a great variety of ﬁbre materials. It is also used for
doubling and twisting multifold and cabled yarns.
Fibre materials must be properly prepared before they can be used on the ring
spinning machine. The preparation processes are dependent on the ﬁbre material.
Figures 3.1 and 3.2 illustrate the typical process routes for cotton and wool. The ultimate objectives of the many preparation processes are to produce a feed material
for the ﬁnal spinning process that is clean, even, homogeneous and free from ﬁbre
entanglement. The ﬁbres must also be in the preferred orientation.
On the ring spinning machine, the feed material is attenuated to the required
linear density by a drafting system, typically a roller drafting system with three lines
of rollers. The drafted ﬁbre strand is then twisted by the ring spindle illustrated in
56. Technical yarns
For combed yarn
For carded yarn
Production of ring-spun cotton yarn.
Production of wool yarn.
The yarn leaving the front rollers is threaded through a yarn guide (the lappet),
which is located directly above the spindle axis. The yarn then passes under the Cshaped traveller onto the bobbin. The bobbin is mounted on the spindle and rotates
with the spindle. When the bobbin rotates, the tension of the yarn pulls the traveller
around the ring. The traveller rotational speed, the spindle rotational speed and the
yarn delivery speed follow Equation 3.1:
Nt = N s -
Handbook of technical textiles
where Nt is the traveller rotational speed (rpm), Ns is the spindle rotational
speed (rpm), Vd is the yarn delivery speed (m min-1) and Db is the bobbin diameter
During production, the bobbin rail moves up and down to spread the yarn along
the length of the bobbin so that a proper package can be built. The movement of the
ring rail is quite complicated, but the aim is to build a package that is stable, easy to
unwind and contains the maximum amount of yarn. As the yarn is wound on the
58. Technical yarns
bobbin, the bobbin diameter increases steadily during production.The spindle speed
and the yarn delivery speed are normally kept constant, it is therefore obvious from
Equation 3.1 that the traveller speed increases during production.
Each rotation of the traveller inserts one full turn in the yarn, so the twist inserted
in a unit length of yarn can be calculated by Equation 3.2:
where t is the yarn twist (turns m-1).
Because the traveller speed is not constant, the twist in the yarn also varies.
However, because this variation is usually very small, it is commonly ignored and
the twist is simply calculated from the spindle speed, Equation 3.3:
As can be seen from Equation 3.3, for a given yarn twist, the higher the spindle
speed the higher the yarn delivery speed. A spindle speed of up to 25 000 rpm is
possible, although speeds of between 15 000 and 20 000 rpm are more usually used.
The spindle speed is restricted by the traveller speed, which has an upper limit of
around 40 m s-1. When the traveller speed is too high, the friction between the traveller and the ring will generate too much heat, which accelerates the wear on the
traveller and the ring and may also cause yarn damage. The yarn between the
yarn guide and the traveller rotates with the traveller and balloons out owing to
centrifugal force. The tension in the yarn increases with the rotational speed of the
yarn balloon. When the spindle speed is too high, the high yarn tension will increase
the yarn breakage. The traveller speed and the yarn tension are the two most critical factors that restrict the productivity of the ring spinning system. The increasing
power cost incurred by rotating the yarn package at higher speeds can also limit the
economic viability of high spindle speeds. For the same traveller linear speed, using
a smaller ring allows a higher traveller rotational speed and increases delivery
speed. A smaller ring also reduces yarn tension, as the yarn balloon is also smaller.
However, a smaller ring leads to a smaller bobbin which results in more frequent
Ring-spun yarns have a regular twist structure and, because of the good ﬁbre
control during roller drafting, the ﬁbres in the yarn are well straightened and
aligned. Ring spun yarns therefore have excellent tensile properties, which are often
important for technical applications.
The ring spinning system can be used for spinning cover yarns where a core
yarn, spun or ﬁlament, is covered by staple ﬁbres. This can provide yarns with a
combination of technical properties. For example, a high strength yarn with
good comfort characteristics may be spun from a high strength ﬁlament core with
natural ﬁbre covering. Other technical yarns, such as ﬂame-retardant and antistatic
yarns can also be made by incorporating ﬂame-retardant and electricity conductive
The main limitation of the ring spinning system is the low productivity. The other
limitations are the high drafting and spinning tensions involved. These high tensions
can become a serious problem for spinning from ﬁbres such as alginate ﬁbres that
have low strength.
Handbook of technical textiles
navel and tube
Rotor spinning principle.
3.2.2 Rotor spinning
The productivity limitation of the ring spinning system was recognised long before
the commercial introduction of rotor spinning in 1967. In ring spinning, the twist
insertion rate is dependent on the rotational speed of the yarn package. This is so
because of the continuity of the ﬁbre ﬂow during spinning. Numerous attempts have
been made since before the end of the 19th century, particularly since the 1950s, to
introduce a break into the ﬁbre ﬂow so that only the yarn end needs to be rotated
to insert twist. Very high twisting speeds can thus be achieved. In addition, by
separating twisting from package winding, there will be much more ﬂexibility in the
form and size of the yarn package built on the spinning machine. This increases the
efﬁciency of both the spinning machine and of subsequent processes. Rotor spinning was the ﬁrst such new technology to become commercially successful and it is
the second most widely used yarn production method after ring spinning.
The principles of rotor spinning are illustrated in Fig. 3.4. The ﬁbre material is
fed into an opening unit by a feed roller in conjunction with a feed shoe. The feed
material is usually a drawn sliver. An opening roller is located inside the opening
unit and is covered with carding wire, usually saw-tooth type metallic wire. The
surface speed of the opening roller is in the region of 25–30 m s-1, approximately
2000 times the feed roller surface speed. This high speed-ratio enables the ﬁbres to
60. Technical yarns
be opened up into a very thin and open ﬁbre ﬂow. The ﬁbres are taken off the
opening roller by an air stream with a speed about twice that of the opening
roller. The ﬁbres are carried by the air stream, through the ﬁbre transportation tube,
into the spinning rotor. The air speed in the transportation tube increases, owing to
the narrowing cross-section of the tube, as the air reaches the exit point inside the
rotor. This ensures that the ﬁbres are kept aligned along the airﬂow direction
and as straight as possible. The exit angle of the ﬁbres from the transportation
tube is at a tangent to the rotor wall and the surface speed of the rotor is faster
than the exit air speed, so the ﬁbres emerging from the transportation tube are
pulled into the rotor, keeping the ﬁbres aligned in the direction of the ﬁbre ﬂow.
The centrifugal force generated by the rotor forces the ﬁbres into the rotor groove.
Because of the high surface speed of the rotor, only a very thin layer of ﬁbres, usually
one or two ﬁbres in the cross-section, is deposited in the rotor when the rotor passes
the ﬁbre exit point of the transportation tube. Many such layers of ﬁbres are needed
to make up the yarn. This doubling up of the ﬁbres in the rotor is called back
The tail of the yarn arm inside the rotor is thrown against the rotor groove
because of the centrifugal force. The yarn arm rotates with the rotor and each rotation of the yarn arm inserts one full turn in the yarn. As the yarn is withdrawn continuously through the navel and tube, the contact point of the yarn arm with the
rotor groove must move around the rotor. Because the yarn arm is rotating axially,
the ﬁbres in the rotor groove are twisted into the yarn. The machine twist of the
yarn can be calculated by Equation 3.4:
where t is the yarn twist (turns m-1), Ny is the rotational speed of the yarn arm (rpm)
and Vd is the yarn delivery speed (m min-1).
The following relationship exists between the yarn arm speed, the rotor speed
and the yarn delivery speed, Equation 3.5:
(N y - N r )pD = Vd
where D is the diameter of rotor groove.
The relative speed between the yarn arm and the rotor is normally very small in
comparison with the rotor speed and the machine twist of the yarn is commonly
calculated by Equation 3.6:
The back-doubling ratio b is equal to the ratio of the rotor speed to the relative
speed between the yarn arm and the rotor, Equation 3.7:
pD = tpD
Ny - Nr Vd
Because there is no need to rotate the yarn package for the insertion of twist,
rotor spinning can attain much higher twisting speeds than ring spinning. The rotor
speed can reach 150 000 rpm. The roving process needed in ring spinning is eliminated in rotor spinning, further reducing the production cost. The package can
Handbook of technical textiles
be much larger, with fewer knots in the product and with a more suitable form for
Because the yarn is formed in an enclosed space inside the rotor, trash particles
remaining in the ﬁbres can accumulate in the rotor groove. This leads to a gradual
deterioration of yarn quality and in severe cases yarn breakage. The cleanliness of
ﬁbres is more critical for rotor spinning than for ring spinning. In order to improve
the cleanliness of the ﬁbres, a trash extraction device is used at the opening roller.
As the twist in the yarn runs into the ﬁbre band in the rotor groove, inner layers
of the yarn tend to have higher levels of twist than outer layers. Fibres landing on
the rotating ﬁbre band close to the yarn tail, or directly on the rotating yarn arm
when the yarn arm passes the exit of the transportation tube, tend to wrap around
the yarn instead of being twisted into the yarn. These wrapping ﬁbres are characteristic of rotor-spun yarns.
Rotor-spun yarns usually have lower strength than corresponding ring-spun
yarns because of the poorer ﬁbre disposition in the yarn. This is the result of using
an opening roller to open up the ﬁbres, of transporting the ﬁbres by airﬂow, and
of the low yarn tension during yarn formation. The wrapping ﬁbres also lead to a
rougher yarn surface. Rotor yarns have better short term evenness than ring-spun
yarns because of the back-doubling action.
The main advantage of rotor spinning is the high production rate. However,
because of the lower yarn strength, rotor spinning is limited to medium to course
yarn linear densities. It is also limited to the spinning of short staple ﬁbre yarns.
3.2.3 Friction spinning
Friction spinning is an open end spinning technique. Instead of using a rotor, two
friction rollers are used to collect the opened-up ﬁbres and twist them into the yarn.
The principle is shown in Fig. 3.5.
The ﬁbres are fed in sliver form and opened by a carding roller. The opened ﬁbres
are blown off the carding roller by an air current and transported to the nip area
of two perforated friction drums. The ﬁbres are drawn onto the surfaces of the friction drums by air suction. The two friction drums rotate in the same direction and
because of the friction between the ﬁbre strand and the two drum surfaces, twist is
inserted into the ﬁbre strand. The yarn is withdrawn in the direction parallel to the
friction drum axis and delivered to a package forming unit. The friction drum diameter is much larger than the yarn diameter. The diameter ratio can be as high as 200.
A high twisting speed can thus be achieved by using a relatively low speed for the
friction drums. Owing to the slippage between the drum surface and the yarn end,
the yarn takes up only 15–40% of the drum rotation. Nevertheless, a high production speed, up to 300 m min-1, can be achieved. For a ﬁner yarn the twist insertion
rate is higher with the same drum speed so the delivery speed can be practically
independent of yarn linear density.
Because the yarn is withdrawn from the side of the machine, ﬁbres fed from the
machine end away from the yarn delivery tend to form the yarn core while ﬁbres
fed from the machine end closer to the yarn delivery tend to form the sheath. This
characteristic can be conveniently exploited to produce core–sheath yarn structures.
Extra core components, ﬁlaments or drafted staple ﬁbres, can be fed from the side
of the machine while the ﬁbres fed from the top of the machine, the normal input,
form the sheath.
62. Technical yarns
DREF 2 friction spinner.
Unlike ring or rotor spinning machines that are produced by many manufacturers around the world, friction spinning machines are only currently made by Dr.
Ernst Fehrer AG of Austria. The diagram shown in Fig. 3.5 is the DREF 2 machine
that has recently been upgraded to DREF 2000. The company also produces the
DREF 3 machine that has an extra drafting unit on the side of the machine for
feeding drafted staple ﬁbres as a core component.
The ﬁbre conﬁguration in friction-spun yarns is very poor. When the ﬁbres come
to the friction drum surface, they have to decelerate sharply from a high velocity to
almost stationary. This causes ﬁbre bending and disorientation. Because of the very
low tension in the yarn formation zone, ﬁbre binding in the yarn is also poor. As a
result, the yarn has a very low tensile strength and only coarse yarns, 100 tex and
above, are usually produced.
The main application of friction spinning is for the production of industrial yarns
and for spinning from recycled ﬁbres. It can be used to produce yarns from aramid
and glass ﬁbres and with various core components including wires. The yarns can
be used for tents, protective fabrics, backing material, belts, insulation and ﬁlter
3.2.4 Wrap spinning
Wrap spinning is a yarn formation process in which a twistless staple ﬁbre strand
is wrapped by a continuous binder. The process is carried out on a hollow
spindle machine as illustrated in Fig. 3.6. The hollow spindle was invented by DSO
‘Textil’ in Bulgaria. The ﬁrst wrap spinning machine was introduced in the 1979
The staple roving is drafted on a roller drafting system similar to those used on
ring frames and is passed through a rotating hollow spindle that carries a binder
bobbin. The rotation of the hollow spindle and the bobbin wraps the binder around
the staple strand.
Handbook of technical textiles
Wrap spinning principle.
To prevent the drafted staple strand falling apart before it is wrapped by the
binder, false twist is usually generated in the staple strand by the spindle. To introduce the false twist, the staple strand is not threaded through the hollow spindle
directly. It is wrapped around either a twist regulator at the bottom of the spindle
or part of the spindle top. The false twist also allows the staple strand to be compacted before the binder is wrapped around it. This improves the yarn strength.
Two hollow spindles can be arranged one above the other to wrap the staple
strand with two binders in opposite directions. This is used to produce special effect
yarns with a more stable structure. Real twist may also be added to the yarn by
passing the wrapped yarn onto a ring spindle, usually arranged directly underneath
the hollow spindle.
Core yarns, mostly ﬁlaments, can be added to the feed.This can be used to provide
extra yarn strength or other special yarn features. An example is to use this method
to spin alginate yarns. Alginate ﬁbres are very weak and cause excessive breakages
during spinning without the extra support of core ﬁlaments.
A variety of binders can be used to complement the staple core or to introduce
special yarn features. For example, a carbon-coated nylon ﬁlament yarn can be used
to produce yarns for antistatic fabrics. Soluble binders can be used for making yarns
for medical applications.
Wrap spinning is highly productive and suitable for a wide range of yarn linear
densities. Yarn delivery speeds of up to 300 m min-1 are possible. Because the binder
is normally very ﬁne, each binder bobbin can last many hours, enabling the pro-
64. Technical yarns
1st Nozzle N1
2nd Nozzle N2
Murata jet spinner.
duction of large yarn packages without piecing. Because the staple core is composed
of parallel ﬁbres with no twist, the yarn has a high bulk, good cover and very low
hairiness. The main limitation of wrap spinning is that it is only suitable for the
production of multicomponent yarns. The binder can be expensive, increasing the
3.2.5 Air-jet spinning
Air-jet spinning technology was ﬁrst introduced by Du Pont in 1963, but it has only
been made commercially successful by Murata since 1980. Du Pont used only one
jet, which produced a low strength yarn. The Murata system has two opposing air
jets, which improves the yarn strength. The twin-jet Murata Jet Spinner is illustrated
in Fig. 3.7. Staple ﬁbres are drafted using a roller drafting system with three or four
pairs of rollers. The ﬁbres are then threaded through the twin-jet assembly. The
second jet N2 has a higher twisting torque than the ﬁrst jet N1. Immediately after
leaving the front drafting rollers, the ﬁbres in the core of the yarn are twisted in the
twist direction of N2. The ﬁbres on the edges of the drafted ribbon are twisted by
the weaker N1 and wrap around the core ﬁbres in the opposite direction. Because
the jet system is located between the front drafting rollers and the yarn delivery
rollers, neither of which rotates around the axis of the yarn, the twist inserted by
the jets is not real twist and after the yarn passes through the jet system, the core
ﬁbres become twistless. The yarn strength is imparted by the wrapping of the edge
ﬁbres. Because of the small jet dimensions, very high rotational jet speeds are possible. Although twist efﬁciency is only 6–12% because of the twist resistance of the
yarn, delivery speeds of up to 300 m min-1 are possible. In a further development by
Murata the second jet is replaced with a pair of roller twisters. The principle of yarn
formation is similar to the twin-jet system. The new machine, the roller-jet spinner,
is capable of delivery speeds of up to 400 m min-1. However, the yarn has a harsher
Air-jet spinning is used mainly for spinning from short staple ﬁbres, especially
cotton and polyester blends. The vortex spinner, the latest addition to the Murata
jet spinner range, was shown in ITMA 99 for spinning from 100% cotton.
Handbook of technical textiles
The air-jet system can be used to produce core–sheath yarn structures by feeding
the core and sheath ﬁbres at different stages of the drafting system. Fibres fed in
from the back of the drafting system tend to spread wider under the roller pressure
and form the sheath of the yarn while ﬁbres fed in nearer to the front tend to form
the yarn core. Filament core can also be introduced at the front drafting roller. Two
spinning positions can be combined to produce a two-strand yarn that is then twisted
using the usual twisting machinery.
Air-jet yarns have no real twist, therefore they tend to have higher bulk than ring
and rotor yarns and better absorbency. They are more resistant to pilling and have
little untwisting tendency. Because the yarn strength is imparted by the wrapping
ﬁbres, not the twisting of the complete ﬁbre strand, air-jet yarns have lower tensile
strength than ring and rotor yarns.The system is only suitable for medium to ﬁne yarn
linear densities as the effectiveness of wrapping decreases with the yarn thickness.
The rigid yarn core of parallel ﬁbres makes the yarn stiffer than the ring and rotor
3.2.6 Twistless spinning
Numerous techniques have been developed to produce staple yarns without twisting so that the limitations imposed by twisting devices, notably the ring traveller
system, can be avoided and production speed can be increased. Because of the
unconventional yarn characteristics, these techniques have not gained widespread
acceptance commercially, but they do offer an alternative and could be exploited to
produce special products economically.
Most of these twistless methods use adhesives to hold the drafted staple ﬁbre
strand together. They can produce low linear density yarns at a high speed. The
adhesives may later be removed after the fabric is made and the ﬁbres are then
bound by the interﬁbre forces imposed by fabric constraints. This type of yarn has
high covering power due to the untwisted yarn structure. However, these processes
mostly involve additional chemicals and require high power consumption. The yarns
can only be used for fabrics that offer good interﬁbre forces.
As an example, the TNO twistless spinning method is shown in Fig. 3.8. In the
system shown here, the roving is drafted under wet conditions, which gives better
ﬁbre control. An inactive starch is then applied to the drafted roving, which is also
false twisted to give it temporary strength. The starch is activated by steaming the
package that is then dried. The later version of TNO twistless system replaces the
starch with PVA (polyvinyl alcohol) ﬁbres (5–11%), which melt at above 80 °C to
bind the staple ﬁbres. This is also known as the Twilo system.
Another twistless spinning method is the Bobtex process, which can produce
high strength yarns for industrial/leisure fabrics, such as tents, workwear and
sacks. In this process, staple ﬁbres (30–60%) are bonded to a ﬁlament core (10–50%)
by a layer of molten polymer (20–50%). Production speeds of up to 1000 m min-1
can be achieved. The process can use all types of staple ﬁbres including waste
3.2.7 Ply yarn
Single yarns are used in the majority of fabrics for normal textile and clothing
applications, but in order to obtain special yarn features, particularly high strength
66. Technical yarns
TNO twistless yarn production method.
and modulus for technical and industrial applications, ply yarns are often needed.
A folded yarn is produced by twisting two or more single yarns together in one
operation, and a cabled yarn is formed by twisting together two or more folded
yarns or a combination of folded and single yarns.
The twisting together of several single yarns increases the tenacity of the yarn by
improving the binding-in of the ﬁbres on the outer layers of the component single
yarns. This extra binding-in increases the contribution of these surface ﬁbres to the
yarn strength. Ply yarns are also more regular, smoother and more hard wearing.
By using the appropriate single yarn and folding twists, a perfectly balanced ply yarn
can be produced for applications that require high strength and low stretch, for
example, for tyre cords.
A typical process route of a ply yarn involves the following production
single yarn production
single yarn winding and clearing
assembly winding: to wind the required number of single yarns as one
(doubling) on a package suitable for folding twisting
Twisting can be carried out in a two-stage process or with a two-for-one twister. In
the two-stage process, the ring frame is used to insert a low folding twist in
the ﬁrst stage and an up-twister to insert the ﬁnal folding twist in the second
Handbook of technical textiles
stage. The ring frame uses a low twist to enable higher delivery speeds. A suitable
package is formed on the ring frame for the over-end withdrawal of yarn on the
up-twister. Figure 3.9 shows the principle of the up-twister. The supply package
rotates with the spindle while the yarn is withdrawn over the package end from
the top. The free-rotating ﬂyer is pulled around by the yarn and inserts twist in the
The two-for-one twister is illustrated in Fig. 3.10. The supply yarn package is stationery. After withdrawal from the package, the yarn is threaded through the centre
of the spindle and rotates with the spindle. Each rotation of the spindle inserts one
full turn in the yarn section inside the spindle centre and also one turn in the yarn
section outside the yarn package (the main yarn balloon). The yarn therefore gets
two turns for each spindle rotation. If the supply package is rotated in the opposite
direction of the spindle, then the twisting rate will increase by the package rotational speed. The Saurer Tritec Twister is based on this principle. In the Tritec
Twister, the package rotates at the same speed as the spindle, but in the opposite
direction, so each spindle rotation inserts three twists in the yarn. The package is
The production of a ply yarn is much more expensive than the production of
a single yarn of equivalent linear density. Not only does the ply yarn production
require the extra assembly winding and twisting processes, but the production of
the ﬁner component single yarn is also much more expensive.
68. Technical yarns
The two-for-one twister.
A ﬁlament yarn is made from one or more continuous strands called ﬁlaments where
each component ﬁlament runs the whole length of the yarn. Those yarns composed
of one ﬁlament are called monoﬁlament yarns, and those containing more ﬁlaments
are known as multiﬁlament yarns. For apparel applications, a multiﬁlament yarn may
contain as few as two or three ﬁlaments or as many as 50 ﬁlaments. In carpeting, for
example, a ﬁlament yarn could consist of hundreds of ﬁlaments. Most manufactured
ﬁbres have been produced in the form of a ﬁlament yarn. Silk is the only major
natural ﬁlament yarn.
According to the shape of the ﬁlaments in the yarn, ﬁlament yarns are classiﬁed
into two types, ﬂat and bulk. The ﬁlaments in a ﬂat yarn lie straight and neat, and
are parallel to the yarn axis. Thus, ﬂat ﬁlament yarns are usually closely packed and
have a smooth surface. The bulked yarns, in which the ﬁlaments are either crimped
or entangled with each other, have a greater volume than the ﬂat yarns of the same
Texturing is the main method used to produce the bulked ﬁlament yarns. A textured yarn is made by introducing durable crimps, coils, and loops along the length
of the ﬁlaments. As textured yarns have an increased volume, the air and vapour
permeability of fabrics made from them is greater than that from ﬂat yarns.
Handbook of technical textiles
(a) Melt spinning process, (b) drawing process.
However, for applications where low air permeability is required, such as the fabrics
for air bags, ﬂat yarns may be a better choice.
3.3.2 Manufacture of ﬁlament yarns
Most manufactured ﬁbres are extruded using either melt spinning, dry spinning, or
wet spinning, although reaction spinning, gel spinning and dispersion spinning are
used in particular situations. After extrusion, the molecular chains in the ﬁlaments
are basically unoriented and therefore provide no practical strength. The next step
is to draw the extruded ﬁlaments in order to orient the molecular chains. This is conventionally carried out by using two pairs of rollers, the second of which forwards
the ﬁlaments at approximately four times the speed of the ﬁrst. The drawn ﬁlaments
are then wound with or without twist onto a package. The tow of ﬁlaments at this
stage becomes the ﬂat ﬁlament yarn. Figure 3.11 shows the melt spinning process
and the subsequent drawing process.
For many applications, ﬂat ﬁlament yarns are textured in order to gain increased
bulkiness, porosity, softness and elasticity in some situations. Thermoplastic ﬁlament
yarns are used in most texturing processes. The interﬁbre bonds break and reform
during the texturing process. A ﬁlament yarn is generally textured through three
steps. The ﬁrst step is to distort the ﬁlament in the yarn so that the interﬁbre bond
is broken. Twisting or other means are used to distort the ﬁlaments within a yarn.
The second step is to heat the yarn, which breaks bonds between polymers, allowing the ﬁlaments to stay crimped. The last step is to cool the yarn in the distorted
state to enable new bonds to form between the polymers.When the yarn is untwisted
70. Technical yarns
Principles of main texturing methods: (a) false twist, (b) stuffer box, (c) air-jet,
or otherwise released from its distorted state, the ﬁlaments remain in a coiled or
There are many methods for yarn texturing, including false-twist, air-texturing,
knit-de-knit, stuffer box and gear crimp. Among these, the false-twist is the most popular method. Figure 3.12 shows the principles of the main methods of yarn texturing.
3.3.3 Filament technical yarns
There have been many types of ﬁlament yarns developed for technical applications,
such as reinforcing and protecting. The reinforcing technical yarns have either high
modulus, high strength, or both. Yarns for protecting applications can be resistant
to safety hazards such as heat and ﬁre, chemical and mechanical damage. There
are many types of technical ﬁlament yarns used in various applications, it is only
possible, therefore, to list just a few yarns here that are popularly used in the
development of some technical textile products.
22.214.171.124 Aramid ﬁlament yarns
Aramid ﬁbre is a chemical ﬁbre in which the ﬁbre-forming substance is a long chain
synthetic polyamide where at least 85% of the amide linkages are attached directly
Handbook of technical textiles
to two aromatic rings. Nomex and Kevlar are two well-known trade names of the
aramid ﬁbre, owned by Du Pont. Aramid ﬁbres have high tenacity and high resistance to stretch, to most chemicals and to high temperature. The Kevlar aramid is
well known for its relatively light weight and for its fatigue and damage resistance.
Because of these properties, Kevlar 29 is widely used and accepted for making body
armour. Kevlar 49, on the other hand, has high tenacity and is used as reinforcing
material for many composite uses, including materials for making boat and aircraft
parts. The Nomex aramid, on the other hand, is heat resistant and is used in making
ﬁre ﬁghters’ apparel and similar applications.
Aramid yarns are more ﬂexible than their other high performance counterparts
such as glass and Kevlar, and thus are easier to use in subsequent fabric making
processes, be it weaving, knitting, or braiding. Care should be taken, though, as
aramid yarns are much stronger and much more extensible than the conventional
textile yarns, which could make the fabric formation process more difﬁcult.
126.96.36.199 Glass ﬁlament yarns
Glass is an incombustible textile ﬁbre and has high tenacity too. It has been used
for ﬁre-retardant applications and also is commonly used in insulation of buildings.
Because of its properties and low cost, glass ﬁbre is widely used in the manufacture
of reinforcement for composites. There are different types of glass ﬁbres, such as Eglass, C-glass, and S-glass. E-glass has very high resistance to attack by moisture and
has high electrical and heat resistance. It is commonly used in glass-reinforced plastics in the form of woven fabrics. C-glass is known for its chemical resistance to both
acids and alkalis. It is widely used for applications where such resistance is required,
such as in chemical ﬁltration. The S-glass is a high strength glass ﬁbre and is used
in composite manufacturing.
Glass ﬁlament yarns are brittle compared with the conventional textile yarns. It
has been shown that the speciﬁc ﬂexural rigidity of glass ﬁbre is 0.89 mN mm2 tex-2,
about 4.5 times more rigid than wool. As a result, glass yarns are easy to break in
textile processing. Therefore, it is important to apply suitable size to the glass yarn
to minimise the interﬁbre friction and to hold the individual ﬁbres together in
the strand. Dextrinised starch gum, gelatine, polyvinyl alcohol, hydrogenerated
vegetable oils and non-ionic detergents are commonly used sizes.
When handling glass ﬁbres, protective clothing and a mask should be worn to
prevent skin irritation and inhalation of glass ﬁbres.
188.8.131.52 Carbon ﬁlament yarns
Carbon ﬁbres are commonly made from precursor ﬁbres such as rayon and acrylic.
When converting acrylic ﬁbre to carbon, a three-stage heating process is used. The
initial stage is oxidative stabilisation, which heats the acrylic ﬁbre at 200–300 °C
under oxidising conditions. This is followed by the carbonisation stage, when the
oxidised ﬁbre is heated in an inert atmosphere to temperatures around 1000 °C.
Consequently, hydrogen and nitrogen atoms are expelled from the oxidised ﬁbre,
leaving the carbon atoms in the form of hexagonal rings that are arranged in
oriented ﬁbrils. The ﬁnal stage of the process is graphitisation, when the carbonised
ﬁlaments are heated to a temperature up to 3000 °C, again in an inert atmosphere. Graphitisation increases the orderly arrangement of the carbon atoms, which
72. Technical yarns
are organised into a crystalline structure of layers. These layers are well oriented in
the direction of ﬁbre axis, which is an important factor in producing high modulus
Like the glass yarns, most carbon ﬁbres are brittle. Sizes are used to adhere the
ﬁlaments together to improve the processability. In addition to protecting operatives against skin irritation and short ﬁbre inhalation, protecting the processing
machinery and auxiliary electric and electronic devices needs to be considered too,
as carbon ﬁbre is conductive.
184.108.40.206 HDPE ﬁlament yarns
HDPE refers to high density polyethylene. Although the basic theory for making
super strong polyethylene ﬁbres was available in the 1930s, commercial high
performance polyethylene ﬁbre was not manufactured until recently. Spectra,
Dyneema, and Tekmilon are among the most well-known HDPE ﬁbres. The gel
spinning process is used to produce the HDPE ﬁbre. Polyethylene with an extra
high molecular weight is used as the starting material. In the gel spinning process,
the molecules are dissolved in a solvent and spun through a spinneret. In solution,
the molecules which form clusters in the solid state become disentangled and
remain in this state after the solution is cooled to give ﬁlaments.The drawing process
after spinning results in a very high level of macromolecular orientation in the
ﬁlaments, leading to a ﬁbre with very high tenacity and modulus. Dyneema, for
example, is characterised by a parallel orientation of greater than 95% and a high
level of crystallinity of up to 85%. This gives unique properties to the HDPE ﬁbres.
The most attractive properties of this type of ﬁbre are: (1) very high tenacity, (2)
very high speciﬁc modulus, (3) low elongation and (4) low ﬁbre density, that is lighter
HDPE ﬁbres are made into different grades for different applications. Dyneema,
for example, is made into SK60, SK65 and SK66. Dyneema SK60 is the multipurpose grade. It is used, for example, for ropes and cordage, for protective clothing and for reinforcement of impact-resistant composites. Dyneema SK65 has a
higher tenacity and modulus than SK60. This ﬁbre is used where high performance
is needed and maximum weight savings are to be attained. Dyneema SK66 is specially designed for ballistic protection. This ﬁbre provides the highest energy absorption at ultrasonic speeds.
Table 3.1 compares the properties of the above mentioned ﬁlament yarns to steel.
220.127.116.11 Other technical yarns
There have been many other high performance ﬁbres developed for technical applications, among which are PTFE, PBI, and PBO ﬁbres.
PTFE (polytetraﬂuoroethylene) ﬁbres offer a unique blend of chemical and temperature resistance, coupled with a low fraction coefﬁcient. Since PTFE is virtually
chemically inert, it can withstand exposure to extremely harsh temperature and
chemical environments. The friction coefﬁcient, claimed to be the lowest of all ﬁbres,
makes it suitable for applications such as heavy-duty bearings where low relative
speeds are involved.
PBI (polybenzimidazole) is a manufactured ﬁbre in which the ﬁbre-forming
substance is a long chain aromatic polymer. It has excellent thermal resistance and
a good hand, coupled with a very high moisture regain. Because of these, the PBI
Handbook of technical textiles
Comparison of ﬁlament yarn properties
Aramid – regular
Aramid – composite
Aramid – ballistic
High performance ﬁbres
Density (g cm-3)
Tenacity (mN tex-1)
ﬁbre is ideal for use in heat-resistant apparel for ﬁre ﬁghters, fuel handlers, welders,
astronauts, and racing car drivers.
PBO (polyphenylenebenzobisoxazole) is another new entrant in the high performance organic ﬁbres market. Zylon, made by Toyobo, is the only PBO ﬁbre
in production. PBO ﬁbre has outstanding thermal properties and almost twice the
strength of conventional para-aramid ﬁbres. Its high modulus makes it an excellent
material for composite reinforcement. Its low LOI gives PBO more than twice the
ﬂame-retardant properties of meta-aramid ﬁbres. It can also be used for ballistic
vests and helmets.
Table 3.2 lists some properties of these ﬁbres.
a brearley and j iredale, The Worsted Industry, 2nd edition, WIRA, Leeds, 1980.
j g cook, Handbook of Textile Fibres, Manmade Fibres, 5th edition, Merrow, 1984.
Dyneema – the Top in High Performance Fibres, Properties and Applications, DSM High Performance
Fibres B.V., Eisterweg 3, 6422 PN Heerlen, Netherlands.
e t grifﬁths, ‘Wrap Spun Plain and Fancy Yarns’, Tomorrow’s Yarns, Conference Proceedings, UMIST,
s j kadolph and a l langford, Textiles, 8th edition, Prentice-Hall, 1998.
h kato, ‘Development of MJS Yarns’, J. Text. Machinery Soc. Jpn, 32(4) 1986.
w klein, New Spinning Systems, The Textile Institute, Manchester, 1993.
w klein, Man-made Fibres and Their Processing, The Textile Institute, Manchester, 1994.
w klein, The Technology of Short Staple Spinning, 2nd edition, The Textile Institute, Manchester, 1998.
w e morton and g r wray, An Introduction to the Study of Spinning, 3rd edition, Longmans, London,
74. Technical yarns
w e morton and j w s hearle, Physical Properties of Textile Fibres, 3rd edition, Textile Institute, Heinemann, London, 1993.
e oxtoby, Spun Yarn Technology, Butterworth, London, 1987.
h j selling, Twistless Yarns, Merrow, 1971.
w c smith, High Performance Fibres Protect, Improve Lives, http://www.textileworld.com/
Textile Terms and Deﬁnitions, 10th edition, Textile Institute, Manchester, 1995.
Technical fabric structures – 1. Woven fabrics
Walter S Sondhelm
10 Bowlacre Road, Hyde, Cheshire SK14 5ES, UK
Technical textiles1 are textile materials and products manufactured primarily for
their technical performance and functional properties rather than their aesthetic or
decorative characteristics. Most technical textiles consist of a manufactured assembly of ﬁbres, yarns and/or strips of material which have a substantial surface area in
relation to their thickness and have sufﬁcient cohesion to give the assembly useful
Textile fabrics are most commonly woven but may also be produced by knitting,
felting, lace making, net making, nonwoven processes and tufting or a combination
of these processes. Most fabrics are two-dimensional but an increasing number
of three-dimensional woven technical textile structures are being developed and
Woven fabrics generally consist of two sets of yarns that are interlaced and lie at
right angles to each other. The threads that run along the length of the fabric are
known as warp ends whilst the threads that run from selvedge to selvedge, that is
from one side to the other side of the fabric, are weft picks. Frequently they are
simply referred to as ends and picks. In triaxial and in three-dimensional fabrics
yarns are arranged differently.
Woven technical textiles are designed to meet the requirements of their end use.
Their strength, thickness, extensibility, porosity and durability can be varied and
depend on the weave used, the thread spacing, that is the number of threads per
centimetre, and the raw materials, structure (ﬁlament or staple), linear density (or
count) and twist factors of the warp and weft yarns. From woven fabrics higher
strengths and greater stability can be obtained than from any other fabric structure
using interlaced yarns. Structures can also be varied to produce fabrics with widely
different properties in the warp and weft directions.
76. Technical fabric structures – 1. Woven fabrics
The number of weave structures that can be produced is practically unlimited. In
this section basic structures, from which all other weave structures are developed,
are discussed. Also brieﬂy referred to are lenos, because of their importance in
selvedge constructions, and triaxial fabrics, because they show simple structural
changes which can affect the physical properties of fabrics. Most two-dimensional
woven technical fabrics are constructed from simple weaves and of these at least
90% use plain weave. Simple cloth constructions are discussed in greater detail by
Robinson and Marks2 whilst Watson3,4 describes a large variety of simple and complicated structures in great detail.
18.104.22.168 Construction of a plain weave
Plain weave is the simplest interlacing pattern which can be produced. It is formed
by alternatively lifting and lowering one warp thread across one weft thread. Figure
4.1 shows 16 repeats (four in the warp and four in the weft direction) of a plain
Fabric woven with plain weave – plan view (4 ¥ 4 repeats) and warp and
Handbook of technical textiles
weave fabric in plan view and warp way and weft way cross-sections through the
same fabric. The diagrams are idealized because yarns are seldom perfectly regular
and the pressure between the ends and picks tends to distort the shape of the yarn
cross-sections unless the fabrics are woven from monoﬁlament yarns or strips of
ﬁlm. The yarns also do not lie straight in the fabric because the warp and weft have
to bend round each other when they are interlaced. The wave form assumed by the
yarn is called crimp and is referred to in greater detail in Section 4.4.3.
22.214.171.124 Constructing a point paper diagram
To illustrate a weave either in plan view and/or in cross-section, as in Fig. 4.1, takes
a lot of time, especially for more complicated weaves.A type of shorthand for depicting weave structures has therefore been evolved and the paper used for producing
designs is referred to as squared paper, design paper or point paper. Generally
the spaces between two vertical lines represent one warp end and the spaces
between two horizontal lines one pick. If a square is ﬁlled in it represents an end
passing over a pick whilst a blank square represents a pick passing over an end. If
ends and picks have to be numbered to make it easier to describe the weave, ends
are counted from left to right and picks from the bottom of the point paper design
to the top. The point paper design shown in Fig. 4.2(a) is the design for a plain weave
fabric. To get a better impression of how a number of repeats would look, four
repeats of a design (two vertically and two horizontally) are sometimes shown.
When four repeats are shown the ﬁrst repeat is drawn in the standard way but for
the remaining three repeats crossing diagonal lines may be placed into the squares,
which in the ﬁrsts repeat, are ﬁlled in. This method is shown for a plain weave in
126.96.36.199 Diversity of plain weave fabrics
The characteristics of the cloths woven will depend on the type of ﬁbre used for
producing the yarn and whether it is a monoﬁlament yarn, a ﬂat, twisted or textured
(multi-)ﬁlament yarn or whether it has been spun from natural or manufactured
staple ﬁbres. The stiffness of the fabrics and its weavability will also be affected by
the stiffness of the raw materials used and by the twist factor of the yarn, that is the
number of turns inserted in relation to its linear density. Very highly twisted yarns
are sometimes used to produce special features in plain weave yarns. The resulting
fabrics may have high extensibility or can be semiopaque.
Point paper diagram of a plain weave fabric. (a) One repeat, (b) four repeats.
78. Technical fabric structures – 1. Woven fabrics
The area density of the fabric can be varied by changing the linear density or
count of the yarns used and by altering the thread spacing, which affects the area
covered by the yarns in relation to the total area. The relation between the thread
spacing and the yarn linear density is called the cover factor and is discussed in
Section 4.4. Changing the area density and/or the cover factors may affect the
strength, thickness, stiffness, stability, porosity, ﬁltering quality and abrasion resistance of fabrics.
Square sett plain fabrics, that is fabrics with roughly the same number of ends
and picks per unit area and warp and weft yarns of the same linear densities are
produced in the whole range of cloth area densities and cloth cover factors. Low
area density fabrics of open construction include bandages and cheese cloths, light
area density high cover factor fabrics include typewriter ribbons and medical ﬁlter
fabrics, heavy open cloths include geotextile stabilization fabrics and heavy closely
woven fabrics include cotton awnings.
Warp-faced plain fabrics generally have a much higher warp cover factor than
weft cover factor. If warp and weft yarns of similar linear density are used, a typical
warp faced plain may have twice as many warp ends as picks. In such fabrics the
warp crimp will be high and the weft crimp extremely low. The plan view and crosssections of such a fabric are shown in Fig. 4.3. By the use of suitable cover factors
and choice of yarns most of the abrasion on such a fabric can be concentrated on
the warp yarns and the weft will be protected.
Weft-faced plains are produced by using much higher weft cover factors than
warp cover factors and will have higher weft than warp crimp. Because of the difference in weaving tension the crimp difference will be slightly lower than in warpfaced plain fabrics. Weft-faced plains are little used because they are more difﬁcult
and expensive to weave.
Plan view and cross-sections of warp-faced plain weave fabric with a substantially
higher warp than weft cover factor.
Handbook of technical textiles
4.2.2 Rib fabrics and matt weave fabrics
These are the simplest modiﬁcations of plain weave fabrics. They are produced by
lifting two or more adjoining warp threads and/or two or more adjoining picks at
the same time. It results in larger warp and/or weft covered surface areas than in a
plain weave fabric. As there are fewer yarn intersections it is possible to insert more
threads into a given space, that is to obtain a higher cover factor, without jamming
188.8.131.52 Rib fabrics
In warp rib fabrics there are generally more ends than picks per unit length with a
high warp crimp and a low weft crimp and vice versa for weft rib fabrics. The simplest rib fabrics are the 2/2 warp rib and the 2/2 weft rib shown respectively in Fig.
4.4(a) and (b). In the 2/2 warp rib one warp end passes over two picks whilst in the
2/2 weft rib one pick passes over two adjoining ends. The length of the ﬂoats can be
extended to create 4/4, 6/6, 3/1 or any similar combination in either the warp or weft
direction. 3/1 and 4/4 warp ribs are shown in Fig. 4.4(c) and (d).
In rib weaves with long ﬂoats it is often difﬁcult to prevent adjoining yarns from
overlapping. Weft ribs also tend to be expensive to weave because of their relatively
high picks per unit length which reduces the production of the weaving machine
unless two picks can be inserted at the same time.
184.108.40.206 Matt fabrics (or hopsack)
Simple matt (or hopsack) fabrics have a similar appearance to plain weave. The simplest of the matt weaves is a 2/2 matt shown in Fig. 4.5(a), where two warp ends are
lifted over two picks, in other words it is like a plain weave fabric with two ends and
two picks weaving in parallel. The number of threads lifting alike can be increased
to obtain 3/3 or 4/4 matt structures. Special matt weaves, like a 4/2 matt, shown in
Fig. 4.5(b), are produced to obtain special technical effects. Larger matt structures
give the appearance of squares but are little used because they tend to become
unstable, with long ﬂoats and threads in either direction riding over each other. If
large matt weaves are wanted to obtain a special effect or appearance they can be
stabilized by using fancy matt weaves containing a binding or stitching lift securing
a proportion of the ﬂoats.
Matt weave fabrics can be woven with higher cover factors and have fewer
intersections. In close constructions they may have better abrasion and better ﬁltration properties and greater resistance to water penetration. In more open constructions matt fabrics have a greater tear resistance and bursting strength. Weaving costs
may also be reduced if two or more picks can be inserted at the same time.
4.2.3 Twill fabrics
A twill is a weave that repeats on three or more ends and picks and produces diagonal lines on the face of a fabric. Such lines generally run from selvedge to selvedge.
The direction of the diagonal lines on the surface of the cloth are generally described
as a fabric is viewed along the warp direction. When the diagonal lines are running
upwards to the right they are ‘Z twill’ or ‘twill right’ and when they run in the opposite direction they are ‘S twill’ or ‘twill left’. Their angle and deﬁnition can be varied
Handbook of technical textiles
Matt fabrics. (a) 2/2 Matt, (b) 4/2 matt.
by changing the thread spacing and/or the linear density of the warp and weft yarns.
For any construction twills will have longer ﬂoats, fewer intersections and a more
open construction than a plain weave fabric with the same cloth particulars.
Industrial uses of twill fabrics are mainly restricted to simple twills and only
simple twills are discussed here. Broken twills, waved twills, herringbone twills and
elongated twills are extensively used for suiting and dress fabrics. For details of such
twills see Robinson and Marks2 or Watson.3,4
The smallest repeat of a twill weave consists of 3 ends ¥ 3 picks. There is no theoretical upper limit to the size of twill weaves but the need to produce stable fabrics
with ﬂoats of reasonable length imposes practical limits.
The twill is produced by commencing the lift sequence of adjacent ends on
one pick higher or one pick lower. The lift is the number of picks which an end
passes over and under. In a 2/1 twill, an end will pass over two picks and under one,
whilst in a 1/2 twill the end will pass over one pick and then under two picks. Either
weave can be produced as a Z or S twill. There are, therefore, four combinations of
this simplest of all twills and they are illustrated in Fig. 4.6(a) to (d). To show
how pronounced the twill line is even in a 3 ¥ 3 twill, four repeats (2 ¥ 2) of
Fig. 4.6(a) are shown in Fig. 4.6(e) with all lifted ends shown in solid on the point
paper. 2/1 twills are warp faced twills, that is fabrics where most of the warp yarn
is on the surface, whilst 1/2 twills have a weft face. Weft-faced twills impose less
strain on the weaving machine than warp-faced twills because fewer ends have to
be lifted to allow picks to pass under them. For this reason, warp-faced twills are
sometimes woven upside down, that is as weft-faced twills. The disadvantage of
weaving twills upside down is that it is more difﬁcult to inspect the warp yarns
Twills repeating on 4 ends ¥ 4 picks may be of 3/1, 2/2 or 1/3 construction and
may have ‘Z’ or ‘S’ directions of twill. Weaves showing 4 ¥ 4 twills with a Z twill
line are shown in Fig. 4.7(a) to (c). As the size of the twill repeat is increased further,
the number of possible variations also increases. In the case of a 5 ¥ 5 the possible
combinations are 4/1, 3/2, 2/3 and 1/4 and each of these can be woven with the twill
82. Technical fabric structures – 1. Woven fabrics
4.6 3 ¥ 3 Twill weaves. (a) 2/1 Twill with Z twill line, (b) 2/1 twill with S twill line, (c) 1/2
twill with Z twill line, (d) 1/2 twill with S twill line, (e) four repeats of (a) (2/1 twill with
a Z twist line).
4 ¥ 4 Twill weaves. (a) 3/1 Twill with Z twill line, (b) 2/2 twill with Z twill line,
(c) 1/3 twill with Z twill line.
Handbook of technical textiles
5 ¥ 5 Twill weaves. (a) 4/1 Twill with Z twill line, (b) 1/4 twill with Z twill line.
line in either direction. In Fig. 4.8(a) and (b) 4/1 and 1/4 twills with a Z twill line
4.2.4 Satins and sateens
In Britain a satin is a warp-faced weave in which the binding places are arranged
to produce a smooth fabric surface free from twill lines. Satins normally have a much
greater number of ends than picks per centimetre. To avoid confusion a satin is
frequently described as a ‘warp satin’. A sateen, frequently referred to as a ‘weft
sateen’, is a weft-faced weave similar to a satin with binding places arranged to
produce a smooth fabric free of twill lines. Sateens are generally woven with a much
higher number of picks than ends. Satins tend to be more popular than sateens
because it is cheaper to weave a cloth with a lower number of picks than ends.
Warp satins may be woven upside down, that is as a sateen but with a satin
construction, to reduce the tension on the harness mechanism that has to lift the
To avoid twill lines, satins and sateens have to be constructed in a systematic
manner. To construct a regular satin or sateen weave (for irregular or special ones
see Robinson and Marks2 or Watson3) without a twill effect a number of rules have
to be observed. The distribution of interlacing must be as random as possible and
there has only to be one interlacing of each warp and weft thread per repeat, that
is per weave number. The intersections must be arranged in an orderly manner, uniformly separated from each other and never adjacent. The weaves are developed
from a 1/¥ twill and the twill intersections are displaced by a ﬁxed number of steps.
The steps that must be avoided are:
(i) one or one less than the repeat (because this is a twill),
(ii) the same number as the repeat or having a common factor with the repeat
(because some of the yarns would fail to interlace).
The smallest weave number for either weave is 5 and regular satins or sateens also
cannot be constructed with weave numbers of 6, 9, 11, 13, 14 or 15. The most popular
weave numbers are 5 and 8 and weave numbers above 16 are impracticable because
of the length of ﬂoats. Weave numbers of 2 or 3 are possible for ﬁve-end weaves
and 3 or 5 for 8-end weaves.
84. Technical fabric structures – 1. Woven fabrics
5-End weft sateen. (a) 5-end and two step sateen, (b) 5-end three step sateen.
5-End warp satin. (a) 5-end two step satin, (b) 5-end three step satin.
Figure 4.9(a) and (b) shows 5-end weft sateens with two and three steps, respectively. They have been developed from the 1/4 twill shown in Fig. 4.8(b). Mirror
images of these two weaves can be produced. Five-end warp satins with two
and three steps are shown in Fig. 4.10(a) and (b). It is the cloth particulars, rather
than the weave pattern, which generally decides on which fabric is commercially
described as a sateen or a satin woven upside down. Five-end satins and sateens are
most frequently used because with moderate cover factors they give ﬁrm fabrics.
Figure 4.11(a) and (b) shows 8-end weft sateens with three and ﬁve step repeats and
Fig. 4.12 shows an 8-end warp satin with a 5 step repeat.
Satins and sateens are widely used in uniforms, industrial and protective clothing. They are also used for special fabrics such as downproofs.
In North America a satin is a smooth, generally lustrous, fabric with a thick close
texture made in silk or other ﬁbres in a satin weave for a warp-face fabric or sateen
weave for a ﬁlling (weft) face effect. A sateen is a strong lustrous cotton fabric generally made with a ﬁve-harness satin weave in either warp or ﬁlling-face effect.
In lenos adjoining warp ends do not remain parallel when they are interlaced with
the weft but are crossed over each other. In the simplest leno one standard end and
Handbook of technical textiles
8-End weft sateen. (a) 8-end three step sateen, (b) 8-end ﬁve step sateen.
8-End ﬁve step warp satin.
one crossing end are passed across each other during consecutive picks. Two variations of this structure are shown in plan view and cross-section in Fig. 4.13(a) and
(b).4 Whenever the warp threads cross over each other, with the weft passing
between them, they lock the weft into position and prevent weft movement. Leno
weaves are therefore used in very open structures, such as gauzes, to prevent thread
movement and fabric distortion. When the selvedge construction of a fabric does
not bind its edge threads into position, leno ends are used to prevent the warp
threads at each side of a length of cloth from slipping out of the body of the
fabric. They are also used in the body of fabrics when empty dents are left in weaving because the fabrics are to be slit into narrower widths at a later stage of
Leno and gauze fabrics may consist of standard and crossing ends only or pairs
or multiples of such threads may be introduced according to pattern to obtain the
required design. For larger effects standard and crossing ends may also be in pairs
or groups of three. Two or more weft threads may be introduced into one shed and
86. Technical fabric structures – 1. Woven fabrics
4.13 (a) Leno with standard and crossing ends of same length (woven from one beam),
(b) leno with standard and crossing ends of different length (woven from two beams).
areas of plain fabric may be woven in the weft direction between picks where warp
ends are crossed over to give the leno effect. Gauze fabrics used for ﬁltration generally use simple leno weaves.
Standard and crossing ends frequently come from separate warp beams. If both
the standard and crossing ends are warped on to one beam the same length of
warp is available for both and they will have to do the same amount of bending,
that is they will have the same crimp. Such a leno fabric is shown in plan view
and cross-section in Fig. 4.13(a). If the two series of ends are brought from
separate beams the standard ends and the crossing ends can be tensioned differently and their crimp can be adjusted separately. In such a case it is possible for
the standard ends to lie straight and the crossing ends to do all the bending. Such
a fabric is shown in Fig. 4.13(b). This ﬁgure also shows that crossing threads can be
moved either from the right to the left or from the left to the right on the same pick
and adjoining leno pairs may either cross in the same or opposite directions. The
direction of crossing can affect locking, especially with smooth monoﬁlament yarns.
When using two beams it is also possible to use different types or counts of yarn
for standard and crossing ends for design or technical applications. The actual
method of weaving the leno with doups or similar mechanisms is not discussed in
Handbook of technical textiles
When lenos are used for selvedge construction only one to four pairs of threads
are generally used at each side and the leno selvedge is produced by a special leno
mechanism that is independent of the shedding mechanism of the loom. The leno
threads required for the selvedge then come from cones in a small separate creel
rather than from the warp beam. The choice of selvedge yarns and tensions is particularly important to prevent tight or curly selvedges. The crimps selected have to
take into account the cloth shrinkage in ﬁnishing.
4.2.6 Triaxial weaves
Nearly all two-dimensional woven structures have been developed from plain
weave fabrics and warp and weft yarns are interlaced at right angles or at nearly
right angles. This also applies in principle to leno fabrics (see Section 4.2.5 above)
and to lappet fabrics where a proportion of the warp yarns, that is the yarns forming
the design, are moved across a number of ground warp yarns by the lappet mechanism. The only exceptions are triaxial fabrics, where two sets of warp yarns are generally inserted at 60° to the weft, and tetra-axial fabrics where four sets of yarns are
inclined at 45° to each other. So far only weaving machines for triaxial fabrics are
in commercial production. Triaxial weaving machines were ﬁrst built by the BarberColman Co. under licence from Dow Weave and have been further developed by
Howa Machinery Ltd., Japan.
Triaxial fabrics are deﬁned as cloths where the three sets of threads form a
multitude of equilateral triangles. Two sets of warp yarn are interlaced at 60°
with each other and with the weft. In the basic triaxial fabric, shown in Fig. 4.14(a),
the warp travels from selvedge to selvedge at an angle of 30° from the vertical.
When a warp yarn reaches the selvedge it is turned through an angle of 120°
and then travels to the opposite selvedge thus forming a ﬁrm selvedge. Weft
yarn is inserted at right angles (90°) to the selvedge. The basic triaxial fabric is
fairly open with a diamond-shaped centre. The standard weaves can be modiﬁed
by having biplane, stuffed or basic basket weaves, the latter being shown in
Fig. 4.14(b). These modiﬁed weaves form closer structures with different characteristics. Interlacing angles of 75° to the selvedge can be produced. At present
thread spacing in the basic weave fabric is limited to 3.6 or 7.4 threads per
The tear resistance and bursting resistance of triaxial fabrics is greatly superior
to that of standard fabrics because strain is always taken in two directions. Their
shear resistance is also excellent because intersections are locked. They have a wide
range of technical applications including sailcloths, tyre fabrics, balloon fabrics,
pressure receptacles and laminated structures.
The selvedges form the longitudinal edges of a fabric and are generally formed
during weaving. The weave used to construct the selvedge may be the same, or may
differ from, the weave used in the body of the cloth. Most selvedges are fairly narrow
but they can be up to 20-mm wide. Descriptions may be woven into the selvedge,
using special selvedge jacquards, or coloured or fancy threads may be incorporated
for identiﬁcation purposes. For some end-uses selvedges have to be discarded but,
88. Technical fabric structures – 1. Woven fabrics
Triaxial fabrics (weaving machine: Howa TRI-AX Model TWM). (a) Basic weave,
(b) basic basket weave.
(a) Hairpin selvedge – shuttle loom, (b) leno selvedge with dummy selvedge,
(c) helical selvedge, (d) tucked-in or tuck selvedge.
whenever possible, selvedges should be constructed so that they can be incorporated into the ﬁnal product so as to reduce the cost of waste.
In cloths woven on weaving machines with shuttles selvedges are formed by the
weft turning at the edges after the insertion of each pick. The weft passes continuously across the width of the fabric from side to side. In cloths woven on shuttleless
weaving machines the weft is cut at the end of each pick or after every second pick.
To prevent the outside ends from fraying, various selvedge motions are used to bind
the warp into the body of the cloth or edges may be sealed. The essential requirements are that the selvedges should protect the edge of the fabric during weaving
and subsequent processing, that they should not detract from the appearance of the
cloth and that they should not interfere with ﬁnishing or cause waviness, contraction or creasing. Four types of woven selvedges are shown in Fig. 4.15.
Handbook of technical textiles
4.3.1 Hairpin selvedge – shuttle weaving machine
Figure 4.15(a) shows a typical hairpin selvedge which is formed when the weft
package is carried in a reciprocating media, for example a shuttle. With most weaves
it gives a good edge and requires no special mechanism. Frequently strong two-ply
yarns are incorporated into the selvedge whilst single yarns are used in the body of
the cloth because the edge threads are subjected to special strains during beat-up.
To ensure a ﬂat edge a different weave may be used in the selvedge from the body
of the cloth. For twills, satins and fancy weaves this may also be necessary to ensure
that all warp threads are properly bound into the edge. If special selvedge yarns are
used it is important to ensure that they are not, by mistake, woven into the body of
the fabric because they are likely to show up after ﬁnishing or cause a reduction in
the tear and/or bursting resistance of industrial fabrics.
When two or more different weft yarns are used in a fabric only one weft yarn
is being inserted at a time and the other yarn(s) are inactive until the weft is
changed. In shuttle looms the weft being inserted at any one time will form a normal
selvedge whilst the weft yarn(s) not in use will ﬂoat along the selvedge. If long ﬂoats
are formed in weaving, because one weft is not required for a considerable period,
the ﬂoats may have to be trimmed off after weaving to prevent them from causing
problems during subsequent processing. Whenever a pirn is changed, or a broken
pick is repaired, a short length of yarn will also protrude from the selvedge and this
has to be trimmed off after weaving.
Industrial fabrics with coarse weft yarn are sometimes woven with loop selvedges
to ensure that the thread spacing and cloth thickness remains the same right to the
edge of the cloth. To produce a loop selvedge a wire or coarse monoﬁlament yarn
is placed 3 or 4 mm outside the edge warp end and the pick reverses round the wire
to form a loop. As the wire is considerably stiffer than a yarn it will prevent the weft
pulling the end threads together during beat-up. The wire extends to the fell of the
cloth and is automatically withdrawn during weaving. Great care is required to
ensure that no broken-off ends of wire or monoﬁlament remain in the fabric because
they can cause serious damage to equipment and to the cloth during subsequent
4.3.2 Leno and helical selvedges
In most shuttleless weaving machines a length of weft has to be cut for every pick.
For looms not ﬁtted with tucking motions the warp threads at the edges of the fabric
have to be locked into position to prevent fraying. With some weft insertion systems
the weft has to be cut only after every second pick and it is possible to have a hairpin
selvedge on one side of the fabric and a locked selvedge on the second side. Leno
and helical selvedges are widely used to lock warp yarns into position and these are
shown in Fig. 4.15(b) and (c), respectively. When shuttleless weaving machines were
ﬁrst introduced there was considerable customer resistance to fringe selvedges but,
in the meantime, it has been found that they meet most requirements.
With leno selvedges (see also Section 4.2.5) a set of threads at the edge of the
fabric is interlaced with a gauze weave which locks round the weft thread and prevents ravelling of the warp. As the precut length of the picks always varies slightly,
a dummy selvedge is sometimes used at the edge of the cloth as shown in Fig.
4.15(b). This makes it possible to cut the weft close to the body of the cloth resulting in a narrow fringe which has a better appearance than the selvedge from which
90. Technical fabric structures – 1. Woven fabrics
weft threads of varying lengths protrude. It also has the advantage in ﬁnishing and
coating that there are no long lengths of loose weft that can untwist and shed
ﬂy. Because of the tails of weft and because of the warp in dummy selvedges,
more waste is generally made in narrow shuttleless woven fabrics than in fabrics
woven on shuttle looms. For wide cloth the reverse frequently applies because there
is no shuttle waste. Leno selvedges, sometimes referred to as ‘centre selvedges’, may
be introduced into the body of the cloth if it is intended to slit the width of
cloth produced on the loom into two or more widths either on the loom or after
Helical selvedges consist of a set of threads which make a half or complete
revolution around one another between picks. They can be used instead of leno
selvedges and tend to have a neater appearance.
4.3.3 Tucked-in selvedges
A tuck or tucked-in selvedge is shown in Fig. 4.15(d). It gives a very neat and strong
selvedge and was ﬁrst developed by Sulzer5 Brothers (now Sulzer-Textil), Winterthur, Switzerland, for use on their projectile weaving machines. Its appearance is
close to that of a hairpin selvedge and it is particularly useful when cloths with fringe
selvedges would have to be hemmed. High-speed tucking motions are now available and it is possible to produce tucked-in selvedges even on the fastest weaving
Tucked-in selvedges, even when produced with a reduced number of warp
threads, are generally slightly thicker than the body of the cloth. When large batches
of cloth with such selvedges are produced it may be necessary to traverse the cloth
on the cloth roller to build a level roll. The extra thickness will also have to be
allowed for when fabrics are coated. When tucked-in selvedges can be incorporated
into the ﬁnished product no yarn waste is made because no dummy selvedges are
produced but the reduced cost of waste may be counterbalanced by the relatively
high cost of the tucking units.
4.3.4 Sealed selvedges
When fabrics are produced from yarns with thermoplastic properties the edge of a
fabric may be cut and sealed by heat. The edge ends of fringe selvedges are frequently cut off in the loom and the edge threads with the fringe are drawn away
into a waste container. Heat cutting may also be used to slit a cloth, in or off the
loom, into a number of narrower fabrics or tapes.
For special purposes ultrasonic sealing devices are available. These devices are
fairly expensive and can cut more cloth than can be woven on one loom. Whilst they
can be mounted on the loom they are, because of their cost, more frequently
mounted on a separate cutting or inspection table.
Fabric speciﬁcations and fabric geometry
Fabric speciﬁcations6 describe a cloth but frequently need experience for correct
interpretation. The most important elements are cloth width, threads per centimetre in the warp and weft directions, linear density (count) and type of warp and weft
Handbook of technical textiles
yarns (raw material, ﬁlament or staple, construction, direction of twist and twist
factors), weave structure (see Section 4.2 above) and ﬁnish. From these, if the
weaving machine particulars and ﬁnishing instructions are known, the cloth area
density can be calculated.
It has been assumed that other cloth particulars, such as warp and weft cover
factors, crimp, cloth thickness, porosity and drape, have either to be estimated or
measured by various test methods. Peirce7 showed that standard physical and engineering principles can be applied to textiles and cloth speciﬁcations can be forecast
if the effect of interlacing the warp and weft threads and the distortion of the yarns
caused thereby is allowed for.
4.4.1 Fabric width
The width of fabrics is generally expressed in centimetres and has to be measured
under standard conditions to allow for variations which are caused by moisture and
tension. It is necessary to know whether the cloth width required is from edge to
edge or whether it excludes the selvedges. Before deciding on the weaving speciﬁcations of a fabric, allowance has to be made not only for shrinkage from reed width
to grey width during weaving but also for contraction (if any) during ﬁnishing. If
the cloth width changes, other parameters such as cloth area density and threads
per centimetre, will be effected.
4.4.2 Fabric area density
The fabric area density is generally expressed in grams per square metre although
sometimes it is reported as grams per linear metre. It is essential to specify whether
the area density required is loomstate or ﬁnished. The loomstate area density
depends on the weaving speciﬁcation, that is, yarns, thread spacing and weave, and
on any additives, such as size, which are used to improve the weaving process. During
ﬁnishing the cloth area density is frequently altered by tension and chemical treatments or compressive shrinkage which affect cloth width and length, by the removal
of additives needed in weaving and by substances added during ﬁnishing.
The waviness or crimp1 of a yarn in a fabric, shown in the cross-sections of Fig. 4.1,
is caused during weaving and may be modiﬁed in ﬁnishing. It is due to the yarns
being forced to bend around each other during beat-up. It depends on the warp and
weft cover factors, which are described in Section 4.4.4, the characteristics of the
yarns and the weaving and ﬁnishing tensions.
The crimp is measured by the relation between the length of the fabric sample
and the corresponding length of yarn when it has been straightened after being
removed from the cloth, as shown in Fig. 4.16, which, as drawn, is idealized and
only applies to monoﬁlament yarns. Multiﬁlament and staple yarn will be deformed
to some extent at intersections by the pressure exerted by the warp on the weft
or vice versa depending on yarn particulars and cloth construction. It is most
convenient to express crimp as a percentage, which is 100 divided by the fabric
length and multiplied by the difference between the yarn length and the fabric
92. Technical fabric structures – 1. Woven fabrics
4.16 Crimp – relation of length of yarn in cloth to length of cloth. x is the width of sample,
y is the length of yarn extracted from sample and percentage crimp = (y - x)/x ¥ 100.
Warp crimp is used to decide the length of yarn which has to be placed on to a
warper’s beam to weave a speciﬁed length of fabric. Allowance has to be made for
stretching of the yarns during weaving which is generally low for heavily sized
yarns but can be of importance when unsized or lightly sized warps are used. For
fabrics woven on shuttleless weaving machines, the estimated weft crimp has to be
adjusted for the length of yarn used to produce a selvedge and, sometimes, a dummy
4.4.4 Cover factors
The cover factor1 indicates the extent to which the area of a fabric is covered by
one set of threads. For any fabric there are two cover factors: the warp cover factor
and the weft cover factor. The cloth cover factor is obtained by adding the weft
cover factor to the warp cover factor. The cover factors can be adjusted to allow for
yarns of different relative densities – either because of the yarn structure or because
of the raw material used.
The cover factors in SI units8 are calculated by multiplying the threads per centimetre by the square root of the linear density of the yarn (in tex) and dividing by
10. The resultant cover factor differs by less than 5% from the cotton cover factor
pioneered by Peirce7 and expressed as the number of threads per inch divided by
the square root of the cotton yarn count.
For any given thread spacing plain weave has the largest number of intersections
per unit area. All other weaves have fewer intersections than plain weave. The likely
weavability of all fabrics woven with the same weave and from similar yarns can be
forecast from their cover factors. Plain weave fabrics with warp and weft cover
factors of 12 in each direction are easy to weave. Thereafter weaving becomes more
difﬁcult and for cover factors of 14 + 14 fairly strong weaving machines are required.
At a cover factor of 16 + 16 the plain structure jams and a very strong loom with
heavy beat-up is needed to deform the yarns sufﬁciently to obtain a satisfactory beatup of the weft. Some duck and canvas fabrics woven on special looms achieve much
greater cover factors.Three cloths with cover factors of 12 + 12 are shown in Table 4.1.
It shows how thread spacing and linear density have to be adjusted to maintain the
required cover factor and how cloth area density and thickness are affected.
When widely varying cover factors are used for warp and weft, a high cover factor
in one direction can generally be compensated by a low cover factor in the other
direction. In Fig. 4.3, which shows a poplin-type weave, the warp does all the bending
and the weft lies straight. With this construction warp yarns can touch because they
bend around the weft and cloth cover factors of well above 32 can be woven fairly
easily. Peirce calculated the original adjustment factors for a number of weave
Handbook of technical textiles
Table 4.1 Comparison of fabrics with identical warp and weft cover factors woven with
yarns of different linear densities (in SI units)
n1 are warp threads, n2 are weft threads, N1 is the linear density of warp, N2 is the linear density of weft,
K1 is the warp cover factor, K2 is the weft cover factor.
Allowing for 9% of crimp.
Allowing 25% for ﬂattening and displacement of yarns.
Cover factor adjustment factors for weave
2/2 weft rib
1/2 and 2/1 twills
1/3, 3/1 and 2/2 twills
5 end satin and 5 end sateen
Multiply actual cover factor by adjustment factor to obtain equivalent plain weave cover factor.
structures. Rüti9 published an adjustment factor that they found useful to establish
whether fabrics with various weave structures can be woven in their machines and
these are shown in Table 4.2. Sulzer have prepared graphs showing how easy or difﬁcult it is to weave fabrics with different weave structures, thread spacings and linear
densities in various types of weaving machines.
Yarn properties are as important as cloth particulars when forecasting cloth thickness. It is difﬁcult to calculate the cloth thickness because it is greatly inﬂuenced by
yarn distortion during weaving and by pressures exerted on the cloth during ﬁnishing. It is also difﬁcult to measure thickness because the results are inﬂuenced by the
size of the presser feet used in the test instrument, the pressure applied and the time
that has elapsed before the reading is taken. It is therefore essential to specify the
method of measurement of thickness carefully for many industrial fabrics.
Weaving – machines (looms) and operations
Whilst the principle of weft interlacing in weaving has not changed for thousands
of years, the methods used and the way that weaving machines are activated and
controlled has been modiﬁed. During the last few decades of the 20th century the
94. Technical fabric structures – 1. Woven fabrics
rate of change increased continuously and weft insertion rates, which control
machine productivity, increased ten-fold from around 1950–2000 and they are likely
to double again during the ﬁrst ﬁve to ten years of the 21st century. The productivity of the weaver has increased even more and is likely soon to have increased a
hundred-fold. Weaving, which used to be a labour-intensive industry, is now capital
intensive using the most modern technology.
The essential operations in the weaving of a cloth are:
Shedding, i.e. the separation of the warp threads into two (or more) sheets
according to a pattern to allow for weft insertion
2. Weft insertion (picking) and
3. Beating-up, i.e. forcing the pick, which has been inserted into the shed, up to
the fell of the cloth (line where the cloth terminates after the previous pick has
Provision has also to be made for the supply of warp and weft warp yarns and for
the cloth, after weaving, to be collected. The warp yarn is usually supplied on warp
beam(s) and the weft on pirn (shuttle looms only) or cones. A typical cross-section
through a shuttle weaving machine10 showing the main motions, together with the
arrangement of some ancillary motions, is shown schematically in Fig. 4.17. Most
single phase machines, irrespective of their weft insertion system, use similar
motions and a nearly horizontal warp sheet between the back rest(2) and the front
rest(9).Although this is the most common layout, other successful layouts have been
developed. One of these, for an air jet,11 is shown in Fig. 4.18 and an interesting
double-sided air jet with two vertical warp lines back to back is being developed
4.17 Schematic section through Rüti shuttle weaving machine (machine motions and
parts shown in italics). 1, Weaver’s beam holding warp yarn (controlled by let-off ); 2, back
rest guiding yarn and controlling warp tension; 3, drop wires of warp stop motion; 4, shed
formed by top and bottom warp sheet; 5, healds controlled by shedding motion (crank, cam
or dobby) (Jacquard shedding motions do not use healds); 6, sley carrying reed and shuttle.
It reciprocates for beat-up. (In many shuttleless machines the weft insertion system and the
reed have been separated); 7, shuttle carrying the pirn; 8, fell where cloth is formed; 9, front
rest for guiding cloth; 10, take-up motion controlling the pick spacing and cloth wind-up;
11, cloth being wound on to cloth roller.
Handbook of technical textiles
4.18 Schematic section through Elitex air jet weaving machine (machine motions and
parts shown in italics). 1, Weaver’s beam holding warp yarn (controlled by let-off ); 2, back
rest guiding warp yarn; 3, drop wires of warp stop motion; 4, shed formed by top and
bottom warp sheet; 5, healds controlled by cam shedding motion; 6, weft insertion area (the
reed for beating-up located in this area is not shown); 7, fell where cloth is formed; 8, front
rest for guiding cloth; 9, take-up motion controlling the pick spacing and cloth wind-up;
10, cloth being wound on to cloth roller.
Weaving machines can be subdivided into single phase machines, where one weft
thread is laid across the full width of the warp sheet followed by the beat-up
and the formation of the next shed in preparation for the insertion of the next pick,
and multiphase machines, in which several phases of the working cycle take place
at any instant so that several picks are being inserted simultaneously. Single phase
machines are further subdivided according to their weft insertion system, whilst
multiphase machines are classiﬁed according to their method of shed formation. The
classiﬁcation of weaving machines is summarized in Table 4.3.
In this chapter the details of the different types of weaving machines and their
functions can only be outlined and the most important points highlighted. Weaving
machines and their operation are described and discussed by Ormerod and
For the successful operation of a weaving machine good warps are essential.Warp
preparation is, therefore, discussed in Section 4.5.1. This is followed by shedding in
Section 4.5.2, weft insertion and beating-up in Section 4.5.3 and other motions used
on machines in Section 4.5.4. The importance of machine width is considered in
4.5.1 Warp preparation
The success of the weaving operation depends on the quality of the weaver’s beam
presented to the weaving machine because each fault in the warp will either stop
the machine and require rectiﬁcation, or cause a fault in the cloth, which is woven
Before most fabrics can be woven a weaver’s beam (or beams) holding the warp
yarn has to be prepared. For very coarse warp yarns or when very long lengths of
96. Technical fabric structures – 1. Woven fabrics
Classiﬁcation of weaving machines
Single-phase weaving machines
Machines with shuttles (looms):
Hand operated (hand looms)
Non-automatic power looms (weft supply in shuttle changed by hand)
Automatic weaving machines
• shuttle changing
rotary batteries, stack batteries, box loaders or
pirn winder mounted on machine (Uniﬁl)
• pirn changing
Shuttleless weaving machines:
• rigid rapier(s)
single rapier, single rapier working bilaterally
or two rapiers operating from opposite sides of machine
• air (with or without relay nozzles)
• liquid (generally water)
Multiphase weaving machines
Wave shed machines:
Weft carriers move in straight path
Circular weaving machines (weft carriers travel in circular path)
Parallel shed machines (rapier or air jet)
ﬁlament can be woven without modiﬁcation of the warping particulars, a separate
cone creel placed behind each weaving machine can be used economically. It
improves the weaving efﬁciency by avoiding frequent beam changes but requires a
large amount of space. For most yarns, especially sized yarns, it is more economical
to prepare a weaver’s beam and use it in the weaving machine.
The object of most warp preparation systems is to assemble all ends needed in
the weaving machine on one beam and to present the warp with all ends continuously present and the integrity and elasticity of the yarns as wound fully preserved.
Before this can be done the yarns have ﬁrst to be wound on to a cone, then rewound
on to a warper’s beam and ﬁnally sized before the weaver’s beam is made. The
purpose of warp sizing is to apply a protective coating to the yarn to enable it to
withstand the complex stresses to which it is subjected in the weaving machine.
Some coarse ply yarns and some strong ﬁlament yarns can be woven without
Details of the various warp preparation processes are described by Ormerod and
Irrespective of whether cloth is woven on an ancient handloom or produced on the
most modern high speed multiphase weaving machine a shed has to be formed
before a pick can be inserted prior to beat-up and cloth formation. The shed must
be clean, that is slack warp threads or hairy or taped ends must not obstruct the
Handbook of technical textiles
passage of the weft or of the weft carrier. If the weft cannot pass without obstruction either the machine will stop for rectiﬁcation, a warp end may be cut or damaged
or a faulty weave pattern may be produced.
220.127.116.11 Shedding in single phase machines
In most single phase weaving machines, before pick insertion commences, an upper
and a lower warp sheet is formed and the lifting pattern is not changed until the
weft thread has been inserted across the full width of the warp. The shedding
mechanism is used to move individual ends up or down in a prearranged order governed by the weave pattern. To maintain a good separation of the ends during
weaving and avoid adjoining ends from interfering with each other the ends in each
warp sheet can be staggered but in the area of weft insertion an unobstructed gap
through which the weft can pass has to be maintained. The shedding mechanism
chosen for a given weaving machine depends on the patterns that it is intended to
weave on it. Most shedding mechanisms are expensive and the more versatile the
mechanism the greater its cost. On some weaving machines there are also technical limitations governing the shedding mechanisms that can be ﬁtted.
When crank, cam (or tappet) or dobby shedding is used, ends are threaded
through eyes in healds that are placed into and lifted and lowered by heald frames.
All healds in one heald frame are lifted together and all ends controlled by it will
therefore lift alike. The weave pattern therefore controls the minimum number of
healds required. To prevent overcrowding of healds in a heald frame or to even out
the number of ends on a heald frame, more than one frame may lift to the same
pattern. To weave a plain fabric, for example, 2, 4, 6, or 8 heald frames may be used
with equal numbers of frames lifting and lowering the warp on each pick. Crank
motions are generally limited to 8 shafts, cams to 10 or 12 and dobbies to 18 or 24.
When the necessary lifting pattern cannot be obtained by the use of 24 shafts a
Jacquard shedding mechanism, in which individual ends can be controlled separately, has to be used.
The crank shedding mechanism is the simplest and most positive available. It can
only be used to weave plain weave. It is cheap, simple to maintain and in many high
speed machines increases weft insertion rates by up to 10%. This mechanism has
not been used as much as would be expected because of its lack of versatility. It is
however particularly useful for many industrial fabrics that, like the majority of all
fabrics, are woven with plain weave.
Cam or tappet shedding motions on modern high speed machines use grooved
or conjugate cams because they give a positive control of the heald shafts. Negative
proﬁle cams are, however, still widely used especially for the weaving of fairly open
fabrics of light and medium area density. The cam proﬁle is designed to give the
necessary lifting pattern to healds in the sequence required by the lifting plan which
is constructed from the weave structure.
The third method of controlling heald shafts is by dobby and its main advantage
is that there is practically no limit to the size of pattern repeat that can be woven,
whilst with cam motions it is difﬁcult and expensive to construct a repeat of more
than eight or ten picks. It is also easier to build dobbies for a large number of heald
shafts. Dobbies were controlled by pattern chains containing rollers or pegs which
accentuated the lifting mechanism of the heald shafts. Punched rolls of paper or
plastic were used instead of the heavier wooden pegs or metal chains for long
repeats. During the 1990s electronic dobbies have replaced mechanical ones
98. Technical fabric structures – 1. Woven fabrics
enabling weaving machines to operate at much greater speeds, reducing the cost of
preparing a pattern and the time required for changing to a new design. Following
the development of electronic dobbies, cam machines are becoming less popular
because cams for high speed machines are expensive. If large numbers are required,
because of the weave structure or because of frequent pattern changes, it may be
cheaper to buy machines ﬁtted with dobbies.
Shedding mechanisms are still undergoing intensive development and electronic
control of individual shafts may soon reduce the difference in cost between crank,
cam and dobby machines. Developments are likely to simplify the shedding units,
reduce the cost of shedding mechanisms and their maintenance and make weaving
machines more versatile.
When the patterning capacity of dobbies is insufﬁcient to weave the required
designs, Jacquards have to be used. Modern electronic Jacquards can operate at very
high speeds and impose practically no limitation on the design. Every end across
the full width of the weaving machine can be controlled individually and the weft
repeat can be of any desired length. Jacquards are expensive and, if a very large
number of ends have to be controlled individually, rather than in groups, the
Jacquard may cost as much as the basic weaving machine above which it is mounted.
18.104.22.168 Shedding in multiphase weaving machines
In all multiphase weaving machines1 several phases of the working cycle take place
at any instant so that several picks are being inserted simultaneously. In wave
shed machines different parts of the of the warp sheet are in different parts of the
weaving cycle at any one moment. This makes it possible for a series of shuttles or
weft carriers to move along in successive sheds in the same plane. In parallel shed
machines several sheds are formed simultaneously with each shed extending across
the full width of the warp and with the shed moving in the warp direction. The
difference between the methods of shed formation are shown schematically in
Weaving machines in which shuttles travel a circular path through the wave shed
are generally referred to as ‘circular weaving machines’. They have been widely used
for producing circular woven polypropylene fabrics for large bags for heavy loads.
4.19 Weft insertion on multiphase weaving machines (plain weave). (a) Wave shed
principle, (b) multiphase parallel shed principle. Reproduced by kind permission of
99. Handbook of technical textiles
Schematic drawing of Starlinger circular loom SL4. Reproduced by kind permission
of Starlinger & Co. G.m.b.H. (all dimensions in mm).
Combined shed-forming reed/insertion channel
4.21 Shed formation of Sulzer Textil multiphase parallel shed M8300. Shed-forming reed
with weft insertion channel and beat-up reed mounted on drum. Reproduced by kind
permission of Sulzer Textil.
The layout of a Starlinger circular weaving machine16 is shown in Fig. 4.20. The creels
containing cheeses of polypropylene tape are located on either side of the weaving
unit that is in the centre. The warp yarns are fed into the weaving elements from
the bottom, interlaced with weft carried in either four or six shuttles through the
wave shed in the weaving area, and the cloth is drawn off from the middle top and
wound on to a large cloth roll by the batching motion located on the right.
No wave shed machine using weft carriers moving in a straight path has proved
commercially successful because the shedding elements have no upper constraint,
making it impossible to guarantee a correct cloth structure, and because maintaining a clean shed has proved very difﬁcult. Their attraction was a weft insertion rate
of up to 2200 m min-1 but they became obsolescent when simpler single phase air jet
machines begun to exceed this speed.
The ﬁrst parallel shed machine to win limited commercial acceptance was the
Orbit 112,13 which on a two head machine weaving used rigid rapiers for weft insertion and reached weft insertion rates of up to 3600 m min-1 when weaving bandage
fabrics. Sulzer Textil released their new multiphase linear air jet machine, which is
already operating at up to 5000 m min-1 and is only at the beginning of its operational development. This machine, which needs no healds, has a rotating drum on
which the shed-forming reed and beat-up reed are mounted (Fig. 4.21).17 On this
machine shedding is gentle and individual picks are transported across the warp
sheet at relatively low speeds. Weft yarns do not have to be accelerated and decelerated continuously thus reducing the stresses imposed on the yarns. This reduces
demands on yarn and, for the ﬁrst time, we have a machine with a high insertion
100. Technical fabric structures – 1. Woven fabrics
rate which should be able to weave relatively weak yarns at low stop rate and high
4.5.3 Weft insertion and beat-up (single phase machines)
All single phase weaving machines are classiﬁed in accordance with their weft insertion system. The different types have been summarised in Table 4.3. The main
methods of single phase weft insertion are by shuttle (Fig. 4.22), projectile (Fig. 4.23),
rapier and air or water jet (Fig. 4.24).
22.214.171.124 Weft insertion by shuttle
Looms using shuttles for carrying the weft through the warp sheet dominated cloth
production until the 1980s even in high wage countries like the USA. They are now
obsolete, except for use in weaving a few highly specialised fabrics. In spite of this,
large numbers of automatic bobbin changing looms are still in use but they are being
rapidly replaced by shuttleless weaving machines. Shuttleless machines produce
more regular fabrics with fewer faults and need less labour for weaving and maintenance. Millions of handlooms are still in operation in south east Asia being protected by legislation.
Figure 4.22 shows schematically the production of cloth on a shuttle loom. The
shuttle carrying the pirn, on which the weft is wound, is reciprocated through the
warp by a picking motion (not shown) on each side of the machine. For each pick
the shuttle has to be accelerated very rapidly and propelled along the race board.
Whilst crossing through the shed, one pick of weft is released and when the shuttle
reaches the second shuttle box, the shuttle has to be stopped very rapidly. After each
pick has been inserted it has to be beaten-up, that is moved to the fell of the cloth.
The reed and the race board are mounted on the sley and during the weaving cycle
are reciprocated backward and forward. Whilst the shuttle passes through the shed
the sley is close to the healds to enable the shuttle to pass without damaging the
warp yarns. The sley is then moved forward for beat-up. The need to have an open
shed for weft insertion during a considerable part of the picking cycle, and the
weight of the sley carrying the race board and the reed, impose restrictions on the
picking speed, i.e. the number of revolutions at which the loom can operate.
The basic weakness of ﬂy shuttle weaving machines is the unsatisfactory ratio
existing between the large projected mass of the shuttle and the weft bobbin in relation to the small variable mass of the weft yarn carried in the shuttle.13 Only about
4.22 Weft insertion by shuttle (schematic). 1, Warp yarns; 2, reed; 3, shuttle carrying pirn
(entering shed); 4, fell of cloth. Picking motions and race board not shown. Reproduced by
kind permission of Sulzer Textil.
Handbook of technical textiles
3% of the energy imparted to the shuttle is used for the actual weft insertion.
Further limitations on machine speed are imposed by the need to reciprocate the
heavy sley. Whilst theoretically it is possible to attain weft insertion rates of up to
450 m min-1 for wide machines, few shuttle machines in commercial use exceed 250
In a non-automatic power loom each time a pirn is nearly empty the weaver has
to stop the loom and replace it. Pirns should be replaced when there is still a little
weft left on them to prevent the weft running out in the middle of the shed and creating a broken pick which has to be repaired. In industrialized countries most power
looms have been replaced by automatic pirn changing weaving machines that, in
turn, are now being replaced by shuttleless weaving machines. In automatic weaving
machines the pirns are changed without attention from the weaver and without the
loom stopping. The replacement pirns are periodically placed into a magazine by an
operative so that the machine can activate the pirn replacement whenever necessary. The magazine ﬁllers can be replaced by a ‘box loader’ attachment when the
pirns are brought to the loom in special boxes from where they are transferred automatically to the change mechanism. Shuttle change looms, where the shuttle rather
than the pirn is changed whenever the pirn empties, are available for very weak
yarns. All these methods require pirns to be wound prior to being supplied to the
loom. Alternatively a Uniﬁl attachment can be ﬁtted to wind the pirns on the
weaving machine and feed them into the change mechanism.
There are practically no restrictions on the widths or area density of fabrics which
can be woven on shuttle machines. Automatic looms can be ﬁtted with extra shuttle
boxes and special magazines so that more than one weft yarn can be inserted in
accordance with a prearranged pattern. Compared with similar equipment for shuttleless machines this equipment is clumsy and labour intensive.
126.96.36.199 Projectile machines
Projectile machines can use either a single projectile, which is ﬁred from each side
of the machine alternately and requires a bilateral weft supply, or use a unilateral
weft supply and a number of projectiles which are always ﬁred from the same
side and are returned to the picking position on a conveyor belt. Since Sulzer
commenced series production of their unilateral picking multiple projectile
machines in the 1950s they have dominated the market and have sold more shuttleless machines than any other manufacturer. Sulzer Textil have continuously
developed their machines, improved weft insertion rates and machine efﬁciency
and extended the range of fabrics that can be woven on them. They are now used
not only for weaving a vast range of standard fabrics but also for heavy industrial
fabrics of up to 8 m wide, for sailcloth, conveyor belts, tyre cord fabrics, awnings,
geotextiles, airbags and a wide range of ﬁlter fabrics of varying area density and
One of the major advantages of all shuttleless machines is that weft on cone does
not have to be rewound before it is used. This eliminates one process and reduces
the danger from mixed yarn and ensures that weft is used in the order in which it
is spun. On shuttle looms weft is split into relatively short lengths, each one of which
is reversed during weaving which can show up long periodic faults in a yarn.
The standard projectile is 90 mm long and weighs only 40 g, a fraction of the mass
of a shuttle. For pick insertion on a Sulzer machine (see Fig. 4.23) weft is withdrawn
from the package through a weft brake and a weft tensioner to the shuttle feeder,
102. Technical fabric structures – 1. Woven fabrics
4.23 Weft insertion by projectile (Sulzer system) (schematic). 1, Weft (on cone); 2, yarn
brake (adjustable); 3, weft tensioner; 4, weft presenter; 5, torsion rod; 6, weft cutter
(scissors); 7, gripper (to hold cut end); 8, guide teeth; 9, projectile; 10, projectile brake
(receiving side). Reproduced with kind permission of Sulzer Textil.
which places it into the gripper of the projectile. A torsion bar system is used for
picking which transfers the maximum possible strain-energy to the projectile before
it separates from the picker shoe. The torsion bar can be adjusted to deliver the
energy required to propel the projectile through the guide teeth to the shuttle brake.
Sulzer redesigned the reed and the beat-up mechanism so as to obtain a stronger
and more rapid beat-up thus making a higher proportion of the picking cycle available for weft insertion.
Narrow machines can operate at weft insertion rates of up to 1000 m min-1 whilst
3600 mm wide machines can insert weft at up to 1300 m min-1. Models are available
for weaving heavy fabrics, for weaving coarse and fancy yarns and for up to six weft
colours. The machines can be ﬁtted with a variety of shedding motions and are
equipped with microprocessors to monitor and adjust machine performance.
Because of the increase in weft insertion rates with increases in reed width and
because of the decrease in capital cost per unit width for wider projectile machines,
it is often attractive to weave a number of widths of fabric side by side in one projectile machine.
For even wider and heavier fabrics Jürgens18 build a machine using the Sulzer
Rüti system of pick insertion. They can propel a heavier projectile carrying a weft
yarn of up to 0.7 mm diameter across a reed width of up to 12 m. Their machines
take warp from one, two or three sets of warp beams and maintain weaving tensions of up to 30 000 N m-1, accommodate up to 24 shafts controlled by an extra
heavy dobby, and deliver the cloth on to a large batching motion. Jäger have developed a projectile weaving machine for fabrics of medium area density and up to
12 m wide using a hydraulically propelled projectile.
188.8.131.52 Rapier machines
At ITMA Paris 1999, out of 26 machinery manufacturers showing weaving machines
no fewer than 17 offered rapier machines and some offered machines of more than
one type. Rapier machines were the ﬁrst shuttleless machines to become available
Handbook of technical textiles
but, at ﬁrst, they were not commercially successful because of their slow speed. With
the introduction of precision engineering and microprocessor controls, the separation of the weft insertion from the beat-up and improved rapier drives and heads,
their weft insertion rates have increased rapidly. For machines of up to 2500 mm
reed space they equal those of projectile machines with which they are now in direct
Machines may operate with single or double rapiers. Single rapier machines generally use rigid rapiers and resemble reﬁned versions of ancient stick looms. They
have proved attractive for weaving fairly narrow cloths from coarse yarns. Wide
single rapier machines are too slow for most applications. In single rapier machines
the rapier traverses the full width of the shed and generally picks up the weft and
draws it through the shed on its return. A variation of the single rigid rapier is the
single rapier working bilaterally, sometimes referred to as a two-phase rapier. As it
has not been used to any extent for industrial fabrics it is not considered here but
details can be found in the book by Ormerod and Sondhelm.13
Most rapier machines use double rapiers, one rapier entering the shed from each
side. They meet in the middle and transfer the yarn. With the Gabler system weft is
inserted alternately from both sides of the machine and yarn is cut every second
pick with hairpin selvedges being formed alternately on both selvedges. The Gabler
system has now been largely superseded by the Dewas system where weft is inserted
from one side only and is cut after every pick.
Double rapiers machines use either rigid or ﬂexible rapiers. Rigid rapier
machines need more space than machines ﬁtted with any other weft insertion
system. Rigid rapier machines, of which the Dornier HTV and P19 series are prime
examples, are capable of weaving most types of industrial fabrics with weft linear
densities of up to 3000 tex, in widths of up to 4000 mm and at weft insertion rates
of up to 1000 m min-1. Typical fabrics being produced on them range from opencoated geotextile mesh to heavy conveyor belting. A variation of the rigid rapier is
the telescopic rapier.
By far the largest number of rapier machines use double ﬂexible rapiers which
are available in widths up to 4600 mm with even wider machines being custom built
for industrial applications. Standard machines have a relatively low capital cost and
can be used to weave a wide range of low and medium area density fabrics. They
are ideal for weaving short runs and for fabrics woven with more than one weft
because their weft change mechanism for up to eight colours is simple and cheap.
They are widely used for furnishing and fashion fabrics, often with Jacquards. They
are also used for some industrial cloths.
184.108.40.206 Fluid jet weaving machines
Fluid jet machines use either air or water to propel the yarn through the shed. They
do not need a weft carrier or a rapier for weft insertion and therefore have fewer
moving parts and less mass to move. Water jets are only suitable for hydrophobic
yarns whilst most yarns can be woven on air jets. Water jets generally use a single
nozzle at the picking side to propel the yarn through the full width of the shed and
this limits their width to about 2 m. As the ﬂow of air is more difﬁcult to control
than the ﬂow of water under pressure, air jets with single nozzles have only been
commercially successful in widths of up to 1700 mm. For wider machines, booster or
relay nozzles are placed along the reed to ensure the smooth movement of the weft
across the full reed width. Although theoretically wide air jets can be built, com-
104. Technical fabric structures – 1. Woven fabrics
4.24 Weft insertion by airjet (Sulzer Rüti L5000). 1, Supply package; 2, measuring disc;
3, rollers; 4, storage tube; 5, clamp; 6, main nozzle; 7, relay nozzles; 8, reed with tunnel.
Reproduced by kind permission of Sulzer Textil.
mercially single width machines are most attractive and machinery makers limit
their ranges to 3600 or 4000 mm reed width.
Compressed air is expensive to produce and its ﬂow is difﬁcult to control. The
air ﬂow in the shed has, therefore, to be restricted either by special air guides or
‘confusers’ or by passing the weft through a channel in a special ‘proﬁle’ reed. The
former method was pioneered by Elitex and is used in most of their ‘P’ type weaving
machines (Fig. 4.18) of which a large number are in use for weaving light and
medium weight fabrics up to 150 cm wide. Sulzer Rüti developed the ‘te strake’
proﬁle reeds with relay nozzles and this system is shown schematically in Fig. 4.24.
There is one main nozzle per colour and one set of relay nozzles spaced at regular
intervals along the reed. The weft is measured to length in the weft feeder and then
carried by the air stream of the main nozzle into the weft duct, accelerated and
transported further by air discharged from the relay nozzles. After insertion, a
stretch nozzle at the receiving side holds the pick under tension until it is bound
into the cloth.
Since air jets came into large scale commercial use in the 1970s they have been
developed rapidly. They can now weave the majority of fabrics and are dominant
for the mass production of fairly simple cloths. They have reached weft insertion
rates of up to 3000 m min-1, twice that of any other single phase weft insertion system
and are still under intensive development. Their capital cost per metre of weft
inserted is highly competitive. Their operating costs depend largely on the local cost
of electricity and whether low grade waste heat from the compressors can be used
for other operations in the plant.
Air jet machines ﬁtted with an automatic weft fault repair system can correct the
majority of weft faults, including part picks, which occur between the main nozzle
Handbook of technical textiles
and the selvedge on the receiving side. The unit removes the broken thread from
the shed without disturbing the warp ends and then restarts the machine. Only if
the machine cannot locate and repair the fault will it signal for attention. As weft
stops represent the majority of stops on an air jet, the system greatly reduces the
weaver’s work load, frequently by more than 50%. It also reduces machine interference and improves the quality of many fabrics.
Other motions and accessories for single phase weaving machines
220.127.116.11 Warp supply and let-off motion
Warp yarns are generally supplied to the weaving machine on one or more weaver’s
beams. In special cases, as already mentioned above, cone creels can be used. The
warp yarns assembled on the weaver’s beam should be evenly spaced and under
standard tension to ensure that all are of exactly the same length when they are
unwound for weaving. The larger the diameter of the beams the longer the length
of warp which can be wound on to it and the fewer the warp changes required but
the greater the tension variations which have to be compensated. Different weaving
machines accommodate beams of different maximum diameter but most modern
machines can take beams of up to 1000 mm diameter. If even larger diameter beams
are needed for very coarse warp yarns, for example for industrial fabrics or denims,
the beams can be placed into a separate beam creel outside the loom frame. Such
units cater for beams of up to 1600 mm diameter.
The width of yarn on the weaver’s beam has to be at least as wide as the yarn in
the reed. When the warp width required exceeds 2800 mm, more than one beam is
frequently used to simplify sizing and warp transport. If yarns from more than one
beam are used in one cloth it is essential that both beams are prepared under identical conditions to prevent variations which can cause cloth faults after ﬁnishing. The
let-off tensions of different beams have to be carefully controlled and this has
become simpler with the introduction of electronic sensors. When the cloth design
requires the use of warp yarns of widely differing linear densities or results in different warp yarns weaving with widely differing crimps, two or more warp beams
may have to be used in parallel. They can be placed either above each other or
behind each other in the weaving machine. Comparison of Figs. 4.17 and 4.18 shows
how the layout of machines can be modiﬁed without impairing their efﬁciency.
During weaving the let-off motion will release the required amount of yarn for
each pick cycle. It must also hold the warp yarns under even tension so that they
separate easily into two or more sheets during shedding prior to weft insertion and
so that the required tension is maintained during beat-up when the newly inserted
weft is moved by the reed to the fell of the cloth. Let-off motions used to be
mechanically controlled with tension being measured by the deﬂection of the back
rest but now electronic sensors are used for tension measurements and the let-off
is frequently controlled by separate servo motors.
18.104.22.168 Take-up motion
Take-up motions are required to withdraw the cloth at a uniform rate from the fell.
The speed of withdrawal controls the pick spacing, which has to be regular to
prevent weft bars and other faults. In most weaving machines the take-up motion
also controls the winding of the cloth on to the cloth roller. If large rolls of large
106. Technical fabric structures – 1. Woven fabrics
diameter have to be made, as is common for heavy fabrics, a separate batching
motion is placed outside the loom frame. Batching motions can be on a different
level from the weaving machine, either below or above, to reduce the area required
for the weaving shed. To prevent the weaving of long lengths of reject fabric, batching motions can incorporate cloth inspection facilities, sometimes with an intermediate cloth storage unit.
22.214.171.124 Automatic stop motions
The ﬁrst group, warp protector motions, are only necessary on machines which use
a free ﬂying shuttle or projectile. They are designed to prevent the forward movement of the reed if the shuttle fails to reach the receiving side. This prevents
damage to the machine and the breakage of large numbers of ends if the shuttle
Warp stop motions stop the machine if an end breaks. They are activated when
a drop wire, through which an end has been threaded, drops because a broken end
will no longer support it. Drop wires can be connected to mechanical or electrical
stop motions. Yarns have to be properly sized to prevent them being damaged by
the drop wires. Electronic warp stop motions, which do not require physical contact
with the warp, are now being introduced especially for ﬁne ﬁlament yarns.
Weft stop motions are used to activate weft changes in automatic shuttle looms
and to stop weaving machines if the weft breaks during weft insertion. Electronic
motions are available that will stop the machine even if a broken end catches on
again before it reaches the receiving side. In air jet machines ﬁtted with automatic
repair facilities the weft stop motion also starts the weft repair cycle.
126.96.36.199 Quick style change
QSC (quick style change) equipment, ﬁrst shown by Picanol in 1991 and now available from most manufacturers, greatly reduces the time a weaving machine has to
be stopped for a warp change. The warp beam, back rest, warp stop motion, heald
frames and reed are located on a module which separates from the main frame of
the weaving machine and which is transferred by a special transport unit to and
from the entering and knotting department where the module becomes the preparation frame for a replacement warp.14 Thus 90% of the work load, which is normally carried out on the stopped weaving machine, is eliminated from the warp
replenishment cycle and the weaving machine efﬁciency is improved. It also results
in cleaner reeds and healds resulting in better machine performance and improved
4.5.5 Machine width
The reed width of the machine must be equal to or greater than the width in reed
of the fabric to be woven. Width in reed must allow for the width of selvedge and
dummy ends. If the machine is narrower the cloth cannot be woven in the machine.
Generally it is impossible to increase the available reed width of a machine.
Whilst the machine width cannot be exceeded, it is generally possible to weave
narrower fabrics. In Sulzer projectile machines weaving down by up to 50% is possible. Different manufacturers and models have different arrangements for weaving
down – some allow for only 200 mm which is often insufﬁcient considering likely
changes in materials and styles. It is most economic to use a high proportion of the
Handbook of technical textiles
reed width because weaving down is likely to reduce the weft insertion rate. Wider
machines also tend to have higher capital and running costs. On some occasions it
is economic to weave a number of fabrics side by side in one machine. Five, six or
seven roller towels, each with its own tucked selvedges, can be produced in a wide
Sulzer projectile machine.
Because of rapid technological advances modern weaving machines have become
highly automated with most functions electronically controlled. Machine settings
can be adjusted and transferred and many faults can be repaired without requiring
attention by an operative. The frequency of machine stops and their duration has
been reduced. The cost of labour has been desensitized and the cost of production
has been reduced whilst product quality has improved. Because of the cost of
modern machines it becomes ever more important to use the right equipment for
the job and operate machines at high efﬁciency.
At present projectile weaving machines are the most versatile of conventional
machines and by bolting the right equipment to the machine there is hardly a fabric
they cannot weave well. Most simple fabrics can be woven at much lower capital cost
on air jets ﬁtted with simple shedding systems. Their economic range is being
extended continuously. In between there are fabrics which can be woven most
cheaply on rapiers. Multiphase machines, like Sulzer Textil’s linear air jet M8300, are
likely to become cheap producers of simple fabrics in the not too distant future.
1. The Textile Institute Terms and Deﬁnitions Committee, Textile Terms and Deﬁnitions, 10th edition,
The Textile Institute, Manchester, 1995.
2. a t robinson and r marks, Woven Cloth Construction, The Textile Institute, Manchester, 1973.
3. w watson, Textile Design and Colour–Elementary Weaves and Figured Fabrics, Longmans, London,
1912 (later editions revised by Grosicki and published by Butterworth).
4. w watson, Advanced Textile Design, Longmans, London, 1912 (later editions revised by Grosicki and
published by Butterworth).
5. Sulzer Brothers (now Sulzer-Textil), Winterthur, Switzerland.
6. r marks, An Intoduction to Textiles – Workbook: Fabric Production – Weaving, ed. W S Sondhelm,
Courtaulds Textiles plc, Manchester, 1989.
7. f t peirce, The Geometry of Cloth Structure, Manchester, Journal of the Textile Institute, T45, 1937.
8. The Textile Institute Terms and Deﬁnitions Committee, Textile Terms and Deﬁnitions, 10th edition,
Table of SI Units and Conversion Factors, The Textile Institute, Manchester, 1995.
9. Rüti Machinery Works Ltd, Verkauf, Rüti, Switzerland, 1977.
10. Rüti Machinery Works Ltd, Switzerland, ‘C’ Model shuttle weaving machine.
11. Investa, Czechoslovakia, Elitex air jet, ‘P’ type.
12. Somet, Colzate (BG), Italy, ‘Mach 3’ air jet.
13. a ormerod and w s sondhelm, Weaving–Technology and Operations, Chapter 5: ‘Weaving,’ The
Textile Institute, Manchester, 1995 (reprinted 1999).
14. a ormerod and w s sondhelm, Weaving–Technology and Operations, Chapter 2: ‘Warping’ and
Chapter 3: ‘Sizing,’ The Textile Institute, Manchester, 1995 (reprinted 1999).
15. Sulzer Rüti, Wilmslow, Fabric Structure, 3085/06.10.95/Legler/sei, 1995.
16. Maschinenfabrik Starlinger, Vienna, Austria, Circular Loom SL4, Drwg. 0304A3, 1997.
17. Sulzer Rüti, Wilmslow, Shed Formation, 3138/10.10.95/Legler/kaa, 1995.
18. Jürgens GmbH, Emsdetten, Germany, Projectile weaving machine JP-2000, 1996.
19. Lindauer Dornier GmbH, Germany, 1999.
Technical fabric structures – 2. Knitted fabrics
Subhash C Anand
Faculty of Technology, Bolton Institute, Deane Road, Bolton BL3 5AB, UK
Terms and deﬁnitions
Warp knitting is a method of making a fabric by normal knitting means, in which
the loops made from each warp are formed substantially along the length of the
fabric. It is characterised by the fact that each warp thread is fed more or less in
line with the direction in which the fabric is produced. Each needle within the
knitting width must be fed with at least one separate and individual thread at
each course. It is the fastest method of converting yarn into fabric, when compared with weaving and weft knitting (Fig. 5.1).
Weft knitting is a method of making a fabric by normal knitting means, in which
the loops made by each weft thread are formed substantially across the width
of the fabric. It is characterised by the fact that each weft thread is fed more or
less at right angles to the direction in which the fabric is produced. It is possible
to knit with one thread only, but up to 144 threads can be used on one machine.
This method is the more versatile of the two in terms of the range of products
produced as well as the type of yarns utilised (Fig. 5.2).
Single-jersey fabric is a weft-knitted fabric made on one set of needles.
Double-jersey fabric is a weft-knitted fabric made on two sets of needles, usually
based on rib or interlock gaiting, in a manner that reduces the natural extensibility of the knitted structure. These fabrics can be non-Jacquard or Jacquard.
Course is a row of loops across the width of the fabric. Courses determine the
length of the fabric, and are measured as courses per centimetre.
Wale is a column of loops along the length of the fabric. Wales determine the
width of the fabric, and are measured as wales per centimetre.
Stitch density is the number of stitches per unit area of a knitted fabric (loops
cm-2). It determines the area of the fabric.
Stitch length is the length of yarn in a knitted loop. It is the dominating factor
for all knitted structures. In weft knitting, it is usually determined as the average
length of yarn per needle, while in warp knitting, it is normally determined as
the average length of yarn per course.
Handbook of technical textiles
3 2 1 0
1 - 0 / 1 - 2
Yarn linear density indicates the thickness of the yarn and is normally determined in tex, which is deﬁned as the mass in grams of 1 km of the material. The
higher the tex number, the thicker is the yarn and vice-versa.
Overlap is the lateral movement of the guide bars on the beard or hook side of
the needle. This movement is normally restricted to one needle space. In the
fabric a loop or stitch is also termed the overlap.
Underlap is the lateral movement of the guide bars on the side of the needle
remote from the hook or beard. This movement is limited only by the mechani-
110. Technical fabric structures – 2. Knitted fabrics
WEFT KNITTING MACHINES
Simpliﬁed classiﬁcation of knitting machinery.
cal considerations. It is the connection between stitches in consecutive courses
in a warp knitted fabric.
• Tightness factor K is a number that indicates the extent to which the area of a
knitted fabric is covered by the yarn. It is also an indication of the relative
looseness or tightness of the knitting. (K = tex1/2 l-1), where l is the stitch length.
• Area density is a measure of the mass per unit area of the fabric (g m-2).
Weft knitting machines
Figure 5.3 shows a simpliﬁed classiﬁcation of weft knitting equipment. It will be
noticed from Fig. 5.3 that the latch needle is the most widely used needle in weft
knitting, because it is self-acting or loop controlled. It is also regarded as more ver-
Handbook of technical textiles
Compound needle (Kokett needle).
Compound needle (ﬂy
satile in terms of the range of materials that can be processed on latch needle
machines. Bearded needles are less expensive to manufacture, can be produced
in ﬁner gauges and supposedly knit tighter and more uniform stitches compared
with latch needles, but have limitations with regard to the types of material that
can be processed as well as the range of structures that can be knitted on them.
Bearded needle machines are faster than the equivalent latch needle machines.
The compound needle has a short, smooth and simple action, and because it requires
a very small displacement to form a stitch in both warp and weft knitting, its
production rate is the highest of the three main types of needle. Compound needles
are now the most widely used needles in warp knitting and a number of manufacturers also offer circular machines equipped with compound needles. The operation
speeds of these machines are up to twice those of the equivalent latch needle
The main parts of the bearded, latch, compound needle (ﬂy needle frame) and
compound needle (Kokett) are shown in Figs. 5.4, 5.5, 5.6 and 5.7, respectively.
Variations of latch needles include rib loop transfer needles and double-ended purl
112. Technical fabric structures – 2. Knitted fabrics
needles, which can slide through the old loop in order to knit from an opposing bed
and thus draw a loop from the opposite direction.
5.2.1 Loop formation with latch needles
Figure 5.8(a) illustrates the needle at tuck height, that is high enough to receive a
new yarn, but not high enough to clear the old loop below the latch. The needle is
kept at this position because the loop formed at the previous course (A) lies on the
open latch and stops the latch from closing. Note that once a latch is closed, it can
only be opened by hand, after stopping the machine.
In Fig. 5.8(b), the needle has been lifted to the clearing position and the new yarn
(B) is presented. The old loops (A) are below the latch and the new yarn (B) is fed
into the needle hook. A latch guard normally prevents the latch from closing at this
In Fig. 5.8(c), the needle has now moved to its lowest position or knitting point
and has drawn the new loop (B) through the old loop (A) which is now cast-off or
knocked over. The needle now rises and the sequence of movements is repeated for
the next course.
The loop formation on a latch needle machine is also illustrated in Fig. 5.9(a) and
a typical cam system on such a machine is shown in Fig. 5.9(b).
Loop formation with latch needles.
Handbook of technical textiles
Needle positions moving through the CAM
STITCH CAM (ADJUSTABLE)
(a) Loop formation and (b) typical cam system on a latch needle machine.
5.2.2 Single-jersey latch needle machines
This type of machinery is employed throughout the world, either as a basic
machine or with certain reﬁnements and modiﬁcations, to produce fabric ranging
from stockings to single-jersey fabric for dresses and outerwear, as well as a wide
range of fabrics and products for technical applications. The machine sizes vary from
1 feeder 1 inch diameter to 144 feeds 30 inches diameter. Most single-jersey
machines are rotating cylinder type, although a few rotating cam box machines
are still used for specialised fabrics. These machines are referred to as sinker top
machines and use web holding sinkers. Comprehensive reviews of single- and
double-jersey knitting machinery and accessories exhibited at ITMA’95 and
ITMA’99 were published that illustrate the versatility and scope of modern weft
188.8.131.52 Knitting action of a sinker top machine
Figures 5.10(a) to (d) show the knitting action of a sinker top machine during the
production of a course of plain fabric.
Figure 5.10(a) illustrates the rest position. This shows the relative position of
the knitting elements in-between the feeders with the needle at tuck height and the
fabric loop held on the needle latch by the forward movement of the sinker towards
the centre of the machine.
Figure 5.10(b) illustrates the clearing position. The needle has been raised to its
114. Technical fabric structures – 2. Knitted fabrics
Knitting action of a sinker top machine.
highest position by the clearing cam acting on the needle butt; the old loop slides
down from the open latch on to the needle stem.
Figure 5.10(c) illustrates the yarn feeding position. The sinker is partially withdrawn allowing the feeder to present its yarn to the descending needle hook, at the
same time freeing the old loop so that it can slide up the needle stem and under the
open latch spoon.
Figure 5.10(d) illustrates the knock-over position. The needle has now reached
its lowest position and has drawn the new loop through the old loop which is now
knocked over the sinker belly.
Stitch length may be controlled in a number of ways. On machines without
positive feed mechanism, it is controlled mainly by the distance the needle
descends below the sinker belly. Other factors such as input tension (Ti), yarn to
metal coefﬁcient of friction (m) and take-down tension also inﬂuence the ﬁnal
stitch length in the fabric. When a positive feed device is used, the length of
yarn fed to the needles at a particular feed is the factor that decides the stitch
length. Other factors such as input tension Ti , m, stitch cam setting and takedown tension inﬂuence the yarn or fabric tension during knitting, and hence
determine the quality of the fabric. Stitch length is ﬁxed by the positive feed device
The sinker has two main functions and these are:
to hold the fabric loop in a given position whenever the needles rise and
to provide a surface over which the needles draw the loops.
Other advantages of using sinkers include:
The control exerted by the sinker allows minimum tension on the fabric thus
producing a good quality fabric with even loops.
Handbook of technical textiles
Double-jersey machine needle layouts.
Fine adjustments in quality and those required in the knitting of certain difﬁcult
yarns and structures are possible.
The sinker facilitates the setting-up of the machine after a partial or full
press-off (after the latches have been opened manually).
5.2.3 Double-jersey machines
Figure 5.11 shows the needle layout of rib and interlock machines. Both types of
machine are available as circular or ﬂat machines, whereas straight bar or fully fashioned machines are available in rib-type only.
Rib and interlock double-jersey machines are used either as garment length
machines or for producing rolls of fabric. They can be either plain or equipped with
a wide range of mechanical patterning mechanisms at each feed in the cylinder. Both
types can also be equipped with electronic needle mechanisms to produce large area
Jacquard patterns at high speeds.
116. Technical fabric structures – 2. Knitted fabrics
184.108.40.206 Rib machines
Rib machines use two sets of needles and can be ﬂat, circular or fully fashioned. The
needles in the two beds are staggered or have spaces between them (rib gaiting).
Most machines have revolving needle cylinders but in some cases the cams rotate
past stationary needles. Patterning is obtained by altering cam and needle set-out
or by using various needle selection mechanisms including individual needle electronic selection with computer aided design system. Machine diameters range from
71/2–20 inches for garment length and from 30–33 inches for fabric machines. An
example of a modern double-jersey machine is the Monarch V-7E20, a 30 inch diameter, E20, 72 feeders 8-lock machine with RDS on dial and ACT II motorised
automatic friction take-down system. The machine has 2 ¥ 2 cam tracks and can be
converted from rib to interlock or 8-lock timing in minutes. All basic non-jacquard
double-jersey structures can be knitted at a speed factor of 900 (machine diameter
(inches) ¥ machine rpm).
220.127.116.11 Interlock machines
These are latch needle circular machines of the rib type, provided with a cylinder
and dial. Unlike rib machines where the tricks of the dial alternate with the tricks
of the cylinder (rib gaiting) the needle tricks of the cylinder are arranged exactly
opposite those of the dial (interlock gaiting). Long-and short-stemmed needles
are used that are arranged alternately, one long, one short in both cylinder and
dial as shown in Fig. 5.11. An example of a modern high-speed interlock machine
is Sulzer Morat Type 1L 144, which is a 30 inches diameter, 144 feeds, 28 or 32
gauge (npi, needles per inch), 28 rpm, producing at 100% efﬁciency 86.4 m h-1
(15.55 kg h-1) of 76 dtex polyester with 14 cpc (courses per centimetre) and with
an area density of 180 g m-1 (60 inches wide) ﬁnished fabric.
To accommodate the long- and short-stemmed needles, the cam system is
provided with a double cam track. The long dial needles knit with the long cylinder
needles at feeder 1 and the short cylinder needles knit with the short dial needles at
feeder 2. Thus two feeders are required to make one complete course of loop.
18.104.22.168 Needle timing
Two different timings can be employed on 1 ¥ 1 rib and 1 ¥ 1 interlock machines.
Synchronised timing is the timing of a machine that has two sets of needles where
the point of knock-over of one set is aligned with the point of knock-over of the
• Delayed timing is the setting of the point of knock-over of one set of needles
on a two-bed knitting machine out of alignment with that of the other set so
as to permit the formation of a tighter stitch. Broad ribs (i.e. 2 ¥ 2, 3 ¥ 3 etc.),
and rib Jacquard fabrics cannot be produced in delayed timing because there
will not always be cylinder needles knitting either side of the dial needles from
which to draw yarn. Up to nine needles delay is possible, but 4–5 needles delay
22.214.171.124 Knitting action of V-bed ﬂat machine
Figure 5.12 illustrates the different stages of loop formation on a V-bed ﬂat knitting
machine, and Fig. 5.13 shows the cam system used on a simple single system ﬂat
Handbook of technical textiles
Position of needles
Brushes open any
Adjacent needles are
raised to clearing height
Yarn fed to
Loop formation on a V-bed ﬂat knitting machine.
V-bed single-system cams. S are stitch cams, R are raising cams and C
are clearing cams.
118. Technical fabric structures – 2. Knitted fabrics
machine. Power V-bed ﬂat machines are used mainly for the production of knitwear
for children, women and men. They range from simple machines through mechanical jacquard machines to fully electronic and computerised ﬂat machines, even
equipped with presser foot. The developments in the automation of fabric designing, pattern preparation, and electronic needle selection, as well as in the range of
structures and effects which can be produced, have been tremendous and ﬂat
machines and their products are now regarded as extremely sophisticated. High
quality garments can now be produced at competitive prices owing to revolutionary garment production systems feasible with presser foot. Two- and threedimensional structures as well as complete garments without any seams or joins can
be produced on the latest electronic ﬂat knitting machines and the associated design
The basic weft-knitted structures and stitches are illustrated in Fig. 5.14 (A to G),
and the appearance, properties and end-use applications of plain, 1 ¥ 1 rib, 1 ¥ 1
purl and interlock structures are summarised in Table 5.1. These basic stitches are
often combined together in one fabric to produce an enormous range of single- and
double-jersey fabrics or garments. Weft-knitted fabrics are produced commercially
for apparel, household and technical products and they are used for an extremely
large array of products, ranging from stockings and tights to imitation furs and rugs.
The importance and diversity of warp- and weft-knitted fabrics used for various
technical applications has been discussed by Anand,2 who highlighted the fact that
knitted fabrics are being increasingly designed and developed for technical products ranging from scouring pads (metallic) to fully fashioned nose cones for supersonic aircrafts. Warp- and weft-knitted products are becoming popular for a wide
spectrum of medical and surgical products.3
Process control in weft knitting
5.4.1 Main factors affecting the dimensional properties of knitted
fabrics or garments
• Fabric structure: different structures relax differently.
• Fibre(s) type: fabrics or garments made from different ﬁbre(s) relax differently.
• Stitch length: the length of yarn in a knitted loop is the dominating factor for all
• Relaxation/ﬁnishing route: the fabric dimensions vary according to relaxation/
• Yarn linear density: affects the dimensions slightly, but affects fabric tightness,
area density (g m-2) and other physical properties.
Laboratory stages of relaxation
On machine – Strained state: this is predominantly length strain.
Off machine – Dry relaxed state: the fabric moves to this state with time. The dry
Handbook of technical textiles
Plain single-jersey A
Plain single-jersey B
Single Tuck Stitch F
Single Tuck Stitch G
Weft-knitted structures (A–G).
120. Table 5.1
Comparison of appearance and properties
1 ¥ 1 Rib
1 ¥ 1 Purl
Different on face and back;
V-shapes on face, arcs on back
Same on both sides, like
face of plain
Same on both sides, like
back of plain
Same on both sides, like
face of plain
Very high (50–100%)
Thickness and warmth
Thicker and warmer than
plain woven made from same
Much thicker and warmer
Very much thicker and
warmer than plain woven
Very much thicker and
warmer than plain woven
Only from end knitted last
Only from end knitted
Tendency to curl
No tendency to curl
No tendency to curl
No tendency to curl
Men’s and ladies’ shirts
Base fabric for coating
Thick and heavy
Technical fabric structures – 2. Knitted fabrics
Handbook of technical textiles
relaxed state is restricted by fabric structure and ﬁbre type. Only wool can attain
• Static soak in water and dry ﬂat – Wet relaxed state: tight structures do not always
reach a ‘true’ relaxed state. Only wool and silk can attain this state.
• Soak in water with agitation, or Agitation in steam, or Static soak at selected
temperatures (>90 °C) plus, dry ﬂat – Finished relaxed state: the agitation and/or
temperature induces a further degree of relaxation, producing a denser fabric.
Wool, silk, textured yarn fabrics, acrylics.
• Soak in water and Tumble dry at 70 °C for 1 hour – Fully relaxed state:
three-dimensional agitation during drying. All ﬁbres and structures.
Fabric geometry of plain single-jersey structures
Courses per cm (cpc) a 1 l =
Wales per cm (wpc) a 1 l =
s = (cpc ¥ wpc) a 1 l 2 =
kC, kW, kS are dimensionless constants, l is the stitch length and s is the stitch density.
Practical implications of fabric geometry studies
Relationship between yarn tex and machine gauge is given by Equation (5.1):
Optimum tex =
For single-jersey machines, the optimum tex = 1650/G2, and for double-jersey
machines, the optimum tex = 1400/G2, where G is measured in needles per
Tightness factor is given by Equation (5.2):
where l is the stitch length, measured in millimetres. For single-jersey fabrics:
1.29 £ K £ 1.64. Mean K = 1.47. For most weft-knitted structures (including
single- and double-jersey structures and a wide range of yarns): 1 £ K £ 2. Mean
K = 1.5. The tightness factor is very useful in setting up knitting machines. At
mean tightness factor, the strain on yarn, machine, and fabric is constant for a
wide range of conditions.
• Fabric area density is given by Equation (5.3):
Area density =
s ¥ l ¥T
g m -2
122. Technical fabric structures – 2. Knitted fabrics
k-Constant values for wool plain single jerseya
55 ± 2
42 ± 1
2310 ± 10
1.3 ± 0.05
Courses and wales are measured per centimetre and l is measured
For a relaxed fabric cpc/wpc = 1.3. cpc/wpc > 1.3 indicates widthwise
stretching. cpc/wpc < 1.3 indicates lengthwise stretching. ks > 2500
indicates felting or washing shrinkage. Relaxation shrinkage is the
change in loop shape. Felting/washing shrinkage is the change in loop
where s is the stitch density/cm2; l is the stitch length (mm) and T is the yarn tex,
or, Equation (5.4):
g m -2
where ks is a constant and its value depends upon the state of relaxation, that is,
dry, wet, ﬁnished or fully relaxed. The area density can also be given by Equations (5.5) and (5.6)
n ¥ l ¥ cpc ¥ T
g m -1
Area density =
where n is the total number of needles, l is the stitch length (mm) and T is the
yarn tex, or
n ¥ kc ¥ T
g m -1
where kc is a constant and its value depends upon the state of relaxation, that is
dry, wet, ﬁnished or fully relaxed.
• Fabric width is given by Equation (5.7)
Fabric width =
where kw is a constant, and its value depends upon the state of relaxation, that
is, dry, wet, ﬁnished or fully relaxed. It can also be given by Equation (5.8)
n ¥ l = L (course length) Fabric width =
Fabric width depends upon course length and not upon the number of needles
Fabric thickness. In the dry and wet relaxed states, fabric thickness (t) is
dependent upon fabric tightness, but in the fully relaxed state, it is more or less
independent of the fabric tightness factor. In the fully relaxed state t ª 4d where
d is the yarn diameter.
Handbook of technical textiles
5.4.5 Quality control in weft knitting
The dimensions of a weft-knitted fabric are determined by the number of
stitches and their size, which in turn is determined by stitch length. Most knitting
quality control therefore reduces to the control of stitch length; differences in mean
stitch length give pieces of different size; variation of stitch length within the piece
gives appearance defects, by far the most common one being the occurrence of
widthwise bars or streaks owing to variation in stitch length between adjacent
Measurement of stitch length, l
Off machine (in the fabric):
– HATRA course length tester
– Shirley crimp tester.
• On machine (during knitting):
– Yarn speed meter (revolving cylinder only)
– Yarn length counter (both revolving cylinder and cambox machines).
Control of stitch length, l
Positive feed devices:
– Capstan feed: cylindrical or tapered
– Nip feed: garment length machines
– Tape feed: (Rosen feed) circular machines producing plain structures
– Ultrapositive feed: IPF or MPF
• Constant tension device: Storage feed device: ﬂat, half-hose, hose and circular
machines producing either plain or jacquard structures.
• Specialised positive feed devices:
– Positive Jacquard Feeder MPF 20 KIF
– Striper Feeder ITF
– IROSOX Unit (half-hose machines)
– Elastane Feed MER2
– Air controlled feeds for ﬂat and fully fashioned machines. Figure 5.15 shows
a tape feed. A modern ultrapositive feed and a yarn storage feed device are
illustrated in Figs. 5.16 and 5.17, respectively.
End-use applications of weft-knitted fabrics
Weft-knitted fabrics are used for apparel, household and technical products. The
main outlets for the different types of weft-knitted fabrics are as shown below.
The knitting equipment used to produce these fabrics is also given.
Flat bar machines
Machine gauge: normally needles per inch, 3–18 npi
Machine width: up to 78.7 inches
Needle type: latch (compound needle machines are being developed)
Needle bed type: single (hand machines), but mainly rib type
Yarn from top
Wheels may be taken out of action by lowering
the pot-eye plate; thus allowing the yarn to
run free below the level of the tape
Tape positive feed device.
Ultrapositive feed device.
Handbook of technical textiles
Products: jumpers, pullovers, cardigans, dresses, suits, trouser suits, trimmings,
hats, scarves, accessories, ribs for straight-bar machines (fully fashioned
machines). Cleaning clothes, three-dimensional and fashioned products for
technical applications, multiaxial machines are under development.
Yarn storage feed device.
Machine gauge: normally needles per inch, 5–40 npi
Machine diameter: up to 30 inches. Up to 60 inch diameter machines are now
• Needle type: latch, (bearded on sinker wheel and loop wheel, some compound
• Needle bed type: single, rib, interlock, double cylinder
– Hose machines: seamfree hose, tights, industrial use dye bags, knit-de-knit
yarns, industrial fabrics
– Half-hose machines: men’s and boy’s half-hose, ladies’ stockings, children’s
tights, sports socks
– Garment blank machines: underwear, T-shirts, jumpers, pullovers, cardigans,
dresses, suits, trouser suits, vests, briefs, thermal wear, cleaning cloths, technical fabrics
– Fabric machines: rolls of fabric with the following end-uses: jackets, ladies’
126. Technical fabric structures – 2. Knitted fabrics
tops, sports and T-shirts, casual wear, suits, dresses, swimwear, bath robes,
dressing gowns, track suits, jogging suits, furnishing, upholstery, automotive
and technical fabrics, household fabrics.
Straight-bar machines (fully fashioned machines)
Machine gauge: normally needles per 11/2 inch, 9–33 (up to 60 gauge machines
have been produced)
Machine width: from 2–16 section machines – each section up to 36 inches wide
(up to 40 section machines have been produced)
Needle type: bearded or bearded and latch
Needle bed type: single and rib
Products: jumpers, pullovers, cardigans, dresses, suits, trouser suits, fully
fashioned hose, sports shirts, underwear, thermal wear.
The ﬁrst weft-knitting machine was built by William Lee in 1589. In 1775, just under
200 years later, the ﬁrst warp-knitting machine was invented by Crane, an Englishman. It was a single guide bar machine to make blue and white zig-zag striped silk
hosiery and these fabrics were named after Van Dyck, the painter. With the advent
of acetate continuous-ﬁlament yarns after World Ward I, the ﬁrst bulk production
of tricot fabrics was commenced by British Celanese on German Saupe 2-guide bar,
28 gauge machines. Locknits replaced the single guide bar atlas fabrics for lingerie,
the latter being difﬁcult to ﬁnish and laddered easily.
From 1950 to 1970, the growth of the warp-knitting industries in the UK and
other western countries was phenomenal. The main reasons for this colossal
expansion are summarised below (although developments in the various ﬁelds
mentioned here were taking place concurrently). The state of the art and current
developments in tricot and raschel machinery have been summarised below.
Anand also published a review of warp-knitting equipment exhibited by Karl
Mayer at ITMA in 19954 and ITMA’99.8
The discovery of thermoplastic yarns and their suitability, even in very low linear
densities (deniers) and in ﬂat or low-twist form, to be knitted with very low yarn
breakage rates on modern high speed tricot and raschel machines
The extra design scope offered by differential dye yarns
Improved cover-comfort attained through textured and producer-bulked yarns
Elastomeric yarns, which have given a tremendous ﬁllip to the raschel powernet industry.
Higher machine speeds, (up to 3500 cpm)
Finer gauges (up to 40 needles per inch)
Handbook of technical textiles
Wider machines (up to 260 inches)
Increased number of guide bars (up to 78 guide bars)
Special attachments such as cut presser, fallplate, swanwarp, etc.
Some speciality raschel machines such as Co-we-nit and Jacquard machines
and, more recently, redesigned full-width weft insertion raschel and tricot
High speed direct-warping machines and electronic yarn inspection equipment
Electronic stop motions for the knitting machines
Larger knitting beams and cloth batches
Modern heat-setting and beam-dyeing machinery
Electronic warp let-off, electronic patterning, electronic jacquard and electronic
fabric take-up mechanisms
Stable constructions, such as sharkskins, queenscord, etc.
Various net constructions utilising synthetic yarns
Mono-, bi-, tri- and multiaxial structures for technical applications
Three-dimensional and shaped (fashioned) structures for medical and other high
It is well known that the warp-knitting sector, particularly tricot knitting has grown
in step with the expansion of manufactured ﬁbres. In 1956, 17.8 million lbs of regenerated cellulosic and synthetic ﬁbre yarns were warp knitted; the ﬁgure reached a
staggering 70.6 million lbs in 1968.
In the mid-1970s, the tricot industry suffered a major setback, mainly because
of a signiﬁcant drop in the sale of nylon shirts and sheets, which had been the
major products of this sector. It is also true that the boom period of textured polyester double-jersey was also a contributing factor in the sudden and major decline
in the sales of tricot products. A change in fashion and the growth in the demand
for polyester/cotton woven fabrics for shirting and sheeting was another cause of
this decline. The two major manufacturers of warp-knitting equipment, Karl
Mayer and Liba, both in West Germany, have been actively engaged in redesigning their machinery in order to recapture some of the lost trade. The compound
needle is the major needle used on both tricot and raschel machines, and many
specialised versions of warp-knitting machines are now available for producing
household and technical products. One of the major developments in warp
knitting has been the commercial feasibility of using staple-ﬁbre yarns for a wide
range of products. It is also signiﬁcant to note that the warp-knitting sector has
broadened its market base and has expanded into household and technical
fabric markets, such as lace, geotextiles, automotive, sportswear and a wide spectrum of surgical and healthcare products. The current and future potential of
warp-knitted structures in engineering composite materials has been discussed by
5.6.2 Tricot and raschel machines
The principal differences between tricot and raschel machines are listed here:
Latch needles are generally used in raschel machines, while bearded or compound needle machines are referred to as tricot machines. Compound needle
128. Technical fabric structures – 2. Knitted fabrics
raschel machines are also now fairly common. The compound needle is the most
commonly used needle on warp knitting equipment.
Raschel machines are normally provided with a trick plate, whereas tricot
machines use a sinker bar.
In raschel machines the fabric is taken up parallel to the needle stems; in the
tricot machines, however, it is taken up at approximately right angles to the
Raschel machines are normally in a coarser gauge; they are also slower
compared with tricot machines, because more guide bars are frequently used
and they also require a longer and slower needle movement.
Raschel machines are much more versatile in terms of their ability to knit most
types of yarns such as staple yarns, and split ﬁlms, etc. Only continuous-ﬁlament
yarns can be successfully knitted on most tricot machines.
Generally, warp beams are on the top of the machine on raschel machines; on
tricot machines, they are generally at the back of the machine.
A simpliﬁed classiﬁcation of warp-knitting equipment is given in Fig. 5.18; it will be
noticed that apparel, household and technical fabrics are produced on modern
warp-knitting machinery. It is in fact in the technical applications that the full potential of warp knitting is being exploited. It is virtually possible to produce any product
on warp-knitting equipment, but not always most economical.
The simplest warp-knitted structures are illustrated in Fig. 5.19. It can be seen
that both closed- and open-loop structures can be produced and there is normally
very little difference in the appearance and properties between the two types of
5.6.3 Knitting action of compound needle warp-knitting machine
In Fig. 5.20(a) the sinkers move forward holding the fabric down at the correct level
in their throats. The needles and tongues rise with the needle rising faster until the
hook of the needle is at its highest position and is open. In Fig. 5.20(b) the guides
then swing through to the back of the machine and Fig. 5.20(c) shows the guides
shog for the overlap and swing back to the front of the machine.
Figure 5.20(d) shows the needles and the tongues starting to descend, with the
tongues descending more slowly thus closing the hooks. The sinkers start to withdraw as the needles descend so that the old loop is landed onto the closed hook and
the new loops are secured inside the closed hook.
In Fig. 5.20(e) the needle descends below the sinker belly and the old loop is
knocked-over. At this point, the underlap occurs and in Fig. 5.20(f) the sinkers move
forward to hold down the fabric before the needles commence their upward rise to
form a fresh course.
5.6.4 Knitting action of standard raschel machine
In Fig. 5.21(a) the guide bars are at the front of the machine completing their
underlap shog. The web holders move forward to hold the fabric down at the
correct level, whilst the needle bar starts to rise from knock-over to form a fresh
Figure 5.21(b) shows that the needle bar has risen to its full height and the old
Handbook of technical textiles
(Latch, Compound needle)
(Bearded, Compound needle)
Single needle bar
Double needle bar
Single needle bar
Double needle bar
(High pile, technical,
car and domestic
(curtain lace, corsetry,
up to 78 Bars
up to 18 Bars
(with or without
Simpliﬁed classiﬁcation of knitting machinery.
loops slip down from the latches onto the stems after opening the latches. The
latches are prevented from closing by the latch guard. The web holders then start
to withdraw to allow the guide bars to form the overlap movement.
In Fig. 5.21(c) the guide bars swing to the back of the machine and then shog for
the overlap and in Fig. 5.21(d) the guide bars swing back to the front and the warp
threads are laid into the needle hooks. Note: only the front guide bar threads have
formed the overlap movement, the middle and back guide bar threads return
through the same pair of needles as when they swung towards the back of the
machine. This type of movement is called laying-in motion.
In Fig. 5.21(e) the needle bar descends so that the old loops contact and
130. Technical fabric structures – 2. Knitted fabrics
Single-guide bar warp-knitted fabrics. (a) Closed lap fabric, (b) open lap fabric.
Knitting action of compound needle warp-knitting machine.
Handbook of technical textiles
Front guide bar
5.21 Knitting action of a standard raschel machine. (a) Start of new course, (b) start of
overlap, (c) guide bar swinging motion, (d) return swing after overlap, (e) old loop closing
latch, (f) knock-over and underlap movements.
close the latches, trapping the new loops inside. The web holders now start to
Figure 5.21(f) shows the needle bar continuing to descend, its head passing below
the surface of the trick-plate, drawing the new loops through the old loops, which
are cast-off, and as the web holders advance over the trick-plate, the underlap shog
of the guide bar is commenced.
The knitting action of bearded needle warp-knitting machines has not been
given here because in the main the machines likely to be used for technical textile
products would use either latch or compound needles. Also the proportion of new
bearded needle machines sold has decreased steadily over the years. This is mainly
due to the lack of versatility of these machines in terms of the variety of yarns that
can be processed and the range of structures that can be normally knitted on them.
The displacement curves for the three main types of needle are shown in Fig. 5.22.
132. Technical fabric structures – 2. Knitted fabrics
60° 90° 120° 150° 180° 210° 240° 270° 300° 330° 360°
Rotation of mainshaft (Degree)
Displacement curves of various needles.
It is obvious that compound needle machines would operate at faster rates,
provided all other factors are similar.
5.7.1 Stitch notation
Some of the more popular stitches used in the production of warp-knitted fabrics
are given in Fig. 5.23. These stitches, together with the number of guide bars used,
a comprehensive range of types and linear densities of yarns available, fancy threading, controlling individual run-ins and run-in ratios, and various ﬁnishing techniques
are combined and modiﬁed to construct an endless variety of fabrics. The lapping
movements of the individual guide bars throughout one repeat of the pattern are
normally indicated on special paper, called point paper. Each horizontal row of
equally spaced dots represents the same needles at successive courses. The spaces
between the dots, or needles, are numbered 0, 1, 2, 3, 4, and so on, and show the
number of needles transversed by each guide bar. Although three links per course
are normally employed, only two are actually required; the third (last link) is only
used to effect a smoother movement of the guide bar during the underlap. The ﬁrst
link determines the position of the guide bars at the start of the new course. The
second link determines the direction in which the overlap is made. The links, therefore, are grouped together in pairs and the lapping movements at each course are
separated by a comma. For instance, the lapping movements shown in Fig. 5.23(c)
are interpreted as follows:
(1-0) is the overlap at the ﬁrst course
(0,1) is the underlap at the same course, but made in the opposite direction to
(1-2) is the overlap at the second course, and
Handbook of technical textiles
5.23 Stitch notation in tricot knitting. (a) Open pillar, (b) closed pillar, (c) tricot stitch,
(d) 2 ¥ 1 closed lap, (e) 3 ¥ 1 closed lap, (f) 4 ¥ 1 closed lap, (g) open tricot stitch,
(h) two-course atlas, (i) misslapping, ( j) laying-in.
(2,1) is the underlap at the second course, but made in the opposite direction
to the previous underlap.
It will also be observed from Fig. 5.23 that when the underlap is made in the opposite direction to the immediately preceding overlap, a closed loop is formed, but
when the underlap is made in the same direction as the immediately preceding
overlap, or no underlap is made, then an open loop will result.
It is vital to ensure when placing a pattern chain around the drum that the correct
link is placed in contact with the guide bar connecting rod, otherwise the underlap
will occur on the wrong side of the needles, or open loops may be formed instead
of the intended closed loops.
5.7.2 Single-guide bar structures
Although it is possible to knit fabrics using a single fully threaded guide bar, such
fabrics are now almost extinct owing to their poor strength, low cover, lack of
stability and pronounced loop inclination on the face of the fabric. Three examples
of single guide bar structures are shown in Fig. 5.24.
5.7.3 Two-guide bar full-set structures
The use of two guide bars gives a much wider pattern scope than is possible
when using only one, and a large proportion of the fabrics produced in industry
134. Technical fabric structures – 2. Knitted fabrics
Single-guide bar structures.
are made with two guide bars. The ﬁrst group of fabrics to consider are those
made with fully threaded guide bars, as many different effects may be obtained
by altering the lapping movements and these effects may be increased still further
by the use of colour, mixing different yarn, linear densities or using different
yarn types, such as yarns with different dyeing characteristics, textured yarns, and
126.96.36.199 Loop plating
With two fully threaded guide bars, each loop in the fabric will contain two threads,
one supplied by each bar. The underlaps made by the front guide bar are plated on
the back of the fabric and the loops from this bar are plated on the face of the fabric,
whereas the loops and the underlaps formed by the back guide bar are sandwiched
between those from the front guide bar (see Fig. 5.25). It will be observed from
Fig. 5.20(c) that when the guide bars swing through the needles to form the overlap,
the ends will be crossed on the needle hook (normally the two bars form overlaps
in opposite directions). As the guide bars return to the front of the machine, the
threads of the front guide bar are ﬁrst to strike the needles and are wrapped around
the needle hook ﬁrst, whereas the back guide bar threads are placed later and
above those from the front guide bar. If the tensions of the two warp sheets are
similar and the heights of the guide bars are correctly adjusted, the front bar loops
will always be plated on the face of the fabric. Any coloured thread in the front
guide bar will thus appear prominent on both fabric surfaces, an important
factor to be remembered in warp-knit fabric designing (see Fig. 5.25 for loop
Handbook of technical textiles
188.8.131.52 Different structures
The two guide bars may make their underlaps in the same or opposite directions.
If made in the same direction, the fabric will show distortion similar to the single
bar fabric (see Fig. 5.29(a)) as the loops will be inclined. If, however, the underlaps
are made in opposite directions, an equal tension will be imposed in both directions,
and loops will be upright.
The structure of the simplest fabric made with two guide bars is shown in
Fig. 5.25 and is known as full tricot. The appearance of full tricot may be varied by
threading the guide bars with different coloured threads to give vertical stripes of
The most common fabric of all is locknit and its structure and the lapping movements are shown in Fig. 5.26. When correctly knitted, the fabric shows even rows of
upright loops on the face of the fabric, and the two needle underlaps on the back
of the fabric give a smooth sheen. It has a soft handle and is very suitable for lingerie. If the lapping movements for the bars are reversed to give reverse locknit,
the fabric properties are completely changed (Fig. 5.29(e)). The short underlaps will
now appear on the back of the fabric and will trap in the longer ones to give a more
stable and stiff structure, with far less width shrinkage from the needles than ordinary locknit. The underlaps of the back guide bar may be increased to give even
greater stability and opacity with practically no width shrinkage from the needles.
An example of this is sharkskin, whose structure and lapping movements are shown
in Fig. 5.27. Another stable structure is shown in Fig. 5.28, and is know as queens
cord. The long back guide bar underlaps are locked ﬁrmly in the body of the fabric
by the chain stitches of the front guide bar. Both sharkskin and queenscord structures can be made more stable, heavier and stronger by increasing the back guide
underlaps to four or ﬁve needle spaces. The vertical chains of loops from the front
136. Technical fabric structures – 2. Knitted fabrics
guide bar may be used to give single wale vertical stripes of colour, such as pin
stripes in men’s suiting.
If the guide bars making a sharkskin are reversed, that is, if the front bar makes
the longer underlaps, the resultant fabric is known as satin which is a lustrous soft
fabric similar to the woven satin. Because of the long ﬂoats on the back of the fabric,
Handbook of technical textiles
satin laps are used to make loop-raised fabrics. The raising machine is set so that
the underlaps are raised into loops without actually breaking any ﬁlaments. In order
to achieve the maximum raising effect, the two guide bars in a loop-raised fabric
are normally made to traverse in the same direction, and open loops may also be
used. The lapping movements of three-needle satin are shown in Fig. 5.29(b) and
those for a three-needle loop-raised fabric are shown in Fig. 5.29(a). The density
and height of pile can be increased by increasing the front guide bar underlaps to
four, ﬁve or six needle spaces.
Yarns may be introduced into the fabric without actually knitting. Figure 5.30
shows the structure lapping movements and pattern chains of a laid-in fabric. The
laid-in thread is trapped between the loop and the subsequent underlap of the guide
bar which must be situated in front of the laying-in bar. In order to lay-in a yarn,
therefore, that yarn must be threaded in a guide bar to the rear of the guide bar
(knitting bar), and it must make no overlaps. Laying-in is a useful device because a
laid-in thread never goes round the needle, and therefore very thick or fancy yarns
may be introduced into the fabric, such as heavy worsted yarn or metallic threads.
Figure 5.31 shows the laid-in thread being trapped in the fabric by the front guide
bar threads knitting an open tricot stitch (0-1, 2-1).
5.7.4 Grey speciﬁcation of a warp-knitted fabric
A complete grey speciﬁcation of a warp-knitted fabric should include the following
gauge of machine in needles per inch
number of guide bars in use
138. Technical fabric structures – 2. Knitted fabrics
Some two-guide bar full set structures. (a) Loop raised, (b) satin, (c) locknit, (d) full
tricot, (e) reverse locknit, (f) sharkskin, (g) queenscord, (h) laid-in fabric.
number of ends in each warp
types and linear densities of yarns used
run-in per rack for each warp
knitted quality of the fabric in courses per centimetre
order of threading in each guide bar
lapping movements of each guide bar during one repeat of the pattern or
details of the pattern wheels or pattern chains
9. relative lateral positions of the guide bars at a given point in the lapping
10. any special knitting instructions.
5.7.5 Fabric quality
The main parameter controlling the quality and properties of a given structure is
the run-in per rack, or the amount of yarn fed into the loop. Run-in per rack is
Principle of laying-in.
140. Technical fabric structures – 2. Knitted fabrics
deﬁned as the length of warp fed into the fabric over 480 courses (1 rack = 480
courses). In two-guide bar fabrics, the run-in per rack for each guide bar may be the
same or different, depending upon the fabric structure. For example, in full tricot
structures (front: 1-2, 1-0 and back: 1-0, 1-2), it is normal to use the same run-in per
rack from both beams or 1 : 1, whereas in three-needle sharkskin fabrics (front: 1-2,
1-0 and back: 1-0, 3-4), the run-in per rack required from the back beam would be
more than the front beam say 1 : 1.66.
The run-in may be altered in two different ways, ﬁrst by altering the total run-in
of the bars, and second by altering the ratio or difference between the bars. Altering the total run-in will affect the ﬁnished number of courses per centimetre and
hence the area density of the fabric, the stability and the cover, but not the general
shape of the loop. Altering the difference between the guide bars will change the
balance of the fabric, affect the inclination of the loops and, because it puts more
or less strain on the individual yarns, change the strength.
Fabric take-up on the machine is adjusted to attain trouble-free knitting and also
to effect ease of ﬁnishing.
5.7.6 Tightness factor
The tightness factor K of a knitted fabric is deﬁned as the ratio of the fabric area
covered by the yarn to the total fabric area. It is regarded as a measure of looseness or tightness of the structure, and inﬂuences dimensions such as the length,
width, and thickness and many other fabric characteristics such as area density,
opacity, abrasion resistance, modulus, strength and shrinkage.
If the tightness factor of a single-guide bar fabric is deﬁned as in Equation 5.2
where l is the stitch length, measured in millimetres, and tex is the yarn linear density,
then the tightness factor of a two-guide bar, full-set fabric is given by Equation (5.10)
where sufﬁxes f and b refer to front and back guide bars, and l is the stitch length
equal to (run-in/rack)/480 and is measured in millimetres. If the same tex is
employed in both bars, then
K = tex
Ê 1 1ˆ
Ë lf lb ¯
For most commercial two-guide bar full-set fabrics 1 £ K £ 2 with a mean tightness
factor value of 1.5.6
5.7.7 Area density
The area density of a single-guide bar fabric can be determined from Equation
Mass of the fabric = cpc ¥ wpc ¥ l ¥ T ¥ 10-2 gm-2
= s ¥ l ¥ T ¥ 10-2 gm-2
Handbook of technical textiles
where s is the stitch density (cm-2) or (cpc ¥ wpc), l is the stitch length (mm) and
T is the yarn tex.
Similarly, the area density of a two-guide bar full-set fabric would be Equation
Mass of the fabric = s[(l f ¥ Tf ) + (l b ¥ Tb )] ¥ 10 -2 gm -2
where sufﬁxes f and b refer to the front and back guide bars. If the same tex is
used in both guide bars, then the above equation can be written as Equation
Mass of the fabric = s ¥ T ¥ 10 -2 (l f + l b )gm -2
= s ¥ T ¥ 10 -2
Ê Total run-in ˆ
If the stitch density, that is, the number of loops cm-2, stitch length in millimetres of the individual guide bars and tex of yarns employed in individual beams are known, the fabric area density can be readily obtained using the
above equation in any fabric state, that is, on the machine, dry relaxed or fully
The geometry and dimensional properties of warp-knitted structures have been
studied by a number of researchers including Anand and Burnip.6
5.7.8 End-use applications of warp-knitted fabrics
Speciﬁcation for tricot machines is:
Type of needle: compound or bearded
Machine gauge: from 18 to 40 needles per inch (E18–E40)
Machine width: from 213 to 533 cm (84–210 inches)
Machine speed: from 2000 to 3500 courses per minute (HKS 2 tricot machine
operates at 3500 cpm)
Number of needle bars: one or two
Number of guide bars: from two to eight
Products: lingerie, shirts, ladies’ and gents’ outerwear, leisurewear, sportswear,
swimwear, car seat covers, upholstery, technical fabrics, bed linen, towelling,
lining, nets, footwear fabrics, medical textiles.
Speciﬁcation for raschel machines is:
Type of needle: latch or compound
Machine gauge: from 12 to 32 needles per inch (E12–E32).
Machine width: from 191 to 533 cm (75–210 inches)
Machine speed: from 500 to 2000 courses per minute
Number of needle bars: one or two
Number of guide bars: from two to seventy-eight
Products: marquisettes, curtains, foundation garments, nets, ﬁshing nets, sports
nets, technical fabrics, curtain lace, power nets, tablecloths, bed covers, elastic
bandages, cleaning cloths, upholstery, drapes, velvets, carpets, ladies’ underwear,
fruit and vegetable bags, geotextiles, medical textiles.
142. Technical fabric structures – 2. Knitted fabrics
1. s c anand, ‘ITMA ’95 review of circular knitting machines and accessories’, Asian Textile J.,
February 1996, 49.
2. s c anand, ‘Contributions of knitting to current and future developments in technical textiles’, Inaugural
Conference of Technical Textiles Group, The Textile Institute, Manchester, 23–24 May, 1988.
3. s c anand, ‘Knitting’s contribution to developments in medical textiles’, Textile Technol. Int., 1994,
4. s c anand, ‘Fine array of warp knitting machines from Karl Mayer’, Asian Textile J., April 1996, 51.
5. s c anand, ‘Warp knitted structures in composites’, ECCM-7 Proceedings, Volume 2, Woodhead Publishing, Cambridge, UK, 14–16 May 1996, p. 407.
6. s c anand and m s burnip, ‘Warp–knit construction’, Textile Asia, September 1981, 65.
7. s c anand, ‘Speciality knitting equipment at ITMA’99’, Asian Textile J., December 1999, 49.
8. s c anand, ‘Karl Mayer warp knitting equipment at ITMA’99’, Asian Textile J., September 1999, 49.
Technical fabric structures – 3. Nonwoven
Philip A Smith
Department of Textile Industries, University of Leeds, Leeds LS2 9JT, UK
It is an unfortunate fact that there is no internationally agreed deﬁnition of nonwovens, in spite of the fact that the International Standards Organization published
a deﬁnition in 1988 (ISO 9092:1988). Many countries, particularly those that have
played an active part in the development of nonwovens, still prefer their own
national deﬁnition, which is generally wider in its scope than the very narrow deﬁnition of ISO 9092.
As it is essential to be clear on the subject matter to be included in this chapter,
I have decided to use the deﬁnition of the American Society for Testing Materials
(ASTM D 1117-80). This deﬁnition is as follows: ‘A nonwoven is a textile structure produced by the bonding or interlocking of ﬁbres, or both, accomplished by
mechanical, chemical, thermal or solvent means and combinations thereof. The term
does not include paper or fabrics that are woven, knitted or tufted.’ It has to be admitted that this deﬁnition is not very precise, but it has been chosen because it
includes many important fabrics which most people regard as nonwovens, but which
are excluded by ISO 9092. Nonwovens are still increasing in importance; production is increasing at the rate of 11% per annum.
One of the major advantages of nonwoven manufacture is that it is generally
done in one continuous process directly from the raw material to the ﬁnished fabric,
although there are some exceptions to this. This naturally means that the labour cost
of manufacture is low, because there is no need for material handling as there is in
older textile processes. In spite of this mass-production approach, the nonwovens
industry can produce a very wide range of fabric properties from open waddings
suitable for insulation containing only 2–3% ﬁbres by volume to stiff reinforcing
fabrics where the ﬁbre content may be over 80% by volume. How is this wide range
of properties produced? All nonwoven processes can be divided into two stages, the
preparation of the ﬁbres into a form suitable for bonding and the bonding process
itself. There are a number of different ways of ﬁbre processing, each producing its
144. Technical fabric structures – 3. Nonwoven fabrics
own particular characteristic in the ﬁnal fabric. Equally there are a number of
different bonding methods which have an even bigger effect on the ﬁnished fabric
properties. Almost all the ﬁbre processing methods can be combined with all the
bonding methods, so that the range of different possible manufacturing lines is
enormous, allowing a great range of ﬁnal properties.
However, this does raise a difﬁculty in describing the nonwoven process. We
know that the process is essentially a continuous one in which the ﬁbre processing
and bonding take place in two machines tightly linked together, but it is impossible
to describe the combined machines together owing to the wide number of machine
combinations that are possible. Instead it is necessary to explain the methods of
ﬁbre processing and the methods of bonding separately.
In ﬁbre processing it is common to make ﬁrst a thin layer of ﬁbre called a web
and then to lay several webs on top of each other to form a batt, which goes directly
to bonding. The words web and batt are explained by the previous sentence,
but there are cases where it is difﬁcult to decide if a ﬁbre layer is a web or a batt.
Nevertheless the ﬁrst stage of nonwoven processing is normally called batt
Methods of batt production using carding machines
The principles of carding and the types of carding machines have already been discussed in Chapter 3. The machines in the nonwoven industry use identical principles and are quite similar but there are some differences. In particular in the process
of yarn manufacture there are opportunities for further opening and for improving
the levelness of the product after the carding stage, but in nonwoven manufacture
there is no further opening at all and very limited improvements in levelness are
possible. It therefore follows that the opening and blending stages before carding
must be carried out more intensively in a nonwoven plant and the card should be
designed to achieve more opening, for instance by including one more cylinder,
though it must be admitted that many nonwoven manufacturers do not follow
Theoretically either short-staple revolving ﬂat cards or long-staple roller cards
could be used, the short-staple cards having the advantages of high production and
high opening power, especially if this is expressed per unit of ﬂoor space occupied.
However, the short-staple cards are very narrow, whereas long-staple cards can be
many times wider, making them much more suitable for nonwoven manufacture,
particularly since nonwoven fabrics are required to be wider and wider for many
end-uses. Hence a nonwoven installation of this type will usually consist of automatic ﬁbre blending and opening feeding automatically to one or more wide longstaple cards. The cards will usually have some form of autoleveller to control the
mass per unit area of the output web.
6.2.1 Parallel laying
The mass per unit area of card web is normally too low to be used directly in a nonwoven. Additionally the uniformity can be increased by laying several card webs
over each other to form the batt. The simplest and cheapest way of doing this is by
parallel laying. Figure 6.1 shows three cards raised slightly above the ﬂoor to allow
a long conveyor lattice to pass underneath. The webs from each card fall onto the
Handbook of technical textiles
Alternative layout for parallel laying.
lattice forming a batt with three times the mass per unit area. If the cards are longer
this method becomes unwieldy and instead the cards are placed side-by-side as in
The card webs are turned through a right angle by a guide at 45°, but the batt
produced by this method is identical in all respects to the previous method. It is
important to recognise that it is not cross laid, as in Section 6.2.2, in spite of the
similarities between the layouts.
In any card web there is a marked tendency for the ﬁbres to lie along the web
rather than across it. Since in parallel laying all the card webs are parallel to each
other (and to the batt), it follows that most of the ﬁbres will lie along the batt and
very few across it. At this stage it is important to introduce two terms used widely
in nonwovens. The direction along the batt is called the ‘machine direction’ and the
direction at right angles is called the ‘cross direction’. Whatever method of bonding
is used it is found that the bonds are weaker than the ﬁbres. A tensile test on a
bonded parallel-laid material in the machine direction will depend mainly on the
ﬁbre strength, whereas in the cross direction it will depend more on the bond
strength. The effect of these facts on the relative ﬁbre frequency and on the directional strength of a typical parallel-laid fabric in various directions is shown in
The weakness of the fabric in the cross direction has a profound effect on possible uses of the fabric. Brieﬂy it can be used when strength is not required in either
146. Technical fabric structures – 3. Nonwoven fabrics
Polar diagrams showing (a) the relative frequency of ﬁbres lying in various directions
and (b) the relative strength in various directions for a parallel-laid fabric.
direction, for example, a ﬁlter fabric which is completely supported or as a wiping
cloth. It is especially useful when high strength is required in one direction but
strength in the other direction is not important, but examples of this are rare; the
one usually quoted is a narrow tape cut in the machine direction and used mainly
for medical purposes.
This situation has been altered by the advent of cards designed especially for the
nonwoven industry. These cards are given a randomising doffer, which as its name
implies, makes the ﬁbre directions more random, together with ‘scrambling rollers’
that condense the card web in length, having the effect of buckling those ﬁbres lying
in the machine direction and forming segments lying in the cross direction.
By using these two techniques together it is possible to bring the strength ratio of
parallel-laid fabric down from the normal 10 or 20 : 1 to 1.5 : 1, which is about as
isotropic as any nonwoven. It may also be worth mentioning that similar carding
techniques have been expanded even further to make a card that produces a really
thick web, making laying unnecessary. However, all parallel-lay processes suffer
from a further fundamental problem; the width of the ﬁnal fabric cannot be wider
than the card web, while current trends demand wider and wider fabrics.
6.2.2 Cross laying
When cross laying, the card (or cards) are placed at right angles to the main conveyor just as in Fig. 6.2, but in this case the card web is traversed backwards and
forwards across the main conveyor, which itself is moving. The result is a zig-zag as
shown in Fig. 6.4.
Usually the conveyor B is moving only slowly so that many layers of card web
are built up, as shown in the diagram. The thickness of the card web is very small
in comparison with the completed batt, so that the zig-zag marks, which appear so
prominent in the ﬁgure, do not usually show much. There are two major problems
with cross layers; one is that they tend to lay the batt heavier at the edges than in
the middle. This fault can be corrected by running the traversing mechanism
rather slower in the centre and more rapidly at the edges, with a very rapid change
Handbook of technical textiles
Cross laying. A, card web; B, main conveyor; C, traverse mechanism; q, angle of
of direction at the edge. The other problem is trying to match the input speed of the
cross layer with the card web speed. For various reasons the input speed of the cross
layer is limited and the speed of the card web has to be reduced to match it. Because
for economic reasons the card is forced to run at maximum production, the card
web at the lower speed is thicker and the cross-laying marks discussed above will
tend to show more. In spite of these problems, cross layers are used much more
frequently than parallel layers.
The diagram in Fig. 6.4 showing webs crossing at an angle seems to imply that
the batt will be fairly isotropic. However, this is not so because the cross-laying angle
(q in Fig. 6.4) is normally less than 10°, so that the great majority of ﬁbres lie in or
near the cross direction. Cross-laid fabrics are consequently very strong in the
cross direction and weak in the machine direction. In many cases this may not
matter, because cross-laid fabrics are often quite heavy and may not require much
strength, but in many other cases a more isotropic batt is required. The obvious solution is to combine parallel laying and cross laying together; this is done very occasionally but it is uncommon because it combines the limitations of both systems,
that is, the relatively narrow width of parallel laying and the slow output speed of
the cross laying. The common solution is to stretch the batt in the machine direction as it exits from the cross layer. Various machines are available for doing this;
the important criterion is that the stretching should be even, otherwise it could
create thick and thin places in the batt. Cross laying, with or without stretching, is
much more popular than parallel laying and is probably the most widely used system
The air-laying method produces the ﬁnal batt in one stage without ﬁrst making a
lighter weight web. It is also capable of running at high production speeds but is
similar to the parallel-lay method in that the width of the ﬁnal batt is the same as
the width of the air-laying machine, usually in the range of 3–4 m.
148. Technical fabric structures – 3. Nonwoven fabrics
The degree of ﬁbre opening available in an air-lay machine varies from one
manufacturer to another, but in all cases it is very much lower than in a card. As a
consequence of this more ﬁbre opening should be used prior to air laying and the
ﬁbres used should be capable of being more easily opened, otherwise the ﬁnal batt
would show clumps of inadequately opened ﬁbre. In the past the desire for really
good ﬁbre opening (which is needed for lightweight batts) led to a process consisting of carding, cross laying, then feeding the cross-laid batt to an air-laying machine.
The only purpose of the air-lay machine in this example was to obtain the desired
machine : cross-direction strength ratio, but it is a very expensive way compared to
the stretching device discussed above and such a process would not be installed
The diagram in Fig. 6.5 shows the principle of an air-lay machine, although the
actual machines may vary considerably from this outline. Opened ﬁbre from the
opening/blending section is fed into the back of hopper A, which delivers a uniform
sheet of ﬁbres to the feed rollers. The ﬁbre is then taken by the toothed roller B,
which is revolving at high speed. There may or may not be worker and stripper
rollers set to the roller B to improve the opening power. A strong air stream C dislodges the ﬁbres from the surface of roller B and carries them onto the permeable
conveyor on which the batt is formed. The stripping rail E prevents ﬁbre from recirculating round the cylinder B. The air ﬂow at D helps the ﬁbre to stabilise in the
Figure 6.6 shows the formation zone in more detail. This shows that the ﬁbres
fall onto an inclined plane, and that the angle between this plane and the plane of
the fabric depends on the width of the formation zone, w, and the thickness of the
Principle of air-lay machine. A, Hopper/chute feed; B, opening roller; C, air ﬂow from
fan; D, suction to fan; E, stripping rail; F, batt conveyor.
Close-up of the formation zone.
Handbook of technical textiles
batt, t. It is possible when making thick fabrics to reduce the width, w, so that the
ﬁbres lie at a substantial angle to the plane of the batt. It is claimed that for this
reason air-laid fabrics show better recovery from compression compared with crosslaid fabrics. It is often thought because the ﬁbres are deposited without control
from an air stream that they will be random in the plane of the batt. This belief is
so widespread that air-laid fabrics are frequently called ‘random-laid’ fabrics. The
use of this term should be strongly discouraged, because it gives a false impression.
In fact air-laid fabrics can have strength ratios as high as 2.5 : 1, which is far from
random. It is thought that the increase in the machine direction strength is caused
by the movement of the conveyor; a ﬁbre in the air-stream approaching the conveyor will tend to be pulled into the machine direction as it lands on the moving
The parallel-laid, cross-laid and air-laid methods discussed so far, are collectively known as dry-laid processes. They are the most similar to traditional textile
processing and currently account for slightly less than half the total nonwoven
The wet-laid process is a development from papermaking that was undertaken
because the production speeds of papermaking are very high compared with textile
production. Textile ﬁbres are cut very short by textile standards (6–20 mm), but at
the same time these are very long in comparison with wood pulp, the usual raw
material for paper. The ﬁbres are dispersed into water; the rate of dilution has to
be great enough to prevent the ﬁbres aggregating. The required dilution rate turns
out to be roughly ten times that required for paper, which means that only specialised forms of paper machines can be used, known as inclined-wire machines. In
fact most frequently a blend of textile ﬁbres together with wood pulp is used as the
raw material, not only reducing the necessary dilution rate but also leading to a big
reduction in the cost of the raw material. It is now possible to appreciate one of the
problems of deﬁning ‘nonwoven’. It has been agreed that a material containing 50%
textile ﬁbre and 50% wood pulp is a nonwoven, but any further increase in the wood
pulp content results in a ﬁbre-reinforced paper. A great many products use exactly
50% wood pulp. Wet-laid nonwovens represent about 10% of the total market, but
this percentage is tending to decline. They are used widely in disposable products,
for example in hospitals as drapes, gowns, sometimes as sheets, as one-use ﬁlters,
and as coverstock in disposable nappies.
Dry laying wood pulp
The paper industry has attempted for many years to develop a dry paper process
because of the problems associated with the normal wet process, that is, the removal
of very large volumes of water by suction, by squeezing and ﬁnally by evaporation.
Now a dry process has been developed using wood pulp and either latex binders or
thermoplastic ﬁbres or powders to bond the wood pulp together to replace hydrogen bonding which is no longer possible. Owing to the similarity of both the bonding
methods and some of the properties to those of nonwovens, these products are being
150. Technical fabric structures – 3. Nonwoven fabrics
referred to as nonwovens in some areas, although it is clear from the deﬁnition
above they do not pass the percentage wood pulp criterion. Hence although the drylaid paper process cannot be regarded as a nonwoven process at present, it is very
likely that the process will be modiﬁed to accept textile ﬁbres and will become
very important in nonwovens in the future. It is for this reason that it has been
Spun laying includes extrusion of the ﬁlaments from the polymer raw material,
drawing the ﬁlaments and laying them into a batt. As laying and bonding are normally continuous, this process represents the shortest possible textile route from
polymer to fabric in one stage. In addition to this the spun-laid process has been
made more versatile. When ﬁrst introduced only large, very expensive machines
with large production capabilities were available, but much smaller and relatively
inexpensive machines have been developed, permitting the smaller nonwoven producers to use the spun-laid route. Further developments have made it possible to
produce microﬁbres on spun-laid machines giving the advantages of better ﬁlament
distribution, smaller pores between the ﬁbres for better ﬁltration, softer feel and
also the possibility of making lighter-weight fabrics. For these reasons spun-laid production is increasing more rapidly than any other nonwoven process.
Spun laying starts with extrusion. Virtually all commercial machines use thermoplastic polymers and melt extrusion. Polyester and polypropylene are by far the
most common, but polyamide and polyethylene can also be used. The polymer chips
are fed continuously to a screw extruder which delivers the liquid polymer to a
metering pump and thence to a bank of spinnerets, or alternatively to a rectangular spinneret plate, each containing a very large number of holes. The liquid polymer
pumped through each hole is cooled rapidly to the solid state but some stretching
or drawing in the liquid state will inevitably take place. Up to this stage the technology is similar to the ﬁbre or ﬁlament extrusion described in Chapter 2, except
that the speeds and throughputs are higher, but here the technologies tend to divide.
In spun laying the most common form of drawing the ﬁlaments to obtain the correct
modulus is air drawing, in which a high velocity air stream is blown past the ﬁlaments moving down a long tube, the conditions of air velocity and tube length being
chosen so that sufﬁcient tension is developed in the ﬁlaments to cause drawing to
take place. In some cases air drawing is not adequate and roller drawing has to be
used as in normal textile extrusion, but roller drawing is more complex and tends
to slow the process, so that air drawing is preferred.
The laying of the drawn ﬁlaments must satisfy two criteria; the batt must be as
even as possible in mass per unit area at all levels of area, and the distribution of
ﬁlament orientations must be as desired, which may not be isotropic. Taking the
regularity criterion ﬁrst, the air tubes must direct the ﬁlaments onto the conveyor
belt in such a way that an even distribution is possible. However, this in itself is not
sufﬁcient because the ﬁlaments can form agglomerations that make ‘strings’ or
‘ropes’ which can be clearly seen in the ﬁnal fabric. A number of methods have been
suggested to prevent this, for instance, charging the spinneret so that the ﬁlaments
become charged and repel one another or blowing the ﬁlaments from the air tubes
against a bafﬂe plate, which tends to break up any agglomerations. With regard to
Handbook of technical textiles
Diagram of a spun-laid process.
the ﬁlament orientation, in the absence of any positive traversing of the ﬁlaments
in the cross direction, only very small random movements would take place.
However, the movement of the conveyor makes a very strong machine direction
orientation; thus the fabric would have a very strong machine-direction orientation.
Cross-direction movement can most easily be applied by oscillating the air tubes
backwards and forwards. By controlling the speed and amplitude of this oscillation
it is possible to control the degree of cross-direction orientation. A simpliﬁed
diagram of a spun-laid plant is shown in Fig. 6.7.
Flash spinning is a specialised technique for producing very ﬁne ﬁbres without the
need to make very ﬁne spinneret holes. It is used in making only two fabric types.
Flash spinning depends on the fact that the intramolecular bonds in polyethylene
and polypropylene are much weaker than similar bonds in polyester and polyamide.
When a thin sheet of polyoleﬁn is very highly drawn (10 or 12 to 1) the molecules
align in the direction of drawing giving high strength in that direction, but across
the drawing direction the strength is based only on the intramolecular bonds and
so is very low, so low that any mechanical action such as bending, twisting or abrasion causes the sheet to split. Depending on the original thickness of the sheet and
the amount of splitting, the result may be ﬁbre-like but with a rectangular crosssection. The process is known as ﬁbrillation.
In ﬂash spinning the polymer is dissolved in a solvent and is extruded as a sheet
at a suitable temperature so that when the pressure falls on leaving the extruder the
152. Technical fabric structures – 3. Nonwoven fabrics
solvent boils suddenly. This blows the polymer sheet into a mass of bubbles with a
large surface area and consequently with very low wall thickness. Subsequent
drawing of this sheet, followed by mechanical ﬁbrillation, results in a ﬁbre network
of very ﬁne ﬁbres joined together at intervals according to the method of production. This material is then laid to obtain the desired mass per unit area and directional strength.
Flash-spun material is only bonded in two ways, so that it seems sensible to
discuss both the bonding and the products at this juncture. One method (discussed
later in Section 6.10.3) involves melting the ﬁbres under high pressure so that virtually all ﬁbres adhere along the whole of their length and the fabric is almost solid
with very little air space. This method of construction makes a very stiff material
with high tensile and tear strengths. It is mainly used in competition with paper for
making tough waterproof envelopes for mailing important documents and for
making banknotes. The fact that the original ﬁbres were very ﬁne means that the
material is very smooth and can be used for handwriting or printing. The alternative method of bonding is the same, that is, heat and pressure (see Section 6.10.4)
but is only applied to small areas, say 1 mm square, leaving larger areas, say 4 mm
square, completely unbonded. The bonded areas normally form a square or diagonal pattern. This material, known as Tyvek, has a lower tensile strength than the fully
bonded fabric, but has good strength and is ﬂexible enough to be used for clothing.
Because the ﬁne ﬁbres leave very small pores in the fabric, it is not only waterproof
but is also resistant to many other liquids with surface tensions lower than water.
The presence of the pores means that the fabric is permeable to water vapour and
so is comfortable to wear. Tyvek is used principally for protective clothing in the
chemical, nuclear and oil industries, probably as protection for the armed forces and
certainly in many industries not requiring such good protection but where it is found
to be convenient. The garments can be produced so cheaply that they are usually
regarded as disposable.
The process of melt blowing is another method of producing very ﬁne ﬁbres at high
production rates without the use of ﬁne spinnerets. Figure 6.8 shows that the
polymer is melted and extruded in the normal way but through relatively large
As the polymer leaves the extrusion holes it is hit by a high speed stream of hot
air at or even above its melting point, which breaks up the ﬂow and stretches the
many ﬁlaments until they are very ﬁne. At a later stage, cold air mixes with the hot
and the polymer solidiﬁes. Depending on the air velocity after this point a certain
amount of aerodynamic drawing may take place but this is by no means as satisfactory as in spun laying and the ﬁbres do not develop much tenacity. At some point
the ﬁlaments break into staple ﬁbres, but it seems likely that this happens while the
polymer is still liquid because if it happened later this would imply that a high
tension had been applied to the solid ﬁbre, which would have caused drawing before
breaking. The ﬁne staple ﬁbres produced in this way are collected into a batt on a
permeable conveyor as in air laying (Section 6.3) and spun laying (Section 6.6). The
big difference is that in melt blowing the ﬁbres are extremely ﬁne so that there are
many more ﬁbre-to-ﬁbre contacts and the batt has greater integrity.
Handbook of technical textiles
Diagram of melt-blown equipment.
For many end-uses no form of bonding is used and the material is not nonwoven, but simply a batt of loose ﬁbres. Such uses include ultraﬁne ﬁlters for air
conditioning and personal face masks, oil-spill absorbents and personal hygiene
products. In other cases the melt-blown batt may be laminated to another nonwoven, especially a spun-laid one or the melt-blown batt itself may be bonded but the
method must be chosen carefully to avoid spoiling the openness of the very ﬁne
ﬁbres. In the bonded or laminated form the fabric can be used for breathable protective clothing in hospitals, agriculture and industry, as battery separators, industrial wipes and clothing interlinings with good insulation properties. Melt blowing
started to develop rapidly in about 1975, although the process was known before
1950. It is continuing to grow at about 10% per annum.
Chemical bonding involves treating either the complete batt or alternatively isolated
portions of the batt with a bonding agent with the intention of sticking the ﬁbres
together. Although many different bonding agents could be used, the modern industry uses only synthetic lattices, of which acrylic latex represents at least half and
styrene–butadiene latex and vinyl acetate latex roughly a quarter each. When the
bonding agent is applied it is essential that it wets the ﬁbres, otherwise poor adhesion
will be achieved. Most lattices already contain a surfactant to disperse the polymer
particles, but in some cases additional surfactant may be needed to aid wetting. The
next stage is to dry the latex by evaporating the aqueous component and leaving the
polymer particles together with any additives on and between the ﬁbres. During this
stage the surface tension of the water pulls the binder particles together forming a
ﬁlm over the ﬁbres and a rather thicker ﬁlm over the ﬁbre intersections. Smaller
binder particles will form a more effective ﬁlm than larger particles, other things
being equal. The ﬁnal stage is curing and in this phase the batt is brought up to a
higher temperature than for the drying.The purpose of curing is to develop crosslinks
both inside and between the polymer particles and so to develop good cohesive
strength in the binder ﬁlm. Typical curing conditions are 120–140 °C for 2–4 min.
6.9.1 Saturation bonding
Although the principles discussed above apply to all forms of chemical bonding
whatever the method of binder application, this latter factor has a profound
154. Technical fabric structures – 3. Nonwoven fabrics
inﬂuence on the properties of the nonwoven material. As implied by the name,
saturation bonding wets the whole batt with bonding agents, so that all ﬁbres are
covered in a ﬁlm of binder. It is clear that saturation bonding would not be suitable
for ﬂash-spun or melt-blown batts, since it would impair the ﬁne ﬁbres, but it is inherently suitable for all other batts, although other methods of bonding are generally
preferred for spun-laid batts.
To saturate the batt, it is carried under the surface of the bonding agent. In most
cases the batt is very open and weak and care is needed to avoid distortion. The
action of the liquid greatly reduces the thickness of the batt and the thickness is
further reduced by the squeeze rollers which follow. Hence saturation bonded
fabrics are generally compact and relatively thin. However, as in most technologies,
there is an exception to this rule; if coarse ﬁbres containing a lot of crimp are used
they can spring back after being crushed by the squeeze rollers and produce a thick
open fabric, but this is very rare.
The drying is often done in a dryer designed basically for woven fabric, modiﬁed
by having a permeable conveyor to support and transport the nonwoven through
the machine. Hot air is blown against the top and bottom surfaces to cause drying,
the top air pressure being slightly greater than the bottom pressure to press and
control the nonwoven against the conveyor. Because the air only penetrates the
immediate surfaces of the nonwoven, drying is conﬁned to these areas and the
central layers of the nonwoven remain wet. The result is that the liquid wicks from
the wet areas to the dry ones, unfortunately carrying the suspended binder particles
with the water. This is the cause of the problem known as binder migration; under
adverse conditions virtually all the binder can be found in the surface layers and
the central layers contain no binder at all, leaving them very weak. Such a fabric
can easily split into two layers, a problem known as delamination. Fortunately a
number of ways have been found to control binder migration, several of them being
rather complicated. Only one method will be mentioned here, through-drying. In
this case only one air stream is used to blow down and through the fabric. Drying
conditions are then almost the same in all parts of the fabric and no binder migration takes place. However, the air pressure may exert a signiﬁcant force on the nonwoven, pressing it against the conveyor so hard that it may be imprinted with the
pattern of the conveyor.
In contrast the curing stage is simpler; it should be done in a separate compartment in order to achieve the correct temperature. However, it is quite common for
curing to be done in the ﬁnal part of the dryer in order to keep down machinery
Many of the physical properties of saturation-bonded fabric derive from the fact
that all ﬁbres are covered with a ﬁlm of binder. First, the fabric feels like the binder
and not the ﬁbres it is made from. However, in some cases this can be an advantage, because by using either a hydrophobic or a hydrophilic binder the reaction of
the fabric to water can be changed regardless of which ﬁbres are used.
The mechanical properties can be explained from a model of a network of ﬁbres
bonded together at close intervals. The fabric cannot stretch without the ﬁbres also
stretching by a similar amount. Hence the fabric modulus is of the order of the ﬁbre
modulus, that is, extremely high. A high modulus in a spatially uniform material
means that it will be stiff, which explains why saturation-bonded fabrics are very
stiff relative to conventional textiles. At the same time tensile strength is low,
because the bonds tend to break before most ﬁbres break. Efforts to make the
Handbook of technical textiles
fabrics more ﬂexible include using a more ﬂexible binder and using a lower percentage of binder, but both of these reduce the tensile strength; in fact the ratio of
fabric modulus to tensile strength remains remarkably constant.
One of the major uses of saturation bonded fabric turns this apparent disadvantage into an advantage. Interlining fabric for textile clothing is required to be
stiff and to have a high modulus. Other uses are as some types of ﬁlter fabric, in
some coverstock and in wiping cloths.
6.9.2 Foam bonding
It can be inferred above that one of the problems of saturation bonding is that too
much water is used. This not only increases the cost of drying but also increases the
risk of binder migration. Application of chemicals as a foam was developed not
only for nonwovens but also for the dyeing and ﬁnishing industry as a means of
using less water during application. The binder solution and a measured volume of
air are passed continuously through a driven turbine which beats the two components into a consistent foam. The foam is then delivered to the horizontal nip of the
impregnating roller, as shown in Fig. 6.9. The foam delivery has to be traversed
because the foam does not ﬂow easily; end plates, which cannot be shown in the
cross-section diagram prevent the foam from running out of the gap at the end of
The rollers serve the dual purpose of metering the amount of foam applied and
also of squeezing the foam into the batt. If the set-up shown in Fig. 6.9 does not give
adequate foam penetration, then the batt can be entered vertically and the foam
can be applied from both sides.
Foam application should only be thought of as an alternative method of saturation bonding. The properties and uses of the fabrics are identical.
6.9.3 Print bonding
Print bonding involves applying the same types of binder to the batt but the application is to limited areas and in a set pattern. The binder does not penetrate well
into the dry batt so the batt is ﬁrst saturated with water and then printed with either
a printing roller or a rotary screen printer. The ﬁnal properties of the fabric depend
156. Technical fabric structures – 3. Nonwoven fabrics
vitally on the printed/unprinted area ratio, which could be changed signiﬁcantly if
the binder migrated sideways from the printed area. To prevent this the binder
formulation must contain some thickener.
Print-bonded fabrics are much softer in feel and also much more ﬂexible owing
to the strong effect of the free ﬁbres in the unbonded areas. They are also signiﬁcantly weaker than saturation-bonded fabrics owing to the ﬁbres slipping in unbonded areas, but knowing the ﬁbre length and the ﬁbre orientation distribution it
is possible to design a print pattern which will minimise the strength loss.
Print-bonded fabrics tend to be used in applications where the textile-like handle
is an advantage. Examples are disposable/protective clothing, coverstock and wiping
cloths, particularly domestic ones (washing-up and dusting).
6.9.4 Spray bonding
Similar latex binders may also be applied by spraying, using spray guns similar to
those used in painting, which may be either operated by compressed air or be airless.
On the ﬁrst passage the spray penetrates about 5 mm into the top surface, then the
batt is turned over for a spray application on the lower surface. Each spray
application reduces the thickness of the batt slightly, but it is still left substantially
lofty; the drying and curing stage also causes some small dimensional changes.
The ﬁnal product is a thick, open and lofty fabric used widely as the ﬁlling in
quilted fabrics, for duvets, for some upholstery and also for some types of ﬁlter
Thermal bonding is increasingly used at the expense of chemical bonding for a
number of reasons. Thermal bonding can be run at high speed, whereas the speed
of chemical bonding is limited by the drying and curing stage.Thermal bonding takes
up little space compared with drying and curing ovens. Also thermal bonding
requires less heat compared with the heat required to evaporate water from the
binder, so it is more energy efﬁcient.
Thermal bonding can use three types of ﬁbrous raw material, each of which
may be suitable in some applications but not in others. First, the ﬁbres may be all
of the same type, with the same melting point. This is satisfactory if the heat is
applied at localised spots, but if overall bonding is used it is possible that all the
ﬁbres will melt into a plastic sheet with little or no value. Second, a blend of
fusible ﬁbre with either a ﬁbre with a higher melting point or a non-thermoplastic
ﬁbre can be used. This is satisfactory in most conditions except where the fusible
ﬁbre melts completely, losing its ﬁbrous nature and causing the batt to collapse in
thickness. Finally, the fusible ﬁbre may be a bicomponent ﬁbre, that is, a ﬁbre
extruded with a core of high melting point polymer surrounded by a sheath of lower
melting point polymer. This is an ideal material to process because the core of the
ﬁbre does not melt but supports the sheath in its ﬁbrous state. Thermal bonding is
used with all the methods of batt production except the wet-laid method, but it is
worth pointing out that the spun-laid process and point bonding (see Section 6.10.4)
complement each other so well that they are often thought of as the standard
Handbook of technical textiles
6.10.1 Thermal bonding without pressure
The batt may be processed through a hot air oven with just sufﬁcient air movement
to cause the fusible portion to melt. This method is used to produce high loft fabrics;
the products are similar to spray-bonded materials except that in this case the
bonding is uniform all the way through and there is virtually no limit to the thickness of fabric made. The uses of the thermal-bonded fabric are basically the same
as those of a spray-bonded fabric but they would be used in situations where a
higher speciﬁcation is required. One interesting example is in the fuel tanks of
Formula 1 cars to limit the rate of fuel loss in the event of a crash.
6.10.2 Thermal bonding with some pressure
This method is basically the same as the previous one, except that as the batt leaves
the thermobonding oven it is calendered by two heavy rollers to bring it to the
required thickness. The products could be used as insulation, as rather expensive
packaging or for ﬁltration.
6.10.3 Thermal bonding with high pressure
The batt is taken between two large heated rollers (calender rollers) that both melt
the fusible ﬁbre and compress the batt at the same time. Provided the batt is not
too heavy in mass per unit area the heating is very rapid and the process can be
carried out at high speed (300 m min-1). The design of calender rollers for this
purpose has become highly developed; they can be 4–5 m wide and can be heated
to give less than 1 °C temperature variation across the rollers. Also the rollers have
to be specially designed to produce the same pressure all the way across the rollers,
because rollers of this width can bend quite signiﬁcantly.
The products tend to be dense and heavily bonded, although of course the
amount of bonding can be adjusted by varying the percentage of fusible ﬁbre in the
blend. Typical properties are high strength, very high modulus and stiffness but good
recovery from bending. The main uses are in some geotextiles, stiffeners in some
clothing and in shoes, some ﬁltration media and in rooﬁng membranes.
6.10.4 Thermal bonding with point contact
Although it is very strong, the fabric produced with bonding all over the batt (area
bonding) is too stiff and non-textile-like for many uses. It is far more common to
use point bonding, in which one of the calender rollers is engraved with a pattern
that limits the degree of contact between the rollers to roughly 5% of the total area.
The bonding is conﬁned to those points where the rollers touch and leaves roughly
95% of the batt unbonded. The area, shape and location of the bonding points are
of great importance.
Fabrics made in this way are ﬂexible and relatively soft owing to the unbonded
areas. At the same time they maintain reasonable strength, especially in the case of
the spun-laid fabrics. These fabrics have many uses, for example, as a substrate
for tufted carpets, in geotextiles, as a ﬁltration medium, in protective/disposable
clothing, as a substrate for coating, in furniture and home furnishings and as
158. Technical fabric structures – 3. Nonwoven fabrics
6.10.5 Powder bonding
Thermoplastic powders may be used as an alternative to thermoplastic ﬁbres for
bonding in all the methods of thermobonding except for point bonding, where
powder in the unbonded areas would be wasted and would drop out in use. Products made by powder bonding seem to be characterised by softness and ﬂexibility
but in general they have relatively low strength. Again there is a very wide range
of uses covering particularly the high bulk applications, protective apparel and
This form of bonding is only rarely used but it is interesting from two points of view;
ﬁrst, the solvent can be recycled, so the process is ecologically sound, although
whether or not recycling is practical depends on the economics of recovering the
solvent. Second, some of the concepts in solvent bonding are both interesting and
unique. In one application of the method, a spun-laid polyamide batt is carried
through an enclosure containing the solvent gas, NO2 which softens the skin of the
ﬁlaments. On leaving the enclosure bonding is completed by cold calender rolls and
the solvent is washed from the fabric with water using traditional textile equipment.
This is a suitable method of bonding to follow a spun-laid line because the speeds
of production can be matched. The other application uses a so-called latent solvent,
by which is meant one that is not a solvent at room temperature but becomes a
solvent at higher temperatures. This latent solvent is used in conjunction with
carding and cross laying and is applied as a liquid before carding. The action of
carding spreads the solvent and at the same time the solvent lubricates the ﬁbres
during carding. The batt is passed to a hot air oven which ﬁrst activates the solvent
and later evaporates it. The product will normally be high loft, but if less loft is
required a compression roller could be used.
All the methods of bonding discussed so far have involved adhesion between the
ﬁbres; hence they can be referred to collectively as adhesive bonding. The ﬁnal three
methods, needlefelting, hydroentanglement and stitch bonding rely on frictional
forces and ﬁbre entanglements, and are known collectively as mechanical bonding.
The basic concept of needlefelting is apparently simple; the batt is led between
two stationary plates, the bed and stripper plates, as shown in Fig. 6.10. While
between the plates the batt is penetrated by a large number of needles, up to about
4000 m-1 width of the loom. The needles are usually made triangular and have barbs
cut into the three edges as shown in Fig. 6.11.
When the needles descend into the batt the barbs catch some ﬁbres and pull them
through the other ﬁbres. When the needles return upwards, the loops of ﬁbre formed
on the downstroke tend to remain in position, because they are released by the
barbs. This downward pressure repeated many times makes the batt much denser,
that is, into a needlefelt.
The above description illustrates how simple the concept seems to be. Without
going into too much detail it may be interesting to look at some of the complica-
Handbook of technical textiles
Diagram of a needleloom.
Diagram of three needle barbs on a section of a needle.
tions. First, the needles can only form vertical loops or ‘pegs’ of ﬁbre and increase
the density of the batt. This alone does not form a strong fabric unless the vertical
pegs pass through loops already present in the horizontal plane of the batt. It follows
from this that parallel-laid fabric is not very suitable for needling since there
are few ﬁbre loops present, so most needling processes are carried out with crosslaid, air-laid and spun-laid batts. Second, the amount of needling is determined
partly by the distance the drawing rollers move between each movement of the
needleboard, the ‘advance’, and partly by the number of needles per metre across
the loom. If the chosen advance happens to be equal to, or even near the distance
between needle rows as shown in Fig. 6.10, then the next row of needles will
come down in exactly the same position as the previous row, and so on for all the
rows of needles. The result will be a severe needle patterning; to avoid this the
distance between each row of needles must be different. Computer programs
have been written to calculate the best set of row spacings. Third, if it is necessary
to obtain a higher production from a needleloom, is it better to increase the number
of needles in the board or to increase the speed of the needleboard? Finally, in
trying to decide how to make a particular felt it is necessary to choose how
many needle penetrations there will be per unit area, how deep the needles will
penetrate and what type of needles should be used from a total of roughly 5000
different types. The variations possible seem to be inﬁnite, making an optimisation
process very difﬁcult.
There are several different types of needleloom. Figure 6.10 is called a ‘downpunch’ because it is pushing the ﬁbres downwards. Similarly an ‘up-punch’ pushes
the ﬁbres upwards. There is some advantage in combining an up-punch with a downpunch when trying to make a dense felt, rather than to punch continually in the
same direction. For this reason some looms are made ‘double-punch’, that is, one
board punching down and one board punching up. Although this type of double
punch loom is better than unidirectional punching, it has the disadvantage that all
the down-punching is completed before the up-punching even starts. The up-punch
and the down-punch are far from symmetrical. In order to improve this situation
the modern form of double-punch loom has been developed in which both boards
penetrate through the same bed and stripper plates. The normal operation is for the
160. Technical fabric structures – 3. Nonwoven fabrics
boards to penetrate the fabric alternately, one from above and the other from below.
To all intents and purposes the two boards are now symmetrical and this appears
to give optimum needling. This type of loom can often be adjusted so that both sets
of needles enter and leave the batt simultaneously. (Alternate rows of needles have
to be taken out of both boards to prevent serious needle damage.) This is not found
to be advantageous with long ﬁbres (50 mm upwards) because there is quite a high
chance that the same ﬁbre may be pulled upwards by one needle and pushed downwards by another, leading to serious ﬁbre breakage. However, the very short mineral
ﬁbres used for high temperature insulation are found to consolidate better using
this form of simultaneous needling.
Needlefelts have a high breaking tenacity and also a high tear strength but the
modulus is low and the recovery from extension is poor. For these last two reasons
any needlefelt which is likely to be subjected to a load has to have some form of
reinforcement to control the extension. Needled carpets, for instance, may be
impregnated with a chemical binder that gives better dimensional stability and
increases the resistance to wear. In other cases thermal bonding may be used for
the same object. For heavy duty applications such as ﬁlter media and papermakers’
felts, yarns are used, either spun yarns or ﬁlament yarns. In some cases with a crosslaid batt the threads may run only in the machine direction, but it is also common
to use a woven fabric as the foundation and to build up the nonwoven on one or
both sides. In both applications the presence of the woven fabric or base fabric
reduces the efﬁciency by restricting the liquid ﬂow; in a few cases ‘baseless’ fabrics,
that is nonwovens without woven supports have been made, but there are still very
many situations where a base fabric is essential.
Needlefelts are used widely in gas ﬁltration media and in some wet ﬁltration. The
principal advantage is that the nonwoven is practically homogeneous in comparison with a woven fabric so that the whole area of a nonwoven ﬁlter can be used for
ﬁltration, whereas in a woven fabric the yarns effectively stop the ﬂow, leaving only
the spaces between the yarns for ﬁltration. In papermakers’ felts the same considerations apply, but in some cases the design of the felt has also to allow for the fact
that the felt is acting as an enormous drive belt to drive some parts of the machine.
In both gas ﬁltration and papermakers’ felts needlefelts hold virtually the whole
market. Needlefelts are used in geotextiles, but in view of the low modulus their
application is mainly in removing water rather than as reinforcement. If the water
is ﬂowing through the fabric this is termed ﬁltration. For instance a simple drain
may be formed by lining a trench with a geotextile, partly ﬁlling it with graded
gravel, drawing the edges of the geotextile together and back-ﬁlling the trench as
shown in Fig. 6.12. The geotextile will keep the drain open for many years by ﬁltering out ﬁne particles. Less frequently the geotextile is required for drainage,
which means water movement in the plane of the fabric. Because of the inevitable
contamination of the surface layers, together with the compression of the geotextile caused by the soil pressure, only a limited part of the fabric cross-section is
actually available for drainage and more complicated compound structures are
frequently used in preference.
Many makers of synthetic leather have taken the view that the structure should
be similar to natural leather. In these cases the backing or foundation of the
synthetic leather is a needlefelt. The method of production is to include heatshrinkable ﬁbres which are made to shrink after intense needling in order to make
the felt even more dense. After shrinking the felt is impregnated using a binder
Handbook of technical textiles
Simple drain using geotextiles.
that ﬁlls the voids in the felt but does not adhere to the ﬁbres, otherwise the felt
would become very stiff. The leather is then ﬁnished by coating the face side with
one or two layers of suitable polymer. Needlefelts are also widely used in home and
commercial carpeting; in many cases the carpet may have either a velour or a loop
pile surface to improve the appearance. Both velour and loop pile are produced in
a separate needling operation using special needles and a special bedplate in the
needleloom. Similar materials in a lighter weight are used for car carpeting, headliners and other decorative features on cars.
The idea of stitch bonding was developed almost exclusively in Czechoslovakia, in
the former East Germany and to some extent in Russia, though there was a brief
development in Britain. The machines have a number of variants which are best discussed separately; many possible variants have been produced but only a limited
number are discussed here for simplicity.
6.13.1 Batt bonded by threads
Stitch bonding uses mainly cross-laid and air-laid batts. The batt is taken into a
modiﬁcation of a warp knitting machine (see Chapter 5) and passes between the
needles and the guide bar(s). The needles are strengthened and are specially
designed to penetrate the batt on each cycle of the machine. The needles are of the
compound type having a tongue controlled by a separate bar. After the needles pass
through the batt the needle hooks open and the guide bar laps thread into the hooks
of the needles. As the needles withdraw again the needle hooks are closed by the
tongues, the old loops knock over the needles and new loops are formed. In this
way a form of warp knitting action is carried out with the overlaps on one side of
the batt and the underlaps on the other. Generally, as in most warp knitting, continuous ﬁlament yarns are used to avoid yarn breakages and stoppages on the
machine. Two structures are normally knitted on these machines, pillar (or chain)
stitch, or tricot. When knitting chain stitch the same guide laps round the same
needle continuously, producing a large number of isolated chains of loops. When
162. Technical fabric structures – 3. Nonwoven fabrics
knitting tricot structure, the guide bar shogs one needle space to the left, then one
to the right. Single-guide bar structure is called tricot, whereas the two-guide bar
structure is often referred to as full tricot.
The nature of this fabric is very textile-like, soft and ﬂexible. At one time it was
widely used for curtaining but is now used as a backing fabric for lamination, as covering material for mattresses and beds and as the fabric in training shoes. In deciding whether to use pillar or tricot stitch, both have a similar strength in the machine
direction, but in the cross direction the tricot stitch fabric is stronger, owing to the
underlaps lying in that direction. A cross-laid web is already stronger in that direction so the advantage is relatively small. The abrasion resistance is the same on the
loop or overlap side, but on the underlap side the tricot fabric has signiﬁcantly better
resistance owing to the longer underlaps. However, continuous ﬁlament yarn is very
expensive relative to the price of the batt, so tricot fabric costs signiﬁcantly more.
The decision then becomes a purely ﬁnancial one; is it worth paying more for the
greater abrasion resistance?
6.13.2 Stitch bonding without threads
In this case the machine is basically the same as in the previous section, but the
guide bar(s) are not used. The needle bar moves backwards and forwards as before,
pushing the needles through the batt. The main difference is that the timing of the
hook closing by the tongues is somewhat delayed, so that the hook of the needle
picks up some of the ﬁbre from the batt. These ﬁbres are formed into a loop on the
ﬁrst cycle and on subsequent cycles the newly formed loops are pulled through the
previous loops, just as in normal knitting. The ﬁnal structure is felt-like on one side
and like a knitted fabric on the other. The fabric can be used for insulation and as
a decorative fabric.
6.13.3 Stitch bonding to produce a pile fabric
To form a pile fabric two guide bars are usually used, two types of warp yarns (pile
yarn and sewing yarn) and also a set of pile sinkers, which are narrow strips of metal
over which the pile yarn is passed and whose height determines the height of the pile.
The pile yarn is not fed into the needle’s hook so does not form a loop; it is held in
place between the underlap of the sewing yarn and the batt itself. It is clear that this
is the most efﬁcient way to treat the pile yarn, since any pile yarn in a loop is effectively wasted. This structure has been used for making towelling with single-sided
pile and also for making loop-pile carpeting in Eastern Europe.The structure has not
been popular in the West owing to competition with double-sided terry towelling and
tufted carpets. Equally it has not been used in technical textiles, but it could be a solution in waiting for the correct problem. Strangely a suitable problem has been proposed. Car seating usually has a polyester face with a foam backing, but this material
cannot be recycled, because of the laminated foam. It has been suggested that a polyester nonwoven pile fabric could replace the foam and would be 100% recyclable.
6.13.4 Batt looped through a supporting structure
In this technique the needles pass through the supporting fabric and pick up as much
ﬁbre from the batt as possible. Special sinkers are used to push ﬁbre into the needle’s
Handbook of technical textiles
hook to increase this pick-up. The ﬁbre pulled through the fabric forms a chain of
loops, with loose ﬁbre from the batt on the other surface of the fabric. The fabric is
ﬁnished by raising, not as one might expect on the loose side of the fabric but instead
the loops are raised because this gives a thicker pile. This structure was widely used
in Eastern Europe, particularly for artiﬁcial fur, but in the West it never broke the
competition from silver knitting, which gives a fabric with similar properties. The
method could be used for making good quality insulating fabrics.
6.13.5 Laid yarns sewn together with binding threads
Two distinct types of fabric can be made using the same principle. The ﬁrst is a
simulated woven fabric in which the cross-direction yarns are laid many at a time
in a process a bit like cross laying. The machine direction yarns, if any are used, are
simply unwound into the machine. These two sets of yarns are sewn together using
chain stitch if there are only cross-direction threads and tricot stitch if machinedirection threads are present, the underlaps holding the threads down. Although
fabric can be made rapidly by this system this turns out to be a situation in which
speed is not everything and in fact the system is not usually economically competitive with normal weaving. However, it has one great technical advantage; the
machine and cross threads do not interlace but lie straight in the fabric. Consequently the initial modulus of this fabric is very high compared with a woven fabric,
which can ﬁrst extend by straightening out the crimp in the yarn. These fabrics are
in demand for making ﬁbre-reinforced plastic using continuous ﬁlament glass and
similar high modulus ﬁbres or ﬁlaments.
The alternative system makes a multidirectional fabric. Again sets of yarns are
cross-laid but in this case not in the cross direction but at, say, 45° or 60° to the cross
direction. Two sets of yarns at, say, +45° and -45° to the cross direction plus another
layer of yarns in the machine direction can be sewn together in the usual way. Again
high modulus yarns are used, with the advantage that the directional properties of
the fabric can be designed to satisfy the stresses in the component being made.
The process of hydroentanglement was invented as a means of producing an entanglement similar to that made by a needleloom, but using a lighter weight batt. A
successful process was developed during the 1960s by Du Pont and was patented.
However, Du Pont decided in the mid-1970s to dedicate the patents to the public
domain, which resulted in a rush of new development work in the major industrial
countries, Japan, USA, France, Germany and Britain.
As the name implies the process depends on jets of water working at very high
pressures through jet oriﬁces with very small diameters. A very ﬁne jet of this sort
is liable to break up into droplets, particularly if there is any turbulence in the water
passing through the oriﬁce. If droplets are formed the energy in the jet stream will
still be roughly the same, but it will spread over a much larger area of batt so that
the energy per unit area will be much less. Consequently the design of the jet to
avoid turbulence and to produce a needle-like stream of water is critical. The jets
are arranged in banks and the batt is passed continuously under the jets held up
by a perforated screen which removes most of the water. Exactly what happens
164. Technical fabric structures – 3. Nonwoven fabrics
to the batt underneath the jets is not known, but it is clear that ﬁbre ends become
twisted together or entangled by the turbulence in the water after it has hit the batt.
It is also known that the supporting screen is vital to the process; changing the
screen with all other variables remaining constant will profoundly alter the fabric
Although the machines have higher throughputs compared with most bonding
systems, and particularly compared with a needleloom, they are still very expensive
and require a lot of power, which is also expensive. The other considerable problem
lies in supplying clean water to the jets at the correct pH and temperature. Large
quantities of water are needed, so recycling is necessary, but the water picks up air
bubbles, bits of ﬁbre and ﬁbre lubricant/ﬁbre ﬁnish in passing through the process
and it is necessary to remove everything before recycling. It is said that this ﬁltration process is more difﬁcult than running the rest of the machine.
Fabric uses include wipes, surgeons’ gowns, disposable protective clothing and
backing fabrics for coating. The wipes produced by hydroentanglement are guaranteed lint free, because it is argued that if a ﬁbre is loose it will be washed away
by the jetting process. It is interesting to note that the hydroentanglement process
came into being as a process for entangling batts too light for a needleloom, but
that the most recent developments are to use higher water pressures (400 bar) and
to process heavier fabrics at the lower end of the needleloom range.
p lennox-kerr (ed.), Needlefelted Fabrics, Textile Trade Press, Manchester, 1972.
g e cusick (ed.), Nonwoven Conference, Manchester, University of Manchester Institute of Science and
a newton and j e ford, ‘Production and properties of nonwoven fabrics’, Textile Progr., 1973 5(3) 1–93.
p j cotterill, ‘Production and properties of stitch-bonded fabrics’, Textile Progr., 1975 7(2) 101–135.
a t purdy, ‘Developments in non-woven fabrics’, Textile Progr., 1980 12(4) 1–97.
k pﬂiegel, ‘Nonwovens for use in the geotextile area’, Textile Institute Ind., 1981 19 178–181.
a krauter and p ehler, ‘Aspects of ﬁbre to binder adhesion in nonwovens’, Textil Praxis Int., 1980, No.
10, 1206–1212; No. 11, 1325–1328.
anon, ‘Foam padder and foam production for the nonwoven industry’, Chemiefaser/Textilindustrie
(English edition), 1981 4, E.35–36 in English (pp. 336–338 in German).
g e cusick and a newton, (eds), ‘Nonwovens Conference’, Manchester, University of Manchester Institute of Science and Technology, 1988.
g e cusick and k l ghandi, (eds), ‘Conference on nonwovens’, Huddersﬁeld, University of Huddersﬁeld,
a j rigby and s c anand, ‘Nonwovens in medical and healthcare products’, Tech. Textiles Int., 1996, Part
I, Sept. pp. 22–28 Part II, Oct. pp. 24–29.
Index 1999 Congress, Geneva, EDANA (European Disposables and Nonwovens Association), Brussels,
Finishing of technical textiles
Michael E Hall
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
The name textile ﬁnishing covers an extremely wide range of activities, which are
performed on textiles before they reach the ﬁnal customer. They may be temporary,
for example the way bed sheets are pressed before packing, or they may be permanent, as in the case of a ﬂame-retardant tenting fabric. However, all ﬁnishing
processes are designed to increase the attractiveness or serviceability of the textile
product. This could involve such techniques as putting a glaze on an upholstery
fabric, which gives it a more attractive appearance, or the production of waterrepellent ﬁnishes, which improve the in-service performance of a tenting fabric.
Thus a further aim of textile ﬁnishing may be described as improvement in customer
satisfaction, which ﬁnishing can bring about. This improvement in the perceived
value of a product to the consumer forms the basis of modern ideas on product marketing. Technical textiles are deﬁned as those materials with non-clothing applications. Thus the fashion aspects of textiles will be ignored, although aesthetic aspects
of say upholstery and drapes will be covered.
The ﬁnishing processes that are available can be divided into four main groups,
Mechanical processes: these involve the passage of the material through
machines whose mechanical action achieves the desired effects. A heating
process, the purpose of which is usually to enhance these desired effects, frequently accompanies this.
These mechanical ﬁnishes, which will be discussed in detail later in this section,
– Calendering: compression of the fabric between two heavy rolls to give a
ﬂattened, smooth appearance to the surface of the fabric.
166. Finishing of technical textiles
Raising: plucking the ﬁbres from a woven or knitted fabric to give a nap
effect on the surface.
– Cropping: cutting the surface hairs from the a fabric to give a smooth appearance, often used on woollen goods where the removal of surface hair by a
singeing process is not possible.
– Compressive shrinkage: the mechanical shrinking of the warp ﬁbres in woven
fabrics so that shrinkage on washing is reduced to the desired level.
• Heat setting: this is a process for the stabilisation of synthetic ﬁbres so that they
do not shrink on heating.
• Chemical processes: these may be described as those processes that involve the
application of chemicals to the fabric. The chemicals may perform various functions such as water repellency or ﬂame retardancy, or may be used to modify the
handle of a fabric. Chemical ﬁnishes are normally applied in the form of an
aqueous solution or emulsion and may be applied via a variety of techniques,
the main one being the pad mangle, which is illustrated in Fig. 7.1.
After the padding or the application stage of the chemical ﬁnishing the fabric
is usually dried to remove the water from the fabric and some form of ﬁxation
of the ﬁnish is then performed. This commonly takes the form of a baking
process, where the fabric is subjected to a high temperature for a short period,
which enables the applied chemicals to form a more durable ﬁnish on the fabric
than would otherwise be achieved.
Surface coating is a most important part of the ﬁnishing of technical textiles and as
such deserves a separate chapter (see Chapter 8).
Calendering may be deﬁned as the modiﬁcation of the surface of a fabric by the
action of heat and pressure.1 The ﬁnish is obtained by passing the fabric between
heated rotating rollers (or bowls as they are frequently called), when both speed of
rotation and pressure applied are variable. The surfaces of the rollers can be either
smooth or engraved to provide the appropriate ﬁnish to the fabric, while the actual
construction of the rollers may be varied from hardened chromium-plated steel to
elastic thermoplastic rollers.
Simple pad mangle.
Handbook of technical textiles
Flattening effect on fabric of calendering.
184.108.40.206 Effects which may be achieved by calendering
Calendering is done for many purposes but the main effects are:
smoothing the surface of the fabric
increasing the fabric lustre
closing the threads of a woven fabric
decreasing the air permeability
increasing the fabric opacity
improving the handle of a fabric, i.e. softening
obtaining silk-like to high gloss ﬁnishes
surface patterning by embossing
consolidation of nonwovens.
The ﬂattening of the fabric is illustrated in Fig. 7.2, which shows the effect of the
ﬂattened yarn structure. This gives a greater light reﬂectance than the original
rounded yarn structure.
220.127.116.11 Types of calender
In general calenders usually have between two and seven rollers, with the most
common being the three-bowl calender. Perhaps the most important factor in
calender design is the composition of the rollers and the surface characteristics
of these.2 Textile calenders are made up from alternate hard steel and elastic bowls.
The elastic bowls are made from either compressed paper or compressed cotton,
however, a lot of modern calenders are made with a thermoplastic thick covering,
which is usually nylon 6. The latter have the advantage that they are less liable to
damage from knots, seams and creases than cotton and paper bowls, damage that
would then mark off onto the calendered fabric. In fact the development of the
‘in situ’ polymerisation technique for nylon 6 has enabled the simple production
of elastic rollers from this material. Because of this improved performance, nylon 6
covered rollers often enable the required effects to be achieved in a single nip thus
reducing the overall number of bowls.
In two-bowl calenders (Fig. 7.3), it is normal to have the steel bowl on top so that
the operator can see any ﬁnish. This type of arrangement is often used with the
nylon bottom bowl mentioned previously, especially where the calender is used for
glazing or the embossed type of ﬁnishes.
The arrangement where two steel bowls are used together only occurs in exceptional circumstances, for example, in the compaction of nonwovens. Here both bowls
168. Finishing of technical textiles
“Soft” paper or nylon
are usually oil heated so that some form of permanent setting occurs. Finally, the
arrangement with two elastic bowls is not common but is sometimes used on cotton
knitgoods to obtain a soft handle.
The three-bowl calender (Fig. 7.4) was developed from the two-bowl calender
and with this type of calender it is normal to use only the top nip, with the bowls
arranged steel–elastic–steel.The bottom bowl is used to keep the central elastic bowl
smooth and thus assist in the ﬁnishing. The same arrangement also serves the same
purpose on embossing calenders, where there is the possibility of permanent indentation from the top roller.
Pressure used in all of the above calenders can be varied between 10 and 40
tonnes, with running speeds up to 60 m min-1. However, these are very much average
ﬁgures with ﬁgures as low as 6 tonnes for a 1 m wide calender to as high as 120
tonnes for a 3 m wide calender. In addition, running speeds of 20 m min-1 are used
on an embossing calender, while on a glazing calender speeds of over 150 m min-1
have been quoted.
The temperatures which are used in calender rollers can, of course, vary from
room temperature to 250 °C. However, it must be stressed that temperature control
is of vital importance, with a tolerance of ±2 °C being commonly quoted. Some generalisations can be made as follows:
Handbook of technical textiles
Cold bowls give a soft handle without much lustre; warm bowls (40–80 °C) give
a slight lustre.
Hot bowls (150–250 °C) give greatly improved lustre, which can be further
improved by the action of friction and waxes.
18.104.22.168 Types of ﬁnish
• Swissing or normal gloss: a cold calender produces a smooth ﬂat fabric.
However, if the steel bowl of the calender is heated then in addition to smoothness the calender produces a lustrous surface. If a seven-bowl multipurpose calender is used then a smooth fabric with surface gloss on both sides is produced.
• Chintz or glazing: this gives the highly polished surface which is associated with
glazed chintz. The effect is obtained by heating the top bowl on a three-bowl
calender and rotating this at a greater speed than that of the fabric. The speed
of this top bowl can vary between 0 and 300% of the speed of the fabric. In
certain cases where a very high gloss is required, the fabric is often preimpregnated with a wax emulsion, which further enhances the polished effect. This type
of calendering is often called friction calendering.
• Embossing: in this process the heated top bowl of a two-bowl calender is
engraved with an appropriate pattern which is then transferred to the fabric
passing through the bowls. The effect can be made permanent by the use of
thermoplastic ﬁbres or in the case of cellulosics by the use of an appropriate
• Schreiner or silk ﬁnishing: this is a silk-like ﬁnish on one side of the fabric. It is
produced (see Fig. 7.5) by embossing the surface of the fabric with a series of
ﬁne lines on the surface of the bowls. These lines are usually at an angle of about
30° to the warp threads. The effect can be made permanent by the use of
thermoplastic fabric or, in the case of cotton, by the use of a resin ﬁnish. This
ﬁnish is particularly popular on curtains and drapes because of the silk-like
appearance this type of ﬁnish gives to the product.
• Delustering: this is commonly achieved by passing the fabric through the bottom
two bowls of a three-bowl calender, where these are elastic. However, steel bowls
with a special matt ﬁnish have been manufactured that are very effective for this
• Chasing: the fabric is threaded through the calender in such a way as to press the
fabric against itself several times. It is common to use a ﬁve- or seven-bowl calender, the fabric passing through each nip of the calender in two or three layers.
Principle of Schreiner calender.
170. Finishing of technical textiles
Palmer ﬁnishing: in this type of ﬁnish the damp fabric is carried on the inside of
a felt blanket round a steam-heated cylinder, often called a Palmer drier. The
face of the fabric, which is run on the surface of the heated cylinder, takes a light
polish from the cylinder, while the back of the fabric, which is in contact with
the felt blanket, takes a roughened effect from the cylinder. This ﬁnish is particularly popular for cotton drill fabric.
These descriptions of calendering should not be regarded in any way as complete
and for a more complete description the reader is recommended to contact the calender manufacturers. Some of these are Küsters in Germany, Parex Mather in the
UK, Kleinewefers in Germany and Metallmeccanica in Italy.
Raising is the technique whereby a surface effect is produced on the fabric that gives
the fabric a brushed or napped appearance. It is achieved by teasing out the individual ﬁbres from the yarns so that they stand proud of the surface.3 The way this
was done originally was to use the seedpod of the thistle, which was known as a
teasel. These teasels were nailed to a wooden board and the fabric was drawn over
them to produce a fabric with a hairy surface, which had improved insulating properties. This method has largely been superseded by the use of rotating wire brushes,
although where a very gentle raising action is required, such as in the case of mohair
shawls, teasels are still used.
22.214.171.124 Modern raising machines
All modern raising machines (see Fig. 7.6) use a hooked or bent steel wire to tease
the ﬁbres from the surface of fabric. The most important factor in the raising operation is the relationship between the point and the relative speed of the cloth. The
raising wires or ‘card’ wires are mounted on a ﬂexible base, which is then wrapped
around a series of rollers, which are themselves mounted on a large cylindrical
frame, illustrated in Fig. 7.6.
The raising action is brought about by the fabric passing over the rotating rollers
and the wire points teasing out the individual ﬁbres in the yarn. Because there are
a large number of points acting on the fabric at any one time, the individual ﬁbres
must be sufﬁciently free to be raised from the ﬁbre surface. This is a combination
of the intraﬁbre friction and the degree of twist in the raised yarns. Thus for ‘ideal’
raising, the yarns should be of low twist and be lubricated. One further point to note
is that because the fabric runs in the warp direction over the machine, only the weft
threads are at right angles to the rotating raising wires and therefore only the weft
threads take part in the raising process.
126.96.36.199 Raising action
From Fig. 7.6 it can be seen that both the card wire rollers and the cylinder to
which these are attached may be rotated; it is the relative speed of these in relation to
that of the fabric that produces the various raising effects that may be achieved.
There are two basic actions in raising and these are governed by the direction in
which the card wires point and the relative speed of rotation of these in relation to
the fabric.These actions are called the pile and the counterpile actions and are shown
in Fig. 7.7.
Handbook of technical textiles
The modern raising machine.
In the counterpile action, the working roller rotates in the opposite direction to
that of the cylinder with the points of the wire moving in the direction of rotation.
This action pulls the individual ﬁbres free from the surface.
In the pile action, the points of the wire are pointing away from the direction
of movement of the fabric. This results in an action where the raised ﬁbres are
subject to a combing action which tends to tuck back the ﬁbres into the body of the
172. Finishing of technical textiles
rotation of the main
The raising action.
The most common raising action uses a combination of both of these actions,
producing an even raise over the whole of the fabric surface. Control of the raising
action has been achieved by measurement of the surface roughness of the raised
fabric.4 It is therefore possible to control the exact height of the nap on the surface
This is a process by which the ﬁbres which protrude from the surface of a fabric,
are cut to an even height. The principle used in this technique is similar to a lawn
mower in that a spiral cutter rotates against a stationary blade and cuts off any material protruding from the fabric surface.5
This principle is illustrated in Fig. 7.8, which shows the fabric passing over the
cutting bed and the protruding hairs on the surface being caught between the rotating head of the spiral cutter and the ledger blade. By raising and lowering the height
of the cutting bed, the depth of cut may be varied. Obviously the cutting action produces a great deal of cut pile and this must be removed by strong suction otherwise
a large amount of ﬂy rapidly accumulates. In order to achieve an even cut and
a smooth surface, several passes through the machine are required or a single
pass through a multiple head machine is required. Average speeds of about
15 m min-1 are commonly encountered.
One important use for this technique is the production of pile fabrics from a
looped terry fabric. When this type of fabric is sheared the top of the loops of the
terry fabric are cut off and a velvet like appearance is produced. When knitted loop
pile fabrics are sheared, knitted velour is produced that has found a great deal of
use in upholstery fabric.
7.3.4 Compressive shrinkage
The shrinkage of fabrics on washing is a well-known phenomenon. It is caused in
part by the production and processing stresses on the fabric. Production stresses are
introduced into the fabric by the yarn tension and also by the tension which is nec-
Handbook of technical textiles
Spiral cutting cylinder
Shearing or cropping.
essary for the satisfactory production of fabric. Processing stresses are introduced
during the bleaching, dyeing and ﬁnishing of fabric when the fabric is pulled in the
warp direction. This tends to remove the warp crimp from the fabric as illustrated
in Fig. 7.9.
In order to replace the warp crimp and thus minimise warp shrinkage, a process
known as compressive shrinkage is carried out on the fabric to replace the crimp
that has been pulled out in the preparation and ﬁnishing processes. This may be
illustrated in the following way. A strip of fabric is placed on a convex rubber surface
and gripped at each end of the rubber. As the rubber is allowed to straighten, the
length of the fabric exceeds that of the rubber as illustrated in Fig. 7.10. However,
if the fabric could be stuck to the surface of the rubber then the fabric would be
subjected to compression and warp crimp would be introduced.
This principle then is applied to the compressive shrinking machine, where the
cloth is fed in a plastic state onto a thick rubber belt at point A as shown in Fig.
7.11. While the belt is in the convex position for A to B the fabric merely lies on
the surface, but at point B the belt starts to wrap its way round a large heated cylinder and thus changes from a convex to a concave shape. Thus the surface of the
rubber belt contracts and the fabric, which is held onto the surface of the rubber, is
174. Finishing of technical textiles
(a) Fabric under tension, (b) tension relaxed.
Complete shrinkage range.
subject to a warp compression over the region C to D. The actual degree of shrinkage which takes place is controlled by the amount of fabric fed onto the rubber belt
and the pressure between the heated metal cylinder and the belt, which increases
or decreases the concave shape of the rubber belt. The principles of compressive
shrinkage have also been reviewed.6
A sketch of the complete compressive shrinkage range is shown in Fig. 7.12.
The main aim of the heat setting process is to ensure that fabrics do not alter their
dimensions during use. This is particularly important for uses such as timing and
driving belts, where stretching of the belt could cause serious problems. It is important to examine the causes of this loss in stability so that a full understanding can
be obtained of the effects that heat and mechanical forces have on the stability of
fabrics. All fabrics have constraints placed on them by their construction and
method of manufacture, but it is the heat-setting mechanism that occurs within the
ﬁbre that will ultimately inﬂuence fabric dimensions.
Handbook of technical textiles
7.4.1 Heat-setting mechanisms
The ﬁrst attempt to describe the various mechanisms of heat setting synthetic ﬁbres
was that of Hearle.7 He describes the various techniques which have been used to
set fabrics into a given conﬁguration and leaving aside the chemical methods of stabilisation, these techniques may be described as inﬂuencing the following:
strong dipole links
all of which are inﬂuenced by temperature, moisture and stress.
Hydrogen bonding is the most important of the factors which inﬂuence setting,
and nylon has a strong hydrogen-bonded structure whereas polyester has not. Thus
relaxation of nylon can occur in the presence of water at its boiling point. In fact
one of the common tests for the nylon fabrics used in timing belts is a 5 min boil in
7.4.2 Fibre structure
All ﬁbre-forming molecules consist of long chains of molecules. In fact, a typical
nylon molecule will have a length which is some 5000 times the molecule diameter.
X-ray diffraction techniques have conﬁrmed that all synthetic ﬁbres contain crystalline and non-crystalline regions. In nylon and polyester these crystalline regions
occupy about 50% of the total space in the ﬁbre.
It can be shown that these ordered or crystalline regions are small compared to the
overall length of the polymer chain. To explain this phenomenon the polymer chains
cannot be perfectly aligned over the whole length of the molecule, but must pass
through alternating regions of order and disorder. The picture that thus emerges is
one of short crystalline regions connected by relative regions of disorder.This view of
molecular structure is now an accepted model and is known as the fringed micelle
model. Figure 7.13 represents this scheme for a disorientated polymer.
The short parallel areas represent regions of order where adjacent chains pack
in an ordered fashion. The non-parallel regions are where the chains do not pack
together in a regular fashion, creating the non-crystalline regions or amorphous
regions in the ﬁbre.
7.4.3 Polymer orientation
During the processing of both polyester and nylon, the ﬁbres are spun through ﬁne
holes and have a structure similar to that in Fig. 7.13. However, to develop the
176. Finishing of technical textiles
strength in the ﬁbre these ﬁbres are then cold drawn to create an orientated structure, which is illustrated in Fig. 7.14. Once the chains have been orientated then the
ﬁbres show a much greater resistance to applied loads and a greater stiffness, hence
the reason for cold drawing.
7.4.4 Transition temperatures
In the previous section the crystalline and amorphous regions of the polymer were
discussed. These do have an effect on two important parameters:
Glass transition temperature: this represents the temperature at which molecular movement starts in the amorphous regions of the polymer, and was given
the name because it is the temperature at which the polymer changes from
a glassy solid to a rubbery solid. This is the temperature at which segmental
loosening takes place and hence dyeing can only take place above this
Melting point: at this point the forces holding the molecules in the crystalline regions of the ﬁbre are overcome by the thermal energy and the polymer
melts. In both polyester and nylon these temperatures are separated by
about 150 °C.
7.4.5 Heat shrinkage
All textile ﬁbres are subjected to a cold drawing process and hence when they are
heated above the point at which molecular motion sets in, they will progressively
shrink until they reach the point of thermodynamic equilibrium represented by
Fig. 7.13. In other words the cold drawing process is reversed by the application
7.4.6 Heat setting
If the model of the drawn ﬁbre (Fig. 7.14) is considered then it can be observed that
in the drawn ﬁbre, the molecules in the amorphous areas, while still random, are
much more parallel than in the non-drawn state. Thus if the ﬁbre is held so that
shrinkage is prevented and heated above its glass transition temperature, the
Handbook of technical textiles
molecules in the amorphous areas start to move, and because of their relative orientation, to crystallise. In practice the ﬁbres are usually heated to about 20–40 °C
below the melting point. It now becomes apparent that the whole process of heat
setting is time dependent, because it takes time for the motion of the molecules to
line themselves up in the ﬁrst place and then to crystallise. It is possible to heat set
at much lower temperatures than are used in practice. However, if low temperatures are used, the ﬁbres are only stabilised up to the heat set temperature and as
soon as this temperature is exceeded, severe shrinkage occurs. In addition the rate
of crystallisation decreases with decreasing temperature and heat setting would be
a long and tedious process.
Obviously it is the temperature the yarns in the fabric actually achieve that is
important in the setting process. This is dependent not only on the fabric construction but also on the method of heating, because it is essential that the setting temperature is achieved quickly and evenly over the width of the fabric. Commonly,
stenters are used for this purpose, because temperature control to ±1% over a 2 m
width can be obtained. Where contact heating is used, special designs are available
to obtain this degree of control.
7.4.7 Essentials of heat setting
From the previous discussion it can be seen that heat setting is a temperaturedependent process and for practical purposes the heat setting temperatures vary for
polyester between 190–200 °C and for nylon 6.6 between 210–220 °C.The ﬁbres must
not be allowed to move during the heating process and the heating must be sufﬁciently long enough to allow crystallisation to take place, after which the ﬁbre must
be cooled down to well below the heat setting temperature before being released.
There is an important difference between the behaviour of the two common
polyamides (nylon 6 and nylon 6.6) and polyester, because of their different behaviour towards water. Polyester is non-absorbent, so the heat setting behaviour is not
affected by water. However, nylon will absorb sufﬁcient water to obtain a temporary set that is based on hydrogen bonding and is destroyed on boiling in water. The
consequence of this is that to obtain a permanent set on nylon, the water has to be
removed from the ﬁbre so that crystallisation can take place. Therefore nylon tends
to be heat set at a higher temperature than polyester.
Heat the fabric to within about 20–40 °C of the ﬁbre melting point.
Hold at this temperature under tension for approximately 20 s.
Cool fabric before removing tension.
The time–temperature relationship will vary depending on the polymer, the fabric
weight and construction.10 The simple way to determine these is to look at the shrinkage of the ﬁnished product, if the material has been correctly heat set then it should
show a residual shrinkage of less than 1% on a 5 min immersion in boiling water.
It has been suggested that by the end of 2000 some 50% of all textile ﬁbre consumption in industrialised countries will be in technical textiles.11 A large percentage of this will consist of safety equipment and protective clothing and in fact this
178. Finishing of technical textiles
comprises the most signiﬁcant portion of the technical textiles market. Protective
clothing must provide resistance to the elements in the workplace, whilst at the same
time providing comfort during wear.The customers for these products demand strict
compliance with the regulations designed to protect the wearer. One of the most
important properties of this type of clothing is its resistance to small burning
sources, thus ﬂame resistance combined with easy cleaning is a most important consideration. The ﬂame retardance must be maintained throughout the lifetime of the
The main regulation governing the use of ﬂame-retardant technical textiles was
the Furniture and Furnishing Fire Safety Regulations which were introduced
into the UK in 1988.12
7.5.1 Durable ﬂame-retardant treatments13,14
Fire-retardant technical textiles have been developed from a variety of textile ﬁbres,
the choice of which is largely dependent on the cost of the ﬁbre and its end-use.
However, the main ﬁbre in this area is cotton and thus treatments of this ﬁbre will
be discussed ﬁrst. Two major ﬂame-retardant treatments are popular. These are
Proban (Rhodia, formerly Albright and Wilson) and Pyrovatex (Ciba).13
The Proban process uses a phosphorus-containing material, which is based on
tetrakis(hydroxymethyl)phosphonium chloride (THPC). This is reacted with urea
and the reaction product is padded onto cotton fabric and dried. The fabric is then
reacted with ammonia and ﬁnally oxidised with hydrogen peroxide. The full reaction scheme is shown in Fig. 7.15.
The Proban process may be summarised as follows:
Chemistry of the Proban process.
Handbook of technical textiles
1. Pad the fabric with Proban CC.
2. Dry the fabric to a residual moisture content of 12%.
3. React the fabric with dry ammonia gas.
4. Oxidise the fabric with hydrogen peroxide.
5. Wash off and dry the fabric.
6. Soften the fabric.
The actual chemistry of the process is fairly straightforward and the Proban forms
an insoluble polymer in ﬁbre voids and the interstices of the cotton yarn. There is
no actual bonding to the surface of the cellulose, but the insoluble Proban polymer
is held by mechanical means in the cellulose ﬁbres and yarns. Because of this the
Proban treated fabric has a somewhat harsh handle and some softening is usually
required before the fabric is ﬁt for sale. The chemistry is shown in Fig. 7.15.
The next method of forming a durable treatment for cellulose is by the use of
Pyrovatex. This material is closely related to the crosslinked resins used in textile
ﬁnishing and is in fact always applied with a crosslinked resin to form a chemical
bond to the cellulose. The application scheme is given in Fig. 7.16.
The Pyrovatex process may be summarised as follows:
1. Pad the Pyrovatex mixture.
2. Dry at 120 °C.
Chemistry of the Pyrovatex process.
180. Finishing of technical textiles
Cure at 160 °C for 3 min.
Wash in dilute sodium carbonate.
Wash in water.
Dry and stenter to width.
As the reaction is with the cellulose, the ﬂame-retardant substance is chemically
bound to the ﬁbre and is therefore durable. However, because the ﬂame-retardant
substance has to be applied with a crosslink resin, then the ﬁnished fabric has good
dimensional stability and also excellent crease-recovery properties making this
ﬁnish the one preferred for curtains. Unfortunately these desirable properties are
not without disadvantages, the main one in the case of Pyrovatex being the loss in
tear strength, which occurs with this and all crosslinking systems.
7.5.2 Synthetic ﬁbres with inherent ﬂame-retardant properties
The Furniture and Furnishing (Fire) (Safety) Regulations12 made it mandatory that all upholstery materials should withstand the cigarette and match test
as speciﬁed in BS 5852:1979: Pt1. This produced an enormous amount of work
in the industry on possible routes which could be used to meet this legislation.
These ranged from the use of materials that would not support combustion to chemical treatments and backcoating techniques. It is now clear, however, that backcoating is the main means by which these regulations are being met. Currently, some
5000 tonnes of backcoating formulations are being used in the UK for upholstery
The majority of backcoating formulations are based on the well-known ﬂameretardant effect of the combination of antimony(III) oxide and a halogen, which is
usually bromine, although chlorine is also used to a lesser degree. The synergistic
mixture for this is one part of antimony(III) oxide to two parts of bromine containing organic compound. A typical formulation which describes the application
level per square metre, is shown in Table 7.1.
To this basic formulation are often added softeners, which modify the fabric
handle and antifungal compounds. In addition, foaming agents are used which
enable the use of foam application techniques, so that a minimum amount of
penetration of the backcoating compound onto the face of the fabric is achieved.
The use of foam application also enables higher precision in the weights applied
and shorter drying times to be achieved.15
Thus Proban, Pyrovatex and backcoating with antimony/bromine compounds
represent the major ﬂame-retardant treatments for cellulose.
7.5.3 Water-repellent ﬁnishes
The early water-repellent ﬁnishes were all based on the application of a mixture of
waxes, which were pliable at normal temperatures, applied to tightly woven cotton
fabrics. These were, of course, well suited to sail cloth and protective clothing, but
problems were encountered when the garments were cleaned. Therefore, the search
was on for water-repellent treatments that were simple to apply but would also allow
the treated fabrics to be cleaned.
It was noted early on that the heavy metal soaps did have water-repellent properties and therefore the ﬁrst attempt at the production of a durable treatment was
Handbook of technical textiles
Typical backcoating formulation
Application level (g m-2)
Cellulose surface with hydroxyl groups
Reaction of the chromium salt of a fatty acid with cellulose.
to use the chromium salt of a fatty acid, which was applied to cotton and then baked.
This gave a certain durability to the fabric thus treated and the mechanism is illustrated in Fig. 7.17.
Some of the later treatments involved the use of other fatty acid derivatives and
some of these are shown in Fig. 7.18.
The most recent treatments involve the use of the ﬂuorocarbons which are
basically esters of polyacrylic acid and a perﬂuorinated hexanol, as illustrated in
Fig. 7.19. A list of ﬁnishes is given in Table 7.2.6
7.5.4 Antistatic ﬁnishes
Static electricity is formed when two dissimilar materials are rubbed together. It
cannot be formed if identical materials are rubbed together. Thus when dissimilar
materials are rubbed together a separation of charges occurs and one of the materials becomes positively charged and the other negatively charged. The actual sign
of the charge depends on the nature of the two materials that are taking part and
this may be deduced from the triboelectric series, shown in Table 7.3. The ma